Lithium-Ion Batteries and Solar Cells: Physical, Chemical, and Materials Properties presents a thorough investigation of
668 134 30MB
English Pages 308  Year 2021
418 32 118MB Read more
This book covers a wide range of topics on work function and band alignment, from the basics to practical examples. Work
369 119 11MB Read more
A major update of solar cell technology and the solar marketplace Since the first publication of this important volume o
484 116 12MB Read more
756 121 5MB Read more
https://www.springer.com/gp/book/9783030363536 This book addresses the rapidly developing class of solar cell materials
1,104 169 14MB Read more
Solar Cells and Light Management: Materials, Strategies and Sustainability provides an extensive review on the latest ad
572 30 35MB Read more
This book presents a state-of-the-art overview of the research and development in designing electrode and electrolyte ma
463 105 14MB Read more
Modern devices Thermodynamics: Batteries, Fuel Cells and Supercapacitors considers various aspects of Modern devices The
471 86 13MB Read more
Table of contents :
Table of Contents
Chapter 1 Introduction
Chapter 2 Diverse Phenomena in Stage-n Graphite Alkali-Intercalation Compounds
2.2 Theoretical Calculations
2.3 Unique Stacking Configurations and Intercalant Distributions
2.4 Metallic and Semimetallic Behaviors
2.5 Concluding Remarks
Chapter 3 Effect of Nitrogen Doping on the Li-Storage Capacity of Graphene Nanomaterials: A First-Principles Study
3.2 Computational Details
3.3 Results and Discussion
3.3.1 Formation Energy of N-Doped Defects in Graphene
3.3.2 Single Li-Adsorption on N-Doped Defects in Graphene
3.3.3 Li-Storage Capacity of N-Doped Defective Graphene
3.3.4 Migration Energy Barrier of N-Doped Defects in Graphene
Chapter 4 Fundamental Properties of Li[sub(+)]-Based Battery Anode: Li[sub(4)]Ti[sub(5)]O[sub(12)]
4.2 Theoretical Simulation Methods
4.3 Rich Geometric Symmetries of 3D Li[sub(4)]Ti[sub(5)]O[sub(12)] Compound
4.4 Rich and Unique Electronic Properties
4.5 Concluding Remarks
Chapter 5 Diversified Properties in 3D Ternary Oxide Compound: Li[sub(2)]SiO[sub(3)]
5.2 Numerical Simulations
5.3 Results and Discussion
5.3.1 Geometric Structures
5.3.2 Rich Electronic Properties
5.3.3 Comparisons, Measurements, and Applications
5.4 Concluding Remarks
Chapter 6 Electrolytes for High-Voltage Lithium-Ion Battery: A New Approach with Machine Learning
6.2 Metrics for Molecular Selection
6.3 Experiments, First-Principles Calculation, and Machine Learning
6.4 Machine Learning Regression Model and Property Predictor
6.5 Property Predictor
6.6 Inverse Design and Deep Generative Machine Learning Model
6.8 Our Adapted Model and Experience
Chapter 7 Geometric and Electronic Properties of Li[sup(+)]-Based Battery Cathode: Li[sub(x)]Co/NiO[sub(2)]Compounds
7.2 Delicately Numerical VASP Calculations
7.3 Unusual Crystal Structures of 3D Ternary Li[sub(x)]Co/NiO[sub(2)] Materials
7.4 Rich and Unique Electronic Properties
7.5 Concluding Remarks
Chapter 8 Graphene as an Anode Material in Lithium-Ion Battery
8.2 Synthesis of Graphene
8.3 Basic Characterizations of Graphene
8.3.1 Structure and Microstructure Analysis
8.3.2 Bonding/Binding Energy/Functional Groups and Phonon Modes
8.4 Graphene as Anode in Lithium-Ion Batteries
8.4.2 Doped Graphene
8.4.3 Porous Graphene
8.4.4 Chemically Modified Graphene for Fast-Charging Lithium-Ion Battery (LIB)
Chapter 9 Liquid Plasma: A Synthesis of Carbon/Functionalized Nanocarbon for Battery, Solar Cell, and Capacitor Applications
9.2 Formation of Various Forms of Nanocarbon in the Liquid Plasma Process
9.2.1 Formation of Unconventional Polymers in the Liquid Plasma Process
9.2.2 Direct Functionalization of Graphene in the Liquid Plasma Process
9.3 Applications of Nanocarbons Synthesized from the Liquid Plasma Process
9.3.1 Application Nanocarbon Hybrids/Composites for Fuel Cell Applications
9.3.2 Application Nanocarbon Hybrids/Composites for Specific Capacitance Applications
9.4 Future Prospective
Chapter 10 Ionic Liquid-Based Electrolytes: Synthesis and Characteristics and Potential Applications in Rechargeable Batteries
10.2 Some Concepts of IL-Based Electrolytes for Li–Ion/Na–Ion Batteries
10.2.1 Low-Melting Alkaline Salts
10.2.1.1 Low-Melting lithium Salts
10.2.1.2 Mixtures of Alkaline Imide Salts
10.2.2 Alkaline Salts Dissolved in Organic Ionic Liquids
10.2.2.1 Effects of Cation Structure
10.2.2.2 Effects of Anion Structure
10.2.2.3 Effect of Organic Solvent Added to ILs
10.2.3 Solvent-in-Salt Electrolytes
10.2.4 Li[sup(+)]-Conducting Polymer Electrolytes Containing Ionic Liquids
10.3 Synthesis of Ionic Liquids
10.3.1 Typical Ionic Liquid Synthetic Route
10.3.1.1 Synthetic Route 1 (Quaternization)
10.3.1.2 Metathesis Reaction
10.4 Applying ILs for Li–Ion/Na–Ion Batteries
Chapter 11 Imidazolium-Based Ionogels via Facile Photopolymerization as Polymer Electrolytes for Lithium–Ion Batteries
11.2.2 Synthesis of Prepolymer, 1-Ethyl-3-Vinylimidazolium Bis (Trifluoromethanesulfonylimide) (1E3V-TFSI)
11.2.3 Anion Substitution of IL Additive
11.2.4 Preparation of Electrolytes
11.2.5 Sample Characterization
11.2.6 Ionic Conductivity and Linear Sweep Voltammetry (LSV) of Measurement
11.2.7 Battery Cell Assembly
11.2.8 Charge–Discharge Performance and Cycle Life
11.3 Results and Discussion
11.3.1 Preparation and Characterization
11.3.2 Thermal Properties of Electrolytes
11.3.3 Ionic Conductivity and Electrochemical Windows
11.3.4 Charge–Discharge Capacity and Cyclic Performance
Chapter 12 Back-Contact Perovskite Solar Cells
12.2 Coplanar Back-Contact Structure
12.3 Non-Coplanar Back-Contact Structure
Chapter 13 Engineering of Conductive Polymer Using Simple Chemical Treatment in Silicon Nanowire-Based Hybrid Solar Cells
13.2 PEDOT:PSS with Tunable Electrical Conductivity
13.2.1 PEDOT:PSS Fabricated by “Baytron P” Routes
13.2.2 PSS Functions in Commercial PEDOT:PSS Complex
13.2.3 PSS Investigations of Electrical Conductivity in PEDOT:PSS
13.3 Treated PEDOT:PSS for Silicon Nanowires-Based Hybrid Solar Cells
Chapter 14 Concluding Remarks
Chapter 15 Open Issues and Potential Applications
Chapter 16 Problems
Lithium-Ion Batteries and Solar Cells
Lithium-Ion Batteries and Solar Cells Physical, Chemical, and Materials Properties
Edited by Ming-Fa Lin, Wen-Dung Hsu, and Jow-Lay Huang
MATLAB® is a trademark of The MathWorks, Inc. and is used with permission. The MathWorks does not warrant the accuracy of the text or exercises in this book. This book’s use or discussion of MATLAB® software or related products does not constitute endorsement or sponsorship by The MathWorks of a particular pedagogical approach or particular use of the MATLAB® software First edition published 2021 by CRC Press 6000 Broken Sound Parkway NW, Suite 300, Boca Raton, FL 33487-2742 and by CRC Press 2 Park Square, Milton Park, Abingdon, Oxon, OX14 4RN © 2021 Taylor & Francis Group, LLC CRC Press is an imprint of Taylor & Francis Group, LLC Reasonable efforts have been made to publish reliable data and information, but the author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use. The authors and publishers have attempted to trace the copyright holders of all material reproduced in this publication and apologize to copyright holders if permission to publish in this form has not been obtained. If any copyright material has not been acknowledged please write and let us know so we may rectify in any future reprint. Except as permitted under U.S. Copyright Law, no part of this book may be reprinted, reproduced, transmitted, or utilized in any form by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying, microfilming, and recording, or in any information storage or retrieval system, without written permission from the publishers. For permission to photocopy or use material electronically from this work, access www.copyright. com or contact the Copyright Clearance Center, Inc. (CCC), 222 Rosewood Drive, Danvers, MA 01923, 978-750-8400. For works that are not available on CCC please contact [email protected]. Trademark notice: Product or corporate names may be trademarks or registered trademarks and are used only for identification and explanation without intent to infringe. Library of Congress Cataloging-in-Publication Data Names: Lin, Ming-Fa, editor. | Hsu, Wen-Dung, editor. | Huang, Jow-Lay, editor. Title: Lithium-ion batteries and solar cells : physical, chemical, and materials properties / edited by Ming-Fa Lin, Wen-Dung Hsu, Jow-Lay Huang. Description: First edition. | Boca Raton, FL : CRC Press/ Taylor & Francis Group, LLC, 2021. | Includes bibliographical references and index. | Summary: “This book presents a thorough investigation of diverse physical, chemical, and material properties and special functionalities of lithium-ion batteries and solar cells. It covers theoretical simulations and high-resolution experimental measurements that promote a full understanding of the basic science to develop excellent device performance. This book will be of interest to materials scientists and engineers developing enhanced batteries and solar cells for peak performance”—Provided by publisher. Identifiers: LCCN 2020043473 (print) | LCCN 2020043474 (ebook) | ISBN 9780367686239 (hardback) | ISBN 9781003138327 (ebook) Subjects: LCSH: Lithium ion batteries—Materials. | Solar cells—Materials. Classification: LCC TK2945.L58 L5554 2021 (print) | LCC TK2945.L58 (ebook) | DDC 621.31/242—dc23 LC record available at https://lccn.loc.gov/2020043473 LC ebook record available at https://lccn.loc.gov/2020043474 ISBN: 9780367686239 (hbk) ISBN: 9781003138327 (ebk) Typeset in Times by codeMantra
Contents Preface......................................................................................................................vii Acknowledgments .....................................................................................................ix Editors .......................................................................................................................xi Contributors ........................................................................................................... xiii Chapter 1
Introduction .......................................................................................... 1 Sanjaya Brahma, Ngoc Thanh Thuy Tran, Wen-Dung Hsu, Chin-Lung Kuo, Shih-Yang Lin, Jow-Lay Huang, Masahiro Yoshimura, Phung My Loan Le, Jeng-Shiung Jan, Chia-Yun Chen, Peter Chen, and Ming-Fa Lin
Diverse Phenomena in Stage-n Graphite Alkali-Intercalation Compounds......................................................................................... 19 Wei-bang Li, Ngoc Thanh Thuy Tran, and Shih-Yang Lin
Effect of Nitrogen Doping on the Li-Storage Capacity of Graphene Nanomaterials: A First-Principles Study ........................... 45 Chin-Lung Kuo and Yu-Jen Tsai
Fundamental Properties of Li+-Based Battery Anode: Li4Ti5O12 ....... 59 Thi Dieu Hien Nguyen, Hai Duong Pham, Shih-Yang Lin, Ngoc Thanh Thuy Tran, and Ming-Fa Lin
Diversified Properties in 3D Ternary Oxide Compound: Li2SiO3 ..... 79 Nguyen Thi Han, Ngoc Thanh Thuy Tran, Vo Khuong Dien, Duy Khanh Nguyen, and Ming-Fa Lin
Electrolytes for High-Voltage Lithium-Ion Battery: A New Approach with Machine Learning ....................................... 103 Ming-Hsiu Wu, Chih-Ao Liao, Ngoc Thanh Thuy Tran, and Wen-Dung Hsu
Geometric and Electronic Properties of Li+-Based Battery Cathode: LixCo/NiO2 Compounds ................................................... 117 Shih-Yang Lin, Hsin-Yi Liu, Sing-Jyun Tsai, and Ming-Fa Lin
Graphene as an Anode Material in Lithium-Ion Battery ................. 149 Sanjaya Brahma, Alex Chinghuan Lee, and Jow-lay Huang
Liquid Plasma: A Synthesis of Carbon/Functionalized Nanocarbon for Battery, Solar Cell, and Capacitor Applications .... 167 Masahiro Yoshimura, Jaganathan Senthilnathan, and Anupama Surenjan
Chapter 10 Ionic Liquid-Based Electrolytes: Synthesis and Characteristics and Potential Applications in Rechargeable Batteries ..................... 181 Linh T. M. Le, Thanh D. Vo, Hoang V. Nguyen, Man V. Tran, and Phung M. L. Le Chapter 11 Imidazolium-Based Ionogels via Facile Photopolymerization as Polymer Electrolytes for Lithium–Ion Batteries .............................. 203 Yu-Chao Tseng and Jeng-Shiung Jan Chapter 12 Back-Contact Perovskite Solar Cells ................................................ 219 Tai-Fu Lin, Ming-Hsien Li, Pei-Ying Lin, Itaru Raifuku, Joey Lin, and Peter Chen Chapter 13 Engineering of Conductive Polymer Using Simple Chemical Treatment in Silicon Nanowire-Based Hybrid Solar Cells .............. 233 Po-Hsuan Hsiao, Ilham Ramadhan Putra, and Chia-Yun Chen Chapter 14 Concluding Remarks ........................................................................ 251 Ngoc Thanh Thuy Tran, Sanjaya Brahma, Wen-Dung Hsu, Shih-Yang Lin, Jow-Lay Huang, Masahiro Yoshimura, Jeng-Shiung Jan, Chia-Yun Chen, Peter Chen, Ming-Fa Lin, Chin-Lung Kuo, and Phung My Loan Le Chapter 15 Open Issues and Potential Applications ........................................... 261 Thi Dieu Hien Nguyen, Ngoc Thanh Thuy Tran, and Ming-Fa Lin Chapter 16 Problems ........................................................................................... 279 Thi Dieu Hien Nguyen, Ngoc Thanh Thuy Tran, and Ming-Fa Lin Index ...................................................................................................................... 287
Preface This book presents thorough investigations on the diversified physical/chemical/ materials properties and special functionalities of certain batteries, covering the development of theoretical simulations, high-resolution experimental measurements, and excellent device performance. It is robust in detail and thoroughly explores the basic sciences, application engineering, and commercial products. Concerning lithium-ion-based batteries, the first-principles method and the machine learning method are utilized to fully explore the rich and unique phenomena of cathodes, anodes, and electrolytes (solid and liquid states). Specifically, the theoretical frameworks are built from them. Parts of theoretical predictions are consistent with the measured results. Distinct experimental methods/techniques are developed to greatly enhance the performance of lithium-ion-based batteries and solar cells, such as the efficient syntheses of ion-battery core materials. Moreover, the emerging open issues are currently under systematic investigations. Very interestingly, the whole content is characterized by concise pictures, so that this work is suitable for senior graduate students and scientists. We have successfully developed the first-principles theoretical framework and the machine learning method, as clearly illustrated for LiCo/NiO/LiSiO/LiTiO/graphite alkali-intercalation compounds and various liquid electrolytes, respectively. Such methods are able to thoroughly explore the geometric structures, electronic properties, and magnetic configurations. Accurate VASP calculations and analyses are achieved from the optimal geometric symmetries, atom-dominated electronic energy spectra, spatial charge density distributions, atom- and orbital-projected density of states, spin distribution configurations, spin-split or spin-degenerate energy bands, and the atom- and orbital-dependent net magnetic moments. Consequently, the concise physical/chemical properties, the single- and/or multi-orbital hybridizations in various chemical bonds and the spin configurations due to distinct atoms and orbitals are clearly identified in this work. The successful syntheses, fabrications, and measurements are outlined in this book. Enhancing the Li+-transport performance is achieved by examining the chemisorption of ions on the undoped/doped (B&N on vacancies)/porous graphene systems for anode materials. Different nanocarbon structures are efficiently generated using submerged liquid plasma. This provides a simple, low capital cost, high yield, and an environmentally friendly approach. The advantages and near-future challenges, which are similar to the use of ionic liquids as electrolytes for distinct chemical batteries, are discussed in detail. The gel polymer electrolytes of lithium-ion batteries are successfully synthesized and measured. The silicon-nanowire-based hybrid solar cells are modified to greatly enhance the photovoltaic performance under the various chemical treatments, such as the doping mechanisms, conformational changes of the
PEDOT segment, arrangement alteration of PEDOT:PS (poly(3,4-ethylenedioxythio phene):poly(styrenesulfonate)), and the removal of excess insulating PSS chains from the PEDOT:PSS film. Moreover, back-contact perovskite solar cells are realized to present a high photon-to-electron conversion efficiency.
MATLAB® is a registered trademark of The MathWorks, Inc. For product information, please contact: The MathWorks, Inc. 3 Apple Hill Drive Natick, MA 01760-2098 USA Tel: 508-647-7000 Fax: 508-647-7001 E-mail: [email protected] Web: www.mathworks.com
Acknowledgments This work was financially supported by the Hierarchical Green-Energy Materials (Hi-GEM) Research Center, from the Featured Areas Research Center Program within the framework of the Higher Education Sprout Project by the Ministry of Education (MOE) and the Ministry of Science and Technology (MOST 109-2634-F006-020) in Taiwan.
Editors Ming-Fa Lin, PhD, is a distinguished professor in the Department of Physics, National Cheng Kung University (NCKU), Taiwan. He earned his PhD in physics in 1993 from the National Tsing-Hua University, Taiwan. His main scientific interests focus on the essential properties of carbon-related materials and low-dimensional systems. He is a member of the American Physical Society, American Chemical Society, and the Physical Society of Republic of China (Taiwan).
Wen-Dung Hsu, PhD, is an associate professor in the Department of Materials Science and Engineering, National Cheng Kung University (NCKU). His expertise is utilizing computational materials science methods including first-principles calculations, molecular dynamics simulations, Monte Carlo methods, and finite-element methods to study materials issues. His research interests are mechanical properties of materials from atomic to macro scale, lithium-ion battery, solid-oxide fuel cell, ferroelectrics, solid catalyst design for biodiesel, and processing design for single-crystal growth. He earned his PhD from the Department of Materials Science and Engineering, University of Florida, in 2007. He then served as a post-doctoral researcher in the Department of Mechanical Engineering at the University of Michigan. He joined National Cheng Kung University in 2008. Jow-Lay Huang, PhD, is a chair professor in the Department of Materials Science and Engineering, National Cheng Kung University (NCKU), Taiwan. He is the director in Hierarchical Green-Energy Materials (Hi-GEM) Research Center, NCKU, Taiwan. He earned his PhD in Materials Science and Engineering in 1983 from the University of Utah, Salt Lake City, Utah, USA. His research interests include the fabrication, development, and application of ceramic nanocomposites, piezo-phototronic thin films for photodetector devices, piezoelectric thin films for high-frequency devices, metal oxide/graphene and SiCx nanocomposites utilized as anode materials for lithium-ion battery, and 2D nanocrystal materials for photoelectrochemical application. xi
Contributors Sanjaya Brahma Hierarchical Green-Energy Materials (Hi-GEM) Research Center National Cheng Kung University Tainan, Taiwan
Jeng-Shiung Jan Department of Chemical Engineering National Cheng Kung University Tainan, Taiwan
Chia-Yun Chen Department of Materials Science and Engineering Hierarchical Green-Energy Materials (Hi-GEM) Research Center National Cheng Kung University Tainan, Taiwan
Chin-Lung Kuo Department of Materials Science and Engineering National Taiwan University Taipei, Taiwan
Peter Chen Department of Photonics Hierarchical Green-Energy Materials (Hi-GEM) Research Center National Cheng Kung University Tainan, Taiwan Vo Khuong Dien Department of Physics National Cheng Kung University Tainan, Taiwan Nguyen Thi Han Department of Physics National Cheng Kung University Tainan, Taiwan and Department of Chemistry Thai Nguyen University of Education Thai Nguyen City, Vietnam Po-Hsuan Hsiao Department of Materials Science and Engineering National Cheng Kung University Tainan, Taiwan
Linh T. M. Le Applied Physical Chemistry Key Laboratory University of Science, Vietnam National University Ho Chi Minh City (VNU HCM), Vietnam Phung My Loan Le Applied Physical Chemistry Key Laboratory University of Science, Vietnam National University Ho Chi Minh City (VNU HCM), Vietnam Alex Chinghuan Lee Hierarchical Green-Energy Materials (Hi-GEM) Research Center National Cheng Kung University Tainan, Taiwan Ming-Hsien Li Department of Photonics National Cheng Kung University Tainan, Taiwan
Wei-bang Li Department of Physics National Cheng Kung University Tainan, Taiwan Chih-Ao Liao Department of Materials Science and Engineering National Cheng Kung University Tainan, Taiwan Joey Lin Department of Photonics National Cheng Kung University Tainan, Taiwan
Hoang V. Nguyen Applied Physical Chemistry Key Laboratory University of Science, Vietnam National University Ho Chi Minh City (VNU HCM), Vietnam Thi Dieu Hien Nguyen Department of Physics National Cheng Kung University Tainan, Taiwan
Pei-Ying Lin Department of Photonics National Cheng Kung University Tainan, Taiwan
Trung T. Nguyen Applied Physical Chemistry Key Laboratory University of Science, Viet Nam National University Ho Chi Minh City (VNU HCM), Vietnam
Shih-Yang Lin Department of Physics National Chung Cheng University Chiayi, Taiwan
Hai Duong Pham Department of Physics National Cheng Kung University Tainan, Taiwan
Tai-Fu Lin Department of Photonics National Cheng Kung University Tainan, Taiwan
Ilham Ramadhan Putra Department of Materials Science and Engineering National Cheng Kung University Tainan, Taiwan
Hsin-Yi Liu Department of Physics National Cheng Kung University Tainan, Taiwan Duy Khanh Nguyen Advance Institute of Materials Science Ton Duc Thang University Ho Chi Minh City, Vietnam
Itaru Raifuku Department of Photonics National Cheng Kung University Tainan, Taiwan Jaganathan Senthilnathan Environmental and Water Resources Engineering Division Department of Civil Engineering Indian Institute of Technology Madras Chennai, India
Anupama Surenjan Department of Civil Engineering National Institute of Technology Karnataka Surathkal, India Man V. Tran Applied Physical Chemistry Key Laboratory University of Science, Vietnam National University Ho Chi Minh City (VNU HCM), Vietnam Ngoc Thanh Thuy Tran Hierarchical Green-Energy Materials (Hi-GEM) Research Center National Cheng Kung University Tainan, Taiwan Sing-Jyun Tsai Department of Physics National Cheng Kung University Tainan, Taiwan Yu-Jen Tsai Department of Materials Science and Engineering National Taiwan University Taipei, Taiwan
Yu-Chao Tseng Department of Chemical Engineering National Cheng Kung University Tainan, Taiwan Thanh D. Vo Applied Physical Chemistry Key Laboratory University of Science, Vietnam National University Ho Chi Minh City (VNU HCM), Vietnam Ming-Hsiu Wu Department of Materials Science and Engineering National Cheng Kung University Tainan, Taiwan Masahiro Yoshimura Promotion Centre for Global Materials Research (PCGMR) Department of Material Science and Engineering National Cheng Kung University Tainan, Taiwan
Introduction Sanjaya Brahma, Ngoc Thanh Thuy Tran, and Wen-Dung Hsu National Cheng Kung University
Chin-Lung Kuo National Taiwan University
Shih-Yang Lin, Jow-Lay Huang, and Masahiro Yoshimura National Cheng Kung University
Phung My Loan Le University of Science, Vietnam National University
Jeng-Shiung Jan, Chia-Yun Chen, Peter Chen, and Ming-Fa Lin National Cheng Kung University
CONTENTS 1.1 Introduction ....................................................................................................... 1 References ................................................................................................................ 11
How to get and use energies very efficiently is the mainstream research topic in terms of the basic sciences/advanced engineering and potential applications. The various theoretical models [1–5] and experimental syntheses [6–11] have been proposed to fully present the essential properties, outstanding functionalities, and commercialized products of green energy materials. The LIBs principally consist of cathode, electrolyte, and anode materials, in which the second systems might be either in solid  or in liquid states [13,14]. The numerical simulations, the first-principles calculations , neural network, and molecular dynamics  are frequently utilized to investigate their rich and unique properties, such as the growth processes, optimal geometric structures within large unit cells, electronic energy spectra, van Hove singularities in density of states, orbital hybridizations of chemical bonds, magnetic configurations, and special optical absorption spectra. The close combinations of core components in batteries are required to display the high-performance 1
Lithium-Ion Batteries and Solar Cells
characteristics: low cost, lightweight, high safety, short charging time, long operation time, controllable temperature, and wide voltage range. Up to now, there exist a lot of well-established products that cover the b attery-driven cell phones and electric vehicles (EVs), the solar cell companies, the hydrogen-based cars, the water-induced electric power, the wind turbines, and so on. By the delicate numerical calculations, successful syntheses, detailed analysis, and w ell-behaved designs, this book thoroughly explores the diversified physical, chemical, and material phenomena of fundamental properties and the unusual f unctionalities in LIBs [1–11], Si nanowire-based solar cells , and perovskite solar cells . Furthermore, the relations between the theoretical predictions and the high-resolution measurements are fully discussed. It provides very useful information about science bases, integrated engineering, and real applications. Table 1.1 provides the diversified materials of anode, cathode, and electrolyte. The anode materials require the large capability of lithium intercalation/adsorption, high efficiency of charge/discharge, excellent cyclability, low reactivity against electrolyte, fast reaction rate, low cost, environmental-friendly, and nontoxic [19–23]. Graphite, which is one of the primary carbon materials, can serve as anode of Li+-ion-based batteries and is predominantly used in commercial products [23–25]. Lithium ions are electrochemically intercalated into the space between the graphitic sheets during the charging process and de-intercalated in the discharging process. A practical reversible capacity is greater than 360 mAh g−1 (theoretically at 372 mAh g−1) with the high discharge/charge efficiency [26–28]. However, graphite has a huge backward in volume expansion. There are new carbon materials, such as carbon nanofibers (CNF) [33–35] and carbon nanotubes (CNT) [31,32], where the single-walled CNTs are expected to exhibit reversible capacities about 300–600 mAh g−1 . Besides the above materials, Li4Ti5O12 is known as a potential anode material for the next-generation LIBs [39–41]. In the current work, Li4Ti5O12 has been focused on the rich and unique essential properties with highly nonuniform environments, clearly revealing the thermodynamic stability, high cycle life performance, and safety, compared to other anode material candidates. The other materials are also available in anode electrode, e.g., TiO2 [19–22], patterned Si , Si film , Si nanowires [36,37], Si nanotubes , MoO3 , SnO2 , ZnO , Fe3O4/carbon foam , MnO , Co3O4 , GaSx [48,49], and MoS2 . The most common cathode materials are LiCoO2 [55,56], Li-Mn-O , LiFePO4 , and lithium-layered metal oxides, mainly owing to the very high capacity. In general, such complicated lithium oxide compounds contain the first-row t ransition metals (including Mn, Fe, Co, and Ni), for example, LiCoO2 is 140 mAh g−1, LiMn2O4 and its variants (LMO) are 100–120 mAh g−1, and LiFePO4 (LFP) is 150–170 mAh g−1 [51,52]. Cathode materials should meet other following requirements: high discharge voltage, high energy capacity, long cycle life, high power density, lightweight, low self-discharge, and absence of environmentally hazardous elements. V2O5 is also one of the potential materials used for cathode electrode, which is successfully synthesized by several methods, such as green route, green method, sol-gel, chemical precipitation, ultrasound-assisted method, and thermal decomposition. For the lithium-ion battery, V2O5 from the microwave-assisted green route clearly displays the specific capacity (225 mAh g−1) at 1.5–4.0 V [53,54].
As potential electrolyte candidates, these materials exhibit the large ionic conductivity of above 10 −4 S cm−1 at room temperature, the negligible electronic conductivity with a high ionic transference number , and the wide electrochemical stability windows . Many types of Li-ion solid electrolytes are verified to possess the above-mentioned properties through the long-time experimental tests, including Na super-ionic conductor (NASICON) , garnet , perovskite , LISICON , LiPON , Li3N , sulfide , argyrodite , anti-perovskite , and so on. Among these systems, LISICON and LiPON types obviously show the low ionic conductivities (~10 –6 to 10 –5 S cm−1), but good at the electrochemical stability. Li3N type exhibits the reasonable ionic conductivities (~10 –4 S cm−1), but the narrow electrochemical stability . The sulfide-, argyrodite-, and anti-perovskite-type solid electrolytes might be unstable in the ambient atmosphere, although they present the high ionic conductivities (~10 –5 to 10 –2, ~10 –7 to 10 –2, and ~10 –4 –10 –2 S cm−1, respectively). In general, NASICON-, garnet-, and perovskite-type solid electrolytes are promising for applications in solid-state batteries because of their performances in electrochemical stability and acceptable ionic conductivities (~10 –4 to 10 –2, ~10 –4 to 10 –3, and ~10 –5 to 10 –4 S cm−1, respectively). For the battery safety, the suitable selection of solid electrolytes has to be done carefully, according to the great reduction in interface resistance. However, Li+-ion-based batteries are required to be encapsulated in avoiding contamination from the ambient environment, which could lead to a decrease in ionic conductivity and change of structure. Solid electrolytes must improve their properties and make compatibly between solid electrolytes and electrodes. Basic science research will be very useful in greatly enhancing the performance of various batteries and their high potential applications. The critical physical, chemical, and material mechanisms, which are closely related to the efficiencies of cathodes, electrolytes, and anodes, cannot be clearly identified from the previous published works up to now, such as the significant roles of the nonuniform environment (the Moire superlattice; [89–91]), the multi-/single-orbital hybridizations of chemical bonds, and the intercalation/substitution of transport ions. The theoretical frameworks, being suitable for the systematic investigations, could be developed in the near-future studies. From the physical points of view, the essential properties have been successfully explored by using the first-principles simulations [92,93] and the phenomenological models . However, such methods need to be strongly modified in most of the emergent materials. The former is available for studying the optimal geometries, electronic properties, magnetic configurations, mechanical stains, phonon spectra, optical absorptions, and Coulomb excitations. It evaluates a lot of reliable data, in which the very close integration of all the useful data would become the most important strategy in the near-future studies. For example, Chapters 2 and 5–7 develop a theoretical framework and can account for the diverse phenomena through the identified orbital hybridizations and spin distributions. On the contrary, the tight-binding model [94,95], the static/dynamic Kubo formula , and the random-phase approximations , respectively, deal with the electronic, transport/optical, and Coulomb excitation properties. Each model might be very difficult for most of the complicated compounds with many atoms in a unit cell. The direct combination of the first and second methods would play the critical roles for the full understanding of ion transports among the different materials. Both physical
Lithium-Ion Batteries and Solar Cells
TABLE 1.1 Various Anodes, Electrolytes, and Cathodes in Li-Ion-Based Batteries Anode
TiO2 Graphite Patterned Si Si film Carbon nanotubes Carbon nanofibers Si nanowires Si nanotubes Li4Ti5O12 MoO3 SnO2 ZnO Fe3O4/carbon foam MnO Co3O4 GaSx MoS2 V2O5 LiCoO2 Nano-LiCoO2 LiMn2O4 Li[Li0.20Mn0.54Ni0.13Co0.13]O2 LiNi1/3Mn1/3Co1/3O2 LiMn1.5Ni0.5O4 0.5Li2MnO3·0.5LiNi0.375Mn0.375Co0.25O2 Li1.2Ni0.2Mn0.6O2 LiNi0.5Mn1.5O4 FePO4 LiFe(Co/Ni)PO4 Garnet (Li7La3Zr2O12) Perovskite (Li3xLa2/3−xTiO3) Na super-ionic conductor (NASICON) LISICON (LiMIV 2 (PO4)3 (MIV = Ti, Zr, Ge, and Hf) LiAlOx Li3PO4 Lithium silicate Li (Ta/Nb)O3 Li3N LiSiAlO2 Sulfide (Li4GeS4, Li10GeP2S12, Li2S-P2S5 Argyrodite (Li6PS5X (X = Cl, Br, I)) Anti-perovskite (Li3OX (X = Cl, Br, I)) LiSi/Ge/SnO
    [31,32]  [36,37]         [48,49]  [53,54] [55,56]    [60,61] [62,63]           [76,77]   [80,81]      [87,88]
interactions and chemical actions frequently come to exist at any position and time during the charging and discharging processes. Their simultaneous considerations in the generalized model must be an extreme challenge. The organization of this work is as follows. Chapter 1 includes the total motivations, especially for the whole developments in the theoretical and experimental researches. As for the former, the machine learning, which is built from the close association of the SMILES format and the neural network, is utilized to explore the best liquid-state electrolytes with the high-voltage lithium-ion batteries. Electron affinity and ionization energy are two critical parameters to choose the most outstanding one from a lot of potential materials. The first-principles calculations are covered in Chapters 3–7. Specifically, Chapter 3 thoroughly explores the nitrogen doping on the vacancies of monolayer graphene and its effects on the storage capacity of Li/Na. The various defects and N-concentrations are taken into consideration. Chapters 4–7, being, respectively, done for LiCo/NiO, LiSiO, LiTiO, and graphite alkali-intercalation compounds, fully investigate the geometric structures, electronic properties, and magnetic configurations of the solid-state cathode/electrolyte/ anode materials. The accurate VASP calculations and analyses are achieved from the optimal geometric symmetries, the atom-dominated electronic energy spectra, the spatial charge density distributions, the atom and orbital-projected density of states, the spin distribution configurations, the spin-split or spin-degenerate energy bands, and the atom- and orbital-dependent net magnetic moments. Consequently, the concise physical and chemical pictures, the single- and/or multi-orbital hybridizations in various chemical bonds and the spin configurations due to distinct atoms and orbitals, are clearly identified under the developed framework. The experimental syntheses and measurements are covered in Chapters 8–13. Chapter 8 is focused on how to enhance the Li+-transport performance by examining the chemisorption of ions on the un-doped/doped (B&N on vacancies)/porous graphene systems (anode materials). The different nanocarbon structures are efficiently generated through the submerged liquid plasma, as clearly illustrated in Chapter 9. This provides a simple, low capital cost, high-yield, and an environmental-friendly approach. Chapter 10 reveals an experimental overview of the usage of ILs as electrolytes for distinct chemical batteries, including the whole advantages and near-future challenges. The polyelectrolytes of lithium-ion batteries, which consist of the imidazolium-based ionogels with various amounts of IL additives, are successfully synthesized and measured in Chapter 11. Concerning solar cells, the Si-nanowire-based hybrids in Chapter 12 are modified for the great enhancement of the photovoltaic performance under the various chemical treatments, such as the doping mechanisms, the conformational changes of poly(3,4-ethylenedioxythiophene) (PEDOT) segment, the arrangement alteration of poly(3,4-ethylenedioxythiophene): poly(styrenesulfonate) (PEDOT:PSS), and the removal of excess insulating PSS chains from the PEDOT:PSS film. Chapter 13 presents the enhanced photon-to-electron conversion efficiency for the back-contact perovskite solar cells. Chapters 14 and 15, respectively, cover concluding remarks and open issues, especially for the latter in the near-future researches. Finally, the battery-related practice problems are stated in Chapter 16. In recent years, there has been a dramatic proliferation of research concerned with machine learning and application of that technology to material science. It is
Lithium-Ion Batteries and Solar Cells
considered as a powerful method, which allows the screening of huge amount of materials to find out the candidates – a process that would take several years or even decades by conventional calculations or experimental techniques. Nowadays, machine learning technology has almost been applied to all aspects of human living to get a smarter and better life. Batteries is one of its potential applications, especially LIBs that are in high demand to solve the environmental issue. Machine learning has been utilized for battery designs based on the properties such as C-rate, electrode thickness, and porosity, which affect the specific power and specific energy of LIBs . Moreover, it has been used to search for high ionic conductivity solid electrolytes  and predict the suitable inorganic solid electrolytes to prevent the dendrite formation with Li metal anode in LIBs . It is worth knowing that highperformance electrolyte molecules that can enable high-voltage battery are also an attracted issue that machine learning can involve in. For a more detailed discussion on the metrics for molecular selection, different training and predicting models can thus help to accelerate the research progress. Nitrogen doping into graphene-based anode materials has been found to effectively enhance the specific capacity of Li/Na-ion batteries, but the mechanisms remain unclear so far. Our results based on the first-principles calculations indicate that introducing N-dopants in graphene can lower down the formation energy of defects and in turn increase the amount of active sites in graphene for Li/Na-adsorption. However, our calculations also found that adding too many N-dopants in graphene may lead to N-aggregation near defect sites and further reduce the reversible Li/Na-storage capacity. Despite the disadvantage coming from the excess amount of N-dopants, an appropriate amount of N-dopants can effectively lift the migration energy barrier of vacancy defects in graphene, which can avoid vacancy aggregation and suppress the loss of reversible Li/Na-capacity. Batteries [101,102], which are driven by the electric supply and chemical energy, have become one of the mainstream energy resources. Up to date, the whole experimental progress clearly shows that the Li+- [101–103], Al+- [104,105], and Fe+-based systems  present the rich merits in the separate functionalities. Specifically, there exist a lot of frequently commercialized products for the first kind of ion transports, e.g., radios [107,108], clocks, cell telephones, notebooks, iPods, modulated planes [107,108], and buses/vehicles [109,110]. All the batteries consist of the critical anode, cathode, and electrolyte materials. Very interesting, the Li+-ion-based batteries might be made up of LiTiO/LiScO/graphite [111–113], LiFe/Co/NiO [114–117], and LiSi/Ge/LiSnO [118–120], respectively. The different combinations of three critical components would have many merits and drawbacks, according to the highperformance criteria. The previous studies show that most of the subsystems have been investigated by the first-principles calculations for their essential properties. For example, the pristine and Li-atom-intercalation graphite systems exhibit the semimetallic and metallic behaviors , respectively, in which the flexible interlayer spacings provide the ion/atom intercalation during the charging and discharging processes . Another anode material, LiTiO, is thoroughly explored in Chapter 4 for the geometric, electronic, and magnetic properties. Maybe, this system provides the excellent heterojunction using the electrolyte of lithium oxide compounds . The important differences with graphite are worthy of detailed discussions .
According to the viewpoints of experimental developments and potential applications, batteries  have become one of the mainstream energy resources . Their charging and discharging processes mainly arise from the rapid ion transports in the internal circuit, such as the quick flowing of lithium/aluminum/ iron ions [127–129], depending on their special functionalities. Up to now, a lot of high-resolution experimental measurements on the Li+-ion-based batteries can provide the necessary information for their fundamental properties; furthermore, they are frequently used in commercialized products. Each battery, at least, consists of three independent components, namely, electrolyte , cathode , and anode compounds. Specifically, the first ones could be in the solid or liquid state, while the latter are very popular in everyday living. All the solid-state Li+-ion-based batteries are thoroughly illustrated in Chapter 4, especially for the electrolyte of 3D ternary Li2SiO3 compound. The previous few theoretical studies are conducted on its geometric and electronic properties through the first-principles calculations. The delicate results and analyses are thoroughly absent up to now. That is to say, the calculated results are insufficient and there are no critical mechanisms (concise physical pictures) in comprehending the diversified phenomena. These drawbacks will be fully solved by developing a generalized theoretical framework (details in Chapter 4). The predicted properties could be further verified by the experimental examinations, e.g., lattice symmetries and valence band energy spectra, respectively, through the X-ray diffraction  and angle-resolve photoemission spectroscopy. Most important, the close and complex relations among electrolyte, cathode, and anode of LiXO-related systems are also discussed in detail. They are worthy of the systematic investigations in the near-future studies. Recently, there are plenty of experimental [133,134] and theoretical researches  on the emergent green energy materials for the great reduction of the room temperature effects . Obviously, the current results show that the successful applications have covered the battery-driven electrochemical devices , the solar energy companies , the hydrogen-operated cars , the methane-gas-created biological energies , the water-induced electric power , the wind turbines , and so on. Specifically, the chemical batteries mainly originate from the ion transports, in which both Li+- and Al+-related [143–145] ones are frequently utilized the different commercialized products, strongly depending on their functionalities. Their critical components consist of the cathode, electrolyte, and anode materials [146–148]. Most important, the charging process starts from the release of ions due to the first subsystem, transports through the second one, and then intercalates into the third one. The opposite is true for the discharging process. The high performance will be evaluated according to the large current density of ions, the negligible electronic current, the wide voltage range, the outstanding matches of different subsystems, the rapid charging/discharging processes, the long lifetime, and the high safety. Three kinds of subsystems, which belong to the lithium oxide compounds, are suitable and reliable in the practical applications, for example, the 3D ternary compounds of LiFe/Co/NiO, LiSi/Ge/SnO, and LiTi/ScO/graphite, respectively, serve as cathode, electrolyte, and anode materials. The first systems are chosen for a model study in Chapter 6 for their essential properties through the VASP calculations. The previous few studies are insufficient in fully comprehending the diversified physical,
Lithium-Ion Batteries and Solar Cells
chemical, and material phenomena. However, the important multi-orbital hybridizations and the atom- and orbital-dependent spin configurations will be proposed under the developed theoretical framework. The created viewpoints could be generalized to the emergent materials even in the presence of external fields and chemical modifications. A bulk graphite is frequently utilized in the commercialized anode material of Li+-ion-based batteries , mainly owing to its layered structure. This condensed matter system has been extensively studied both experimentally and theoretically. In the natural environment, most of the pure graphitic materials exhibit the AB-stacked configuration; that is, they belong to the Bernal graphite . Only a few of them have the ABC-stacking configuration . Recently, the simple hexagonal graphite, with the AA stacking, could be synthesized in the experimental laboratories. Three kinds of graphite systems are semimetals, since the van der Waals interlayer interactions can create a significant overlap of valence and conduction band near the Fermi level. The free conduction electrons and valence holes are responsible for the diversified physical, chemical, and material phenomena. The AA  and ABC stackings, respectively, corresponding to the highest and lowest symmetries, possess the highest and lowest free carrier densities. By the delicate theoretical calculations and analyses, each graphitic sheet presents a very strong σ bonding of C-(2s, 2px, 2py) orbitals, being accompanied with the relatively weak π bondings of C-2pz orbitals along the perpendicular direction. Apparently, the interlayer spacings are easily modulated by the atom, molecule, and ion intercalations. Such metastable geometric structures might be very suitable for the Li+-ion (or Li-atom) intercalation/de-intercalation during the charging/discharging processes. Graphite intercalation compounds have been fully explored more than forty, in which they are classified into the donor- and acceptor-type behaviors under the n- and p-type dopings, respectively. For example, the alkali-atom intercalation leads to high electrical conductivities, as best as copper. Up to now, there are some numerical simulations and phenomenological models on the essential properties of stage-n graphite alkali-intercalation compounds. However, the unusual relations among the stacking configurations, the intercalant concentrations, the atom-dominated band structures, the atom- and orbital-decomposed density of states, and the spatial charge density distributions are worthy of the further investigations through the first-principles calculations (details in Chapter 7). Recently, graphene [153–155] has attracted a lot of interest among the LIB community because of their outstanding electrochemical performance. Graphene is attributed to high surface area, excellent electrical conductivity, flexibility, and Li-ions can intercalate on both the sides and edges of the graphene to yield high electrochemical performance. Graphene can also be doped with other elements such as B/N  or the overall microstructure can be modified [157,158] to enhance the overall capacity and rate capability of the battery. Here, we discuss the variety of synthesis procedure used to prepare graphene and investigate the structure/microstructure/bond vibration and electrochemical properties. Fossil fuels are the most widely used energy resource worldwide. Risks related to resource depletion, environmental pollution, and political unrest with regard to fossil fuel production have led to the rapid emergence of a variety of intermittent renewable and cleaner energy sources such as wind, solar, and wave. In order to integrate these
renewable energies into the electrical grid, a large-scale energy storage system (ESS) is vital to peak shift operation . Among various energy storage technologies, using an electrochemical secondary battery is a promising method for large-scale storage of electricity due to its flexibility, high energy conversion efficiency, and simple maintenance . Lithium-ion batteries (LIBs), which have become common power sources in the portable electronic market since their first commercialization by Sony in the early 1990s, are the primary candidates for ESSs . The introduction of LIBs into the automotive market as the battery of choice for powering hybrid electric vehicles (HEVs), plug-in hybrid electric vehicles (PHEVs), and EVs could reduce dependence on fossil fuels. Although LIBs are the most commonly used for consumer portable electronic devices and are promising for the next-generation large-scale charge storage due to their outstanding energy density and power capacity [162–167], there are still some drawbacks regarding lithium battery safety, lifetime, poor low-temperature performance, and cost. Moreover, the popularity, as well as increasing demand for LIBs with geographically, constrained that Li-mineral resources will drive up the price. Therefore, findings to replace LIBs in the future have attracted a lot of attention of scientists. With the large natural abundance and low cost of sodium, sodium-ion batteries (SIBs) have become a promising candidate for large-scale usage related to energy storage belong to renewable energy sources. In addition, Na and Li have similar chemical properties, and thus, comprehensive knowledge about LIBs can be applied, then making SIBs become competitive to LIBs in cell markets [168–170]. However, the performance of SIBs is still a challenge with respect to scientists, and research conducted on Na-based chemistry is remarkably less compared to that on Li-based chemistry. Further study on electrode materials, electrolytes, and electrode– electrolyte interphase as well as in-depth mechanism, especially safety is required to improve the behavior of SIBs [171,172]. A serious issue in lithium-ion cell technology is safety. Electrodes and electrolytes are both hazard factors in Li-ion cells. In particular, the use of graphite-based electrodes easily leads to the release upon cycling of gaseous products or even more dangerously to lithium plating on the electrode surface at high current regimes. However, electrolytes are the most critical components for the control of the safety of LIBs because of the high vapor pressure and the flammability of the organic solvents in electrolytes. One of the best ways to improve the safety and reliability of the Li-ion battery electrolytes is the use of an emerging class of electrolytes based on ionic liquids (ILs), namely low-temperature molten salts. The ILs are nonvolatile, nonflammable, highly conductive, environmentally compatible, and can safely operate in a wide temperature range. This unique combination of favorable properties makes ILs very appealing materials for stable and safe electrolytes in lithium batteries to reduce the risk of thermal runaways and, eventually, fire accidents, thus drastically improving the overall safety of the cell. Batteries have been developed for more than 100 years and have a great impact on our daily life. Recently, due to the use of mobile devices, a battery with high capacity and high safety is especially in demand. Apart from mobile devices, EVs are now ready to market and also in need of batteries with high capacity as well as
Lithium-Ion Batteries and Solar Cells
high energy density. The LIBs possess the above-mentioned properties; it is now the most promising candidate for commercialization [173–176]. Electrolytes are the most important in batteries, as they carry ions between a pair of electrodes to complete a circuit of charges. The commercial electrolytes are the mixtures of carbonates and lithium salts; however, volatility and flammability are big problems to these kinds of liquid electrolytes [177–179]. To solve this, it is worth researching other materials to replace liquid electrolytes. The ILs have attracted lots of attention to be the suitable solution of these disadvantages due to their negligible flammability, broad electrochemical window, and vapor pressure, which are especially in demand of the electrolytes for the next-generation batteries [180–187]. Poly(ionic liquid)s (PILs), which are macromolecular analogs of ILs, have emerged as a new class of polymer electrolytes due to their combined properties emanating from the IL units and their intrinsic polymeric nature. For IL-based electrolytes, there is a balance between their ionic conductivities and mechanical properties depending on the composition ratio of the polymer phase and additive phase [188–193]. Hence, a membrane composed of a polymer matrix, lithium salt, and IL may have the potential to optimize the system of electrolyte. We demonstrated the preparation of new imidazolium-based ionogels through photopolymerization of 1-ethyl3-vinylimidazolium bis(trifluoromethanesulfonylimide) with poly(ethylene glycol) diacrylate (PEGDA) (Mn = 700 g mol−1), poly(ethylene glycol) methyl ether methacrylate (PEGME) (Mn = 500 g mol−1), and lithium bis(trifluoromethanesulfonyl)imide (LiTFSI) in an IL to obtain mechanically robust membranes. And, their use as the electrolyte system for Li/LiFePO4 cells was studied in particular. Additionally, the thermal stabilities and electrical properties, such as ionic conductivity, electrochemical stability as well as the charge/discharge test of the Li/LiFePO4 cells based on these materials, will also be discussed in the main article. Solar energy is one of the sources offering clean, sustainable, and stable energy. In recent years, Si-based solar cells have been widely used, but it requires a fairly complex process. Therefore, the various types of emerging solar cells and experimental syntheses have been proposed to fully present the essential properties, outstanding functionalities, and commercialized products of green energy materials. From various materials acquired for emerging-cell construction, the arrangement of PEDOT:PSS polymer and n-type crystalline Si was proposed as the preference in hybrid structures considering the superiorities in fabrication aspect, reliability, and sound efficiency. Moreover, many approaches to improve the performance of these hybrid solar cells were discovered as well [194,195]. The PEDOT:PSS material as the p-type layer in this type of cell arrangement surely to have an important impact in the junction section, however, a pristine PEDOT:PSS layer exhibits low electrical conductivity, with a value in the range of 0.2 to 10 S cm−1, which particularly causes the poor device performance in photovoltaic applications. In addition, the deposition on hydrophobic substrates generally yields the nonuniform contact. Therefore, the low-cost, safety, and facile route to enhance the electrical also the adhesion capability of pristine PEDOT:PSS is still in progress. The chemical treatment is highly demanded which allows the low-cost and large-area production based on the solution-processing capability such as by using ethylene glycol (EG) and fluorosurfactant [196,197]. Up to now, there exist several well-established reports
that cover the discussion of treated PEDOT:PSS on planar Si for cell design and proven to improve the photovoltaic performance [198,199]. However, the research for combining PEDOT:PSS thin film with nanowires (SiNWs) is still limited. SiNWs are known to have a light-trapping effect to enable the optimization of incoming light transmitted from the transparent PEDOT:PSS layer . Therefore, PEDOT:PSS/ Sen has been considered an efficient way for the construction of high-performance hybrid solar cells. This study thoroughly explores the diversified physical, chemical, and material phenomena of fundamental properties and the unusual functionalities in PEDOT:PSS films and Si-nanowire-based solar cells. Furthermore, the relations between the theoretical and practical analyses are fully discussed. It is expected to be capable of providing very useful information about science fundamentals, integrated engineering, and real application. The organization of this chapter is as follows. The beginning of the chapter includes the introduction, especially for the various developments in the theoretical and experimental researches. As for the chapter former, the synthesis, structure, and electrical properties of the as-prepared PEDOT:PSS layer is discussed in the following subchapter. The principles of “Baytron P” routes as the most fundamentally convenient PEDOT-based compound fabrication procedure are explained into consideration . Moreover, related to structure and electrical properties, the PSS functions in commercial PEDOT:PSS complex clearly identified under a comprehensive framework [202,203]. The adjustment into higher conductivity values using diverse methods including physical treatment or chemical process is defined in the next discussion [204–206]. Furthermore, the experimental syntheses and measurements are covered in the third subchapter which is focused on how to enhance the pristine PEDOT:PSS conductivity in affordable routes followed by various analyses using four-point probe, Raman spectroscopy, XPS, and many more. The addition of EG into precursors results in the optimum conductivity up to 103 order of magnitude for the reduction of sheet resistance. Concerning the application, the Si-nanowire-based hybrid cells are modified for the great enhancement of the photovoltaic performance under doping mechanisms, the conformational changes of PEDOT segment, the arrangement alteration of PEDOT:PSS, and the removal of excess insulating PSS chains from the PEDOT:PSS film achieving >14% can be realized.
REFERENCES 1. Wu X., Kang F., Duan W., Lia J., Progress in Natural Science: Materials International, 2019, 29, 247–255. 2. Kang J., Kim K. C., Jang S. S., The Journal of Physical Chemistry C, 2018, 122, 10675−10681. 3. Yang S.-J., Qin X.-Y., He R., Shen W., Li M., Zhao L.-B., Physical Chemistry Chemical Physics, 2017, 19, 12480–12489. 4. Urban A., Seo D.-H., Ceder G., npj Computational Materials, 2016, 2, 16002. 5. Meng Y. S., Dompablo M. E. A., Energy and Environmental Science, 2009, 2, 589–609. 6. Zhao Y., Li X., Yan B., Xiong D., Li D., Lawes S., Sun X., Advanced Energy Materials, 2016, 6(1–19), 1502175.
Lithium-Ion Batteries and Solar Cells
7. Deng D., Energy Science and Engineering, 2015, 3(5), 385–418. 8. Wu S., Xu R., Lu M., Ge R., Iocozzia J., Han C., Jiang B., Lin Z., Advanced Energy Materials, 2015, 5(21), 1–40. 9. Goriparti S., Miele E., Angelis F. D., Fabrizio E. D., Zaccaria R. P, Capiglia C., Journal of Power Sources, 2014, 257, 421–443 10. Chen J., Materials, 2013, 6, 156–183. 11. Etacheri V., Marom R., Elazari R., Salitra G., Aurbach D., Energy and Environmental Science, 2011, 4, 3243. 12. Zhao W., Yi J., He P., Zhou H., Electrochemical Energy Reviews, 2019, 2, 574–605. 13. Takami N., Sekino M., Ohsaki T., Kanda M., Yamamoto M., Journal of Power Sources, 2001, 97–98, 677–680. 14. Xu Z., Yang J., Li H., Nuli Y., Wang J., Journal of Materials Chemistry A, 2019, 7, 9432. 15. Ullah A., Majid A., Rani N., Journal of Energy Chemistry, 2018, 27, 219–237. 16. Haskins J. B., Lawson J. W., The Journal of Chemical Physics, 2016, 144, 184707. 17. Bhattacharya S., John S., Scientific Reports, 2019, 9, 12482. 18. Duan J., Xu H., Sha W. E. I., Zhao Y., Wang Y., Yang X., Tang Q., Journal of Materials Chemistry A, 2019, 7, 21036–21068. 19. Cheah S. K., et al., Nano Letters, 2009, 9, 3230. 20. Wang W., Tian M., Abdulagatov A., George S. M., Lee Y. C., Yang R., Nano Letters, 2012, 12, 655. 21. Ban C., Xie M., Sun X., Travis J. J., Wang G., Sun H., Dillon A. C., Lian J., George S. M., Nanotechnology, 2013, 24, 424002. 22. Kim S. W., Han T. H., Kim J., Gwon H., Moon H. S., Kang S. W., Kim S. O., Kang K., ACS Nano, 2009, 3, 1085. 23. Jung Y. S., Cavanagh A. S., Riley L. A., Kang S. H., Dillon A. C., Groner M. D., George S. M., Lee S. H., Advanced Materials, 2010, 22, 2172. 24. Lee M.-L., Su C.-Y., Lin Y.-H., Liao S.-C., Chen J.-M., Perng T.-P., Yeh J.-W., Shih H. C., Journal of Power Sources, 2013, 244, 410–416. 25. Wang H.-Y., Wang F.-M., Journal of Power Sources, 2013, 233, 1. 26. Goriparti S., Miele E., De Angelis F., Di Fabrizio E., Zaccaria R. P., Capiglia C., Journal of Power Sources, 2014, 257, 421–443. 27. Liu Y., Wang Y. M., Yakobson B. I., Wood B. C., Physical Review Letters, 2014, 113, 28304. 28. Raccichini R., Varzi A., Passerini S., Scrosati B., Nature Materials, 2015, 14, 271–279. 29. He Y., Yu X., Wang Y., Li H., Huang X., Advanced Materials, 2011, 23, 4938. 30. Xiao X., Lu P., Ahn D., Advanced Materials, 2011, 23, 3911. 31. Chen S., Chen P., Wang, Y., Nanoscale, 2011, 3(10), 4323. 32. Liu C., Li F., Ma L.-P., Cheng H.-M., Advanced Materials, 2010, 22, 28. 33. Yoon S.-H., Park C.-W., Yang H., Korai Y., Mochida I., Baker R. T. K., Rodriguez N. M., Carbon, 2004, 42, 21. 34. Yan X., Teng D., Jia X., Yu Y., Yang X., Electrochimica Acta, 2013, 108, 196. 35. Yue H., Li F., Yang Z., Tang J., Li X., He D., Materials Letters, 2014, 120, 39. 36. Kohandehghan A., Kalisvaart P., Cui K., Kupsta M., Memarzadeh E., Mitlin D., Journal of Materials Chemistry A, 2013, 1, 12850. 37. Lotfabad E. M., Kalisvaart P., Cui K., Kohandehghan A., Kupsta M., Olsen B., Mitlin D., Physical Chemistry Chemical Physics, 2013, 15 13646. 38. Lotfabad E. M., Kalisvaart P., Kohandehghan A., Cui K., Kupsta M., Farbod B., Mitlin D., Journal of Materials Chemistry A, 2014, 2, 2504. 39. Snyder M. Q., Trebukhova S. A., Ravdel B., Wheeler M. C., DiCarlo J., Tripp C. P., DeSisto W. J., Journal of Power Sources, 2007, 165, 379. 40. Liu J., Li X., Cai M., Li R., Sun X., Electrochimica Acta, 2013, 93, 195. 41. Ahn D., Xiao X., Electrochemistry Communications, 2011, 13, 796.
42. Riley L. A., Cavanagh A. S., George S. M., Jung Y. S., Yan Y., Lee S. H., Dillon A. C., ChemPhysChem, 2010, 11, 2124. 43. Wang D., Yang J., Liu J., Li X., Li R., Cai M., Sham T.-K., Sun X., Journal of Materials Chemistry A, 2014, 2, 2306. 44. Lee J.-H., Hon M.-H., Chung Y.-W., Leu I.-C., Applied Physics A, 2010, 102, 545. 45. Kang E., Jung Y. S., Cavanagh A. S., Kim G.-H., George S. M., Dillon A. C., Kim J. K., Lee J., Advanced Functional Materials, 2011, 21, 2430. 46. Lipson A. L., Puntambekar K., Comstock D. J., Meng X., Geier M. L., Elam J. W., Hersam M. C., Chemistry of Materials, 2014, 26, 935. 47. Meng X., Liu J., Li X., Banis M. N., Yang J., Li R., Sun X., RSC Advances, 2013, 3, 7285. 48. Meng X., Libera J. A., Fister T. T., Zhou H., Hedlund J. K., Fenter P., Elam J. W., Chemistry of Materials, 2014, 26, 1029. 49. Meng X., et al., Advanced Functional Materials, 2014, 24, 158. 50. Li S., Ping Liu P., Huang X. B., Tang Y. G., Wang, H.-Y., Journal of Materials Chemistry A, 2019, 7, 10988. 51. Dimesso L., et al., Chemical Society Reviews, 2012, 41, 5068. 52. Wang J., Sun X., Energy and Environmental Science, 2012, 5, 5163. 53. Liu D., Liu Y., Pan A., Nagle K. P., Seidler G. T., Jeong Y.-H., Cao G., The Journal of Physical Chemistry C, 2011, 115(11), 4959. 54. Karthik K., Phuruangrat A., Chowdhury Z. Z., Pradeeswari K., Kumar R. M., Journals of Science, 2019. 55. Donders M. E., Arnoldbik W. M., Knoops H. C. M., Kessels W. M. M., Notten P. H. L., Journal of the Electrochemical Society, 2013, 160, A3066. 56. Xie J., Zhao J., Liu Y., Wang H., Liu C., Wu T., Hsu P.-C., Lin D. C., Jin Y., Cui Y., Nano Research, 2017, 10(11), 3754. 57. Scott I D., Jung Y. S., Cavanagh A. S., Yan Y., Dillon A. C., George S. M., Lee S. H., Nano Letters, 2011, 11, 414. 58. Miikkulainen V., Ruud A., Østreng E., Nilsen O., Laitinen M., Sajavaara T., Fjellvåg H., The Journal of Physical Chemistry C, 2014, 118, 1258. 59. Seok Jung Y., Cavanagh A. S., Yan Y., George S. M., Manthiram A., Journal of the Electrochemical Society, 2011, 158, A1298. 60. Riley L. A., Van Atta S., Cavanagh A. S., Yan Y., George S. M., Liu P., Dillon A. C., Lee S.-H., Journal of Power Sources, 2011, 196, 3317. 61. Li X., Liu J., Banis M. N., Lushington A., Li R., Cai M., Sun X., Energy and Environmental Science, 2014, 7, 768. 62. Park J. S., Meng X., Elam J. W., Hao S., Wolverton C., Kim C., Cabana J., Chemistry of Materials, 2014, 26, 3128. 63. Xiao X., Ahn D., Liu Z., Kim J.-H., Lu P., Electrochemistry Communications, 2013, 32, 31. 64. Bettge M., Li Y., Sankaran B., Rago N. D., Spila T., Haasch R. T., Petrov I., Abraham D. P., Journals of Power Sources, 2013, 233, 346. 65. Zhang X., Belharouak I., Li L., Lei Y., Elam J. W., Nie A., Chen X., Yassar R. S., Axelbaum R. L., Advanced Energy Materials, 2013, 3, 1299. 66. Park J. S., Meng X., Elam J. W., Hao S., Wolverton C., Kim C., Cabana J., Chemistry of Materials, 2014, 26, 3128. 67. Gandrud K. B., Pettersen A., Nilsen O., Fjellvåg H., Journal of Materials Chemistry A, 2013, 1, 9054. 68. Liu J., Banis M. N., Sun Q., Lushington A., Li R., Sham T. K., Sun X., Advanced Materials, 2014, 26, 6472. 69. Zheng F., Kotobuki M., Songa S.-F., Lai M. O., Lu L., Journal of Power Sources, 2018, 389, 198.
Lithium-Ion Batteries and Solar Cells
70. Chen C., Xie S., Sperling E., Yang A., Henriksen G., Amine K., Solid State Ionics, 2004, 167, 263. 71. Aaltonen T., Alnes M., Nilsen O., Costelle L., Fjellvåg H., Journal of Materials Chemistry, 2010, 20, 2877. 72. Chen C., Amine K., Solid State Ionics, 2001, 144, 51. 73. Aatiq A., Ménétrier M., Croguennec L., Suard E., Delmas C., Journal of Materials Chemistry, 2002, 12, 2971. 74. Deng, Y. et al., ACS Applied Materials and Interfaces, 2017, 9, 7050. 75. Thangadurai V., Weppner W., Ionics, 2006, 12, 81. 76. Aaltonen T., Nilsen O., Magrasó A., Fjellvåg H., Chemistry of Materials, 2011, 23, 4669. 77. Comstock D. J., Elam J. W., The Journal of Physical Chemistry C, 2013, 117, 1677. 78. Hamalainen J., Holopainen J., Munnik F., Hatanpaa T., Heikkila M., Ritala M., Leskela M., Journal of the Electrochemical Society, 2012, 159, A259. 79. Hämäläinen J., Munnik F., Hatanpää T., Holopainen J., Ritala M., Leskelä M., Journal of Vacuum Science and Technology A, 2012, 30, 01A106. 80. Liu J., Banis M. N., Li X., Lushington A., Cai M., Li R., Sham T.-K., Sun X., The Journal of Physical Chemistry C, 2013, 117, 20260. 81. Østreng E., Sønsteby H. H., Sajavaara T., Nilsen O., Fjellvåg H., Journal of Materials Chemistry C, 2013, 1, 4283. 82. Østreng E., Vajeeston P., Nilsen O., Fjellvåg H., RSC Advances, 2012, 2, 6315. 83. Perng Y.-C., Cho J., Sun S. Y., Membreno D., Cirigliano N., Dunn B., Chang J. P., Journal of Materials Chemistry A, 2014, 2, 9566. 84. Kamaya N., Homma K., Yamakawa Y., Hirayama M., Kanno R., Yonemura M., Kamiyama T., Kato Y., Hama S., Kawamoto K., Nature Materials, 2011, 10, 682. 85. Boulineau S., Courty M., Tarascon J.-M., Viallet V., Solid State Ionics, 2012, 221, 1. 86. Zhao Y., Daemen L. L., Journal of the American Chemical Society, 2012, 134, 15042. 87. Tang T., Chen P., Luo W., Luo D., Wang Y., Journal of Nuclear Materials, 2012, 420, 31. 88. Ma S. G., Shen Y.-H., Kong X.-G., Gao T., Chen X.-J., Xiao C.-J., Lu T.-C., Mater Design, 2017, 118, 218. 89. Tada, K., Kitta, M., Ozaki, H., Tanaka, S. Chemical Physics Letters, 2019, 731, 136598. 90. Haregewoin, A. M., Wotango, A. S., Hwang, B., Journal of Energy and Environmental Science, 2016, 9(6), 1955. 91. Khan S. A., Shahid Ali S., Khalid Saeed S., Muhammad Usman M., Khan I., Journal of Materials Chemistry A, 2019, 7, 10159. 92. Lin S. Y., Tran N. T. T., Chang S. L., Chuu C. P., Lin M. F., Structure- and AdatomEnriched Essential Properties of Graphene Nanoribbons, CRC Press, Boca Raton, FL, 2017. 93. Tran N. T. T., Lin S. Y., Lin C. Y., Lin M. F., Geometric and Electronic Properties of Graphene-Related Systems: Chemical Bondings, CRC Press, Boca Raton, FL, 2017. 94. Lin C. Y., Chen R. B., Ho Y. H., Lin M. F., Electronic and Optical Properties of Graphite-Related Systems, CRC Press, Boca Raton, FL, 2017. 95. Grotendorst J., Attig N., Blugel S., Marx D., Multiscale Simulation Methods in Molecular Sciences, NIC Series, Winter School Forschungszentrum Jülich March 2009, 42, pp. 2–6. 96. Nakayama T., Shima H., Physical Review E, 1998, 58(3), 3984. 97. Chen G. P., Voora V. K., Agee M. M., Balasubramani S. G., Furche F., Annual Review of Physical Chemistry, 2017, 68, 421. 98. Wu, B., Han, S., Shin, K. G., Lu, W., Journal of Power Sources 2018, 395, 128–136. 99. Sendek, A. D., Yang, Q., Cubuk, E. D., Duerloo, K. A. N., Cui, Y., Reed, E. J, Energy and Environmental Science, 2017, 10(1), 306–320.
100. Ahmad, Z., Xie, T., Maheshwari, C., Grossman, J. C., Viswanathan, V., ACS Central Science, 2018, 4(8), 996–1006. 101. Blomgren, G. E. Journal of Electrochemical Society, 2017, 164, A5019–A5025. 102. Zubi G., Dufo-López R., Carvalho M., Pasaoglu G., Renewable and Sustainable Energy Reviews, 2018, 89, 292–308. 103. Pistoia G. Lithium-Ion Batteries: Advances and Applications, 1st ed. Elsevier, Amsterdam, Netherlands, 2014. 104. Lin M.-C., Gong M., Lu B., Wu Y., Wang D.-Y., Guan M., Dai H., Nature, 2015, 520(7547), 324–328. 105. Das S. K., Mahapatra S., Lahan, H., Journal of Materials Chemistry A, 2017, 5(14), 6347–6367. 106. Ramaprabhu S., Kumar Saroja A. P. V., Samantaray, S. S., Chemical Communications, 2019, 55, 10416–10419. 107. Liang Y., Zhao C., Yuan H., Chen Y., Zhang W., Huang J., Zhang Q., InfoMat, 2019, 1(1), 6–32. 108. Pistoia, G. Batteries for Portable Devices, 1st ed. Elsevier Science, Amsterdam, Netherlands, 2005. 109. Gao Z., Lin Z., LaClair T. J., Liu C., Li J.-M., Birky A. K., Ward, J. Energy, 2017, 122, 588–600. 110. Gerssen-Gondelach S. J., Faaij A. P. C., Journal of Power Sources, 2012, 212, 111–129. 111. Liu Y., Gorgutsa S., Santato C., Skorobogatiy M., Journal of the Electrochemical Society, 2012, 159(4), A349–A356. 112. Liu Z., Deng H., Zhang S., Hu W., Gao F. Physical Chemistry Chemical Physics, 2018, 20, 22351–22358. 113. Morris R. S., Dixon B. G., Gennett T., Raffaelle R., Heben M. J., Journal of Power Sources, 2004, 138(1–2), 277–280. 114. Matsumura T., Kanno R., Inaba Y., Kawamoto Y., Takano, M. Journal of the Electrochemical Society, 2003, 149(12), A1509–A1513. 115. Qian J., Liu L., Yang J., Li S., Wang X., Zhuang H. L., Lu Y. Nature Communications, 2018, 9(1), 4918. 116. Chen H., Freeman C. L., Harding J. H., Physical Review B, 2011, 84(8), 085108. 117. Chen H., Dawson J. A., Harding J. H. Journal of Materials Chemistry A, 2014, 2(21), 7988. 118. Kuganathan N., Tsoukalas L. H., Chroneos, A. Solid State Ionics, 2019, 335, 61–66. 119. Lau J., DeBlock R. H., Butts D. M., Ashby D. S., Choi C. S., Dunn B. S. Advanced Energy Materials, 2018, 8, 1800933. 120. Sathiya M., Rousse G., Ramesha K., Laisa C. P., Vezin H., Sougrati M. T., Doublet M-L., Foix D., Gonbeau D., Walker W., Prakash A. S., Ben Hassine M., Dupont L., Tarascon J.-M. Nature Materials, 2013, 12(9), 827–835. 121. Zurek E., Jepsen O., Andersen O. K., Physical Chemistry Chemical Physics, 2005, 6, 1934. 122. Kashani H., Tian Y., Ito Y., Fujita J.-I., Oyama Y. Nature Communications, 2019, 10(1), 275. 123. Yao X., Huang B., Yin J., Peng G., Huang Z., Gao C., Liu D., Xu X., Chinese Physics B, 2016, 25(1), 018802. 124. Humana R. M., Ortiz M. G., Thomas J. E., Real S. G., Sedlarikova M., Vondrak J., Visintin A., ECS Transactions, 2014, 63(1), 91–97. 125. Zhang S.S., Journal of Power Sources, 2006, 162, 1379–139. 126. Yadroitsev I., Yadroitsava I., Le Roux S. G., 3D Printing and Additive Manufacturing. doi: 10.1089/3dp.2018.0060. 127. Kuganathan N., Tsoukalas L. H., Chroneos A., Solid State Ionics, 2019, 335, 61–66.
Lithium-Ion Batteries and Solar Cells
128. Wei J., Diaconescu P. L., Diaconescu, P. L. Macromolecules, 2017, 505, 1847–1861. 129. Deng J., Lei Y., Wen S., Chen, Z., International Journal of Mineral Processing, 2015, 140, 43–49. 130. Zhang S. S., Journal of Power Sources, 2006, 162, 1379–1394. 131. Nair J. R., et al., Electrochimica Acta, 2016, 199, 172–179. 132. du Plessis, A., Yadroitsev, I., Yadroitsava, I., Le Roux S. G., 3D Printing and Additive Manufacturing. doi: 10.1089/3dp.2018.0060. 133. GhaffarianHoseini A., Dahlan N. D., Berardi U., GhaffarianHoseini A., Makaremi N., GhaffarianHoseini M., Renewable and Sustainable Energy Reviews, 2013, 25, 1–17. 134. Greeley J., Markovic N. M., Energy and Environmental Science, 2012, 5, 9246–9256. 135. Zhang Q., Sun Y., Xu W., Zhu D. Advanced Materials, 2014, 26, 6829–6851. 136. Wang W. C., Yung Y. L., Lacis A. A., Mo T. A., Hansen, J. E. Science, 1976, 194, 685–690. 137. Orilall, M. C., Wiesner, U., Chemical Society Reviews, 2011, 40, 520–535. 138. Frey H. C., Rouphail N. M., Zhai H., Farias T. L., Gonçalves G. A. Transportation Research Part D: Transport and Environment, 2007, 12, 281–291. 139. Liu J., Barnett S. A. Solid State Ionics, 2003, 158, 11–16. 140. Prasad N. R., Ranade S. J., Hoang H. T., Phuc, N. H., December hydropower energy recovery (hyper) from water-flow systems in Vietnam. In 2012 10th International Power and Energy Conference (IPEC), Ho Chi Minh City, Vietnam, IEEE, 2012, pp. 92–97. 141. Morren J., De Haan S. W., Kling W. L., Ferreira, J. A., IEEE Transactions on Power Systems, 2006, 21, 433–434. 142. Yu Y., Gu L., Zhu C., Van Aken P. A., Maier J., Journal of the American Chemical Society, 2009, 131, 15984–15985. 143. Ambroz F., Macdonald T. J., Nann, T. Advanced Energy Materials, 2017, 7, 1602093. 144. Christiansen A. S., Johnsen R. E., Norby P., Frandsen C., Mørup S., Jensen S. H., Hansen K., Holtappels P., Journal of The Electrochemical Society, 2015, 162, A531–A537. 145. Zhang S. S. Journal of Power Sources, 2006, 162, 1379–1394. 146. Whittingham M. S. Chemical Reviews, 2004, 104, 4271–4302. 147. Stevens D. A., Dahn J. R. Journal of the Electrochemical Society, 2000, 147, 1271–1273. 148. Moura S. J., Argomedo F. B., Klein R., Mirtabatabaei A., Krstic, M., IEEE Transactions on Control Systems Technology, 2016, 25, 453–468. 149. Cheng Q., Scientific Reports, 2017, 7, 14782. 150. Lin C. Y., Wu J. Y., Chiu C. W., Lin M. F., AB-Stacked Graphenes. CRC Press, Boca Raton, FL, 2017. ISBN: 9780429277368. 151. Lin C. Y., Wu J. Y., Chiu C. W., Lin M. F. ABC-Stacked Graphenes. CRC Press, Boca Raton, FL, 2017. ISBN: 9780429277368. 152. Lin C. Y., Wu J. Y., Chiu C. W., Lin M. F. AA-Stacked Graphenes. CRC Press, Boca Raton, FL, 2017. ISBN: 9780429277368. 153. Li X., Zhi L. Chemical Society Reviews, 2018, 47, 3189–3216. 154. Xin H., Li W. Applied Physics Reviews, 2018, 5, 031105. 155. Randviir E. P., Brownson D. A. C., Banks, C. E., Materials Today, 2014, 17(9), 426–432. 156. Wu Z.-S., Ren W., Xu L., Li F., Cheng H.-M., ACS Nano, 2011, 5(7) 5463–5471. 157. Shu K., Wang C., Li S., Zhao C., Yang Y., Liu H., Wallace, G. Journal of Materials Chemistry A, 2015, 3(8), 4428–4434. 158. Han S., Wu D., Li S., Zhang F., Feng X., Advanced Materials, 2014 26(6), 849–864. 159. Dunn B., Kamath H., Tarascon J. M., Science, 2011, 334, 928–935. 160. Pan H., Hu Y.-S., Chen L., Dunn B., Kamath H., Tarascon J. M., Yang Z. G., Energy and Environmental Science, 2013, 6, 2338–2360. 161. Nishi Y., Journal of Power Sources, 2001, 100, 101–106.
162. Le P., Cointeaux L., Strobel P., Leprêtre J.-C., Judeinstein P., Alloin F., The Journal of Physical Chemistry C, 2012, 116, 7712–7718. 163. Le P., Alloin F., Strobel P., Leprêtre J.-C., Pérez del Valle C., Judeinstein P., The Journal of Physical Chemistry B, 2010, 114, 894–903. 164. Wongittharom N., Lee T.-C., Wang C.-H., Wang Y.-C., Chang J.-K., Journal of Materials Chemistry A, 2014, 2, 5655–5561. 165. Wang H., Yeh W., Wongittharom N., Wang C., Tseng J., Lee W., Chang S., Chang K., Journal of Power Sources, 2015, 274, 1016–1023. 166. Etacheri V., Marom R., Elazari R., Salitra G., Aurbach D., Energy and Environmental Science, 2011, 4, 3243–3262. 167. Yang Z., Zhang J., Kintner-Meyer M. C. W., Lu X., Choi D., Lemmon J. P., Liu J., Chemical Reviews, 2011, 111, 3577–3613. 168. Hong Y., Kim Y., Park Y., Choi A., Choi N.-S., Lee K. T., Energy and Environmental Science, 2013, 6, 2067–2081. 169. Palomares V., Serras P., Villaluenga I., Hueso K. B., Carretero-González J., Rojo T., Energy and Environmental Science, 2012, 5, 5884–5901. 170. Kim S. W., Seo D. H., Ma X., Ceder G., Kang K., Advanced Energy Materials, 2012, 2, 710–721. 171. Slater M. D., Kim D., Lee E., Johnson C. S., Advanced Functional Materials, 2013, 23, 947–958. 172. Palomares V., Casas-Cabanas M., Castillo-Martínez E., Han M. H., Rojo T., Energy and Environmental Science, 2013, 6, 2312–2337. 173. Armand M., Tarascon J. M., Nature, 2008, 451, 652–657. 174. Kang B., Ceder G., Nature, 2009, 458, 190–193. 175. Sun Y. K., Myung S. T., Park B. C., Prakash J., Belharouak I., Amine K., Nature Materials, 2009, 8, 320–324. 176. Scrosati B., Garche J., Journal of Power Sources, 2010, 195, 2419–2430. 177. Balakrishnan P. G., Ramesh R., Kumar T. P., Journal of Power Sources, 2006, 155, 401–414. 178. Goodenough J. B., Kim Y., Chemistry of Materials, 2010, 22, 587–603. 179. Lux S. F., Lucas I. T., Pollak E., Passerini S., Winter M., Kostecki R., Electrochemistry Communications, 2012, 14, 47–50. 180. Smiglak M., Reichert W. M., Holbrey J. D., Wilkes J. S., Sun L. Y., Thrasher J. S., Kirichenko K., Singh S., Katritzky A. R., Rogers R. D., Chemical Communications, 2006, 2554–2556. doi: 10.1039/b602086k, 181. Earle M. J., Esperanca J. M. S. S., Gilea M. A., Lopes J. N. C., Rebelo L. P. N., Magee J. W., Seddon K. R., Widegren J. A., Nature, 2006, 439, 831–834. 182. Nakagawa H., Fujino Y., Kozono S., Katayama Y., Nukuda T., Sakaebe H., Matsumoto H., Tatsumi K., Journal of Power Sources, 2007, 174, 1021–1026. 183. Jin Y. D., Fang S. H., Chai M., Yang L., Tachibana K., Hirano S., Journal of Power Sources, 2013, 226, 210–218. 184. Sun X. G., Liao C., Shao N., Bell J. R., Guo B. K., Luo H. M., Jiang D. E., Dai S., Journal of Power Sources, 2013, 237, 5–12. 185. Sakaebe H., Matsumoto H., Tatsumi K., Electrochimica Acta, 2007, 53, 1048–1054. 186. Fernicola A., Croce F., Scrosati B., Watanabe T., Ohno H., Journal of Power Sources, 2007, 174, 342–348. 187. Galinski M., Lewandowski A., Stepniak I., Electrochim Acta, 2006, 51, 5567–5580. 188. Yin K., Zhang Z. X., Li X. W., Yang L., Tachibana K., Hirano S. I., Journal of Materials Chemistry A, 2015, 3, 170–178. 189. Yin K., Zhang Z. X., Yang L., Hirano S. I., Journal of Power Sources, 2014, 258, 150–154.
Lithium-Ion Batteries and Solar Cells
190. Appetecchi G. B., Kim G. T., Montanina M., Carewska M., Marcilla R., Mecerreyes D., De Meatza I., Journal of Power Sources, 2010, 195, 3668–3675. 191. Li X. W., Zhang Z. X., Li S. J., Yang L., Hirano S., Journal of Power Sources, 2016, 307, 678–683. 192. Safa M., Chamaani A., Chawla N., El-Zahab B., Electrochimica Acta, 2016, 213, 587–593. 193. Zhang P. F., Li M. T., Yang B. L., Fang Y. X., Jiang X. G., Veith G. M., Sun X. G., Dai S., Advanced Materials, 2015, 27, 8088–8094. 194. Lu W., Wang C., Yue W., Chen L., Nanoscale, 2011, 3, 9, 3631–3634. 195. Chen C.-Y., Wei T.-C., Hsiao P.-H., Hung C.-H., ACS Applied Energy Materials, 2019, 2(7), 4873–4881. 196. Wichiansee W., Sirivat A., Materials Science and Engineering C, 2008, 29, 78–84. 197. Vosgueritchian M., Lipomi D. J., Bao Z., Advanced Functional Materials, 2012, 22, 2, 421–428. 198. Li Q., Yang J., Chen S., Zou J., Xie W., Zeng X., Nanoscale Research Letters, 2017, 12, 506. 199. Thomas J. P., Zhao L., McGillivray D., Leung K. T., Journal of Materials Chemistry A, 2014, 2(7), 2383. 200. Chen C.-Y., Wong C.-P., Nanoscale, 2015, 7(3), 1216–1223. 201. Groenendaal L., Jonas F., Freitag D., Pielartzik H., Reynolds J. R., Advanced Materials, 2000, 12(7), 481–494. 202. Ahonen H. J., Lukkari J., Kankare J., Macromolecules, 2000, 33(18), 6787–6793. 203. Ghosh S., Inganäs O., Synthetic Metals, 1999, 101(1), 413–416. 204. Kim Y., Ballantyne A. M., Nelson J., Bradley D. D. C., Organic Electronics: Physics, Materials, Applications, 2009, 10(1), 205–209. 205. Sun, K., Zhang, S., Li, P., Xia, Y., Zhang, X., Du, D., Ouyang, J., Journal of Materials Science: Materials in Electronics, 2015, 26(7), 4438–4462. 206. Zhang X., et al., Solar Energy Materials and Solar Cells, 2016, 144, 143–149.
Diverse Phenomena in Stage-n Graphite AlkaliIntercalation Compounds Wei-bang Li and Ngoc Thanh Thuy Tran National Cheng Kung University
Shih-Yang Lin National Chung Cheng University
CONTENTS 2.1 Introduction .................................................................................................... 19 2.2 Theoretical Calculations ................................................................................. 21 2.3 Unique Stacking Configurations and Intercalant Distributions...................... 22 2.4 Metallic and Semimetallic Behaviors ............................................................26 2.5 Concluding Remarks ...................................................................................... 38 References ................................................................................................................ 39
A bulk graphite,1 which could be regarded as the layered graphene systems,2 has attracted a lot of theoretical and experimental researches in the basic science,3–5 engineering,6 and application.7 Each graphene layer is a pure carbon honeycomb lattice,8 and the graphitic layers are attracted together through the weak, but significant van der Waals interactions.9 There exist the very strong intralayer σ bondings of C-(2s, 2px, 2py) orbitals and a significant intra- and interlayer C-2pz orbital hybridizations,10 in which the former determine the most outstanding mechanical materials, and the latter dominate the low-lying energy bands and thus the essential physical properties. Very interesting, the 3D graphite systems might present the AA,11 AB,12 ABC,13 and turbostratic stackings.14 All of them belong to semimetals under the interlayer hopping integrals of C-2pz orbitals. In general, such condensed matter systems become the n- or p-type metals, depending on the kinds of intercalated atoms or molecules. For example, the intercalation of alkali atoms15 and FeCl3 into graphite, respectively, creates many free conduction electrons and valence holes, as observed in pure metal. It is well known that graphite could serve as the best anode materials16 in the commercial Li+-based batteries,17 mainly owing to the lowest cost, the most stable structure for intercalation, and the outstanding ion transport under the charging 19
Lithium-Ion Batteries and Solar Cells
and discharging processes. When the Li+ ions are released from the cathode, they will transport through the electrolyte and then intercalate into the graphitic system. Most important, the flexible interlayer spacings between the graphene layers are capable of providing sufficient positions for the various intercalant concentrations.18 Any intermediate states and meta-stable configurations, which are created during the ion/atom intercalation, could survive through the very strong σ bondings in graphitic sheets. As a result, graphite is rather suitable for studying the structural transformation in the chemical reactions. For example, the close relations between graphene and intercalant layers in lattice symmetries are expected to present the dramatic transformation before and after the intercalation/ de-intercalation processes. Up to now, there are a lot of theoretical and experimental studies on the fundamental properties in graphite-related systems. The former covers the phenomenological models and number simulation methods. For example, the tightbinding model, the random-phase approximation, and the Kubo formula are, respectively, utilized to investigate their electronic properties and magnetic quantization behaviors,19–22 Coulomb excitations23–26 and impurity screenings,27 and optical absorption spectra.28 Furthermore, the first-principles calculations29 are available in understanding the optimal stacking configurations; intercalant lattices, π, σ, and intercalation-induced energy bands; free conduction electrons/ valence holes; and density of states. However, certain critical physical quantities and pictures are absent in the previous studies, such as the atom-dominated band structures, the spatial charge densities between intercalant and graphene layers, the interlayer orbital hybridization of intercalant and carbon atom, the atom- and orbital-projected van Hove singularities, and the spin-dependent state degeneracy/ magnetic moment/density distribution. The main focuses of this work are the features of geometric and electronic properties in stage-n graphite alkali-intercalation compounds using the firstprinciples method.29 Very interesting, the dependences on the kinds of intercalants, their concentrations, and stacking configurations are thoroughly explored through the delicate calculations and analyses, especially for the lattice symmetries of intercalant layers, the dominances of valence and conduction states by carbon and/or alkali atoms, the blueshift of the Fermi level, the interlayer charge density variations after the alkali intercalations, and atom- and orbital-decomposed density of states. Whether the spin-induced Coulomb on-site interactions or the spin-orbital couplings play critical roles will be examined in detail. Most important, the orbital-hybridizations in chemical bonds and the atom-induced spin configurations are determined from the above-mentioned results. How to simulate VASP band structures by the tight-binding model is worthy of detailed discussions, since the interlayer hopping integrals are not very complicated under the concise primitive unit cells of layered graphite compounds. The predicted interlayer distance/intercalant lattice, band overlap, and unusual van Hove singularities could be detected using the high-resolution X-ray diffraction/low-energy electron diffraction,30 angle-resolved photoemission spectroscopy (ARPES),31 and scanning tunneling spectroscopy (STS),32 respectively.
Stage-n Graphite Alkali-Intercalation Compounds
2.2 THEORETICAL CALCULATIONS Both numerical simulations and phenomenological models are available in fully exploring the diversified physical, chemical, and material phenomena. For example, the former and the latter, respectively, cover the first-principles calculations29/ molecular dynamics33/quantum Monte Carlo34and the generalized tight-binding model5,35/Kubo formul36/random-phase approximation.37 Apparently, only the first method is able to investigate the lattice symmetries of the graphite-related systems with/without the chemical modifications. As for pure graphites and graphite alkaliintercalation compounds, the previous VASP results show that the stacking configurations and the intercalant lattice symmetries and concentrations play important roles in determining the semimetallic or metallic behaviors. However, the concise physical and chemical pictures, which are very useful in fully comprehending the fundamental properties, are required in the further studies, as done for 2D layered graphenes38,39 and 1D graphene nanoribbons.40–42 It is well known that the Vienna ab initio simulation package is developed within the density functional theory.43 The up-to-date VASP calculations can provide the sufficient information about the lattice symmetries, valence and conduction bands, charge density distributions/variations after chemical reactions, atom- and orbitaldecomposed density of states,44 being accompanied with the spin-dependent magnetic configurations. Very interesting, a lot of electron quasiparticles experience rather complicated interactions, when their wave packets propagate in any periodical material. Beyond the classical electrodynamics, the many-body electron-electron Coulomb interactions could be classified into the exchange and correlation energies according to the first order and the other orders, respectively. The Perdew–Burke– Ernzerhof formula, which depends on the local electron density, is utilized to deal with many-particle Coulomb effects. As for the frequent electron-crystal scatterings, they are characterized by the projector-augmented wave pseudopotentials. The electron Bloch wave functions are solved using the linear superposition of plane waves, with the maximum kinetic energy of 500 eV. The current study on stage-n graphite compounds shows that the first Brillouin zone is sampled by 9 × 9 × 9 and 100 × 100 × 100 k-point meshes within the Monkhorst–Pack scheme, respectively, for the optimal geometry and band structure. Moreover, the convergence condition of the ground-state energy is set to be ~10 −5 eV between two consecutive evaluation steps, where the maximum HellmannFeynman force for each ion is below 0.01 eV/Å during the atom relaxations. The self-consistent calculations, which are closely related to the local carrier density,45 account for the VASP simulations through the Kohn-Sham equations. According to the initial charge distribution, one evaluates the classical and manyparticle exchange-correlation Coulomb interactions, and the electron-ion scattering potentials. After solving the second-order differential equations, the intermediate electron density and ground-state energy are obtained, and they are utilized to examine the convergence condition on the Feynman force. The significant physical quantities, the lattice symmetries/the various bond lengths in a unit cell, the atomdominated valence and conduction bands, the spatial charge densities/their variations after the creation of chemical bonds, the atom- and orbital-projected van Hove
Lithium-Ion Batteries and Solar Cells
singularities, the atom-induced spin distributions, the spin-split or degenerate states across the chemical potential, and the vanishing or nonvanishing magnetic moments, are available in making a final decision about the critical multi-/single-orbital hybridizations of chemical bonds and the atom-induced spin configurations in the stage-n graphite alkali-intercalation compounds. The above-mentioned theoretical framework, which is built from the first-principles results, presents the successful exploration on the diversified essential properties of 2D layered graphenes,38,39 1D graphene nanoribbons,40–42 and 2D silicene-based systems.18 Now, the developed viewpoints are suitable for the anode, cathode, and electrolyte materials of Li+-based batteries.46 For example, a detailed comparison between graphite and Li4Ti5O12 is interesting and meaningful in terms of well-known anode compounds. The direct linking between numerical simulations and phenomenological models is a very interesting topic. According to the up-to-date results of the low-energy band structures, the combination of the VASP calculations18,46 and the tight-binding model5,35 is rather successful in exploring layered graphene/graphitic systems. For example, both methods can account for the linear and gapless Dirac-cone band structure, two pairs of linear/parabolic valence and conduction bands, three vertical Dirac cones/two pairs of parabolic bands plus one separated Dirac cone/one pair of partially flat, sombrero-shape and linear energy dispersions/oscillatory, sombrero-shaped and parabolic bands, respectively, for the monolayer, bilayer AA-/AB-stacked, and trilayer AAA-/ABA-/ABC-/AAB-stacked graphene systems. Their results are consistent with each other, since the important interlayer atomic interactions are purely due to the carbon-2pz orbitals within the specific unit cells. That is to say, the singleorbital Hamiltonians, with the concise inter- and intralayer hopping integrals, could be expressed in the analytic forms. Furthermore, all the intrinsic interactions, being modified by the external fields, are further included in the generalized tight-binding model. This theoretical framework has been successful in creating and explaining the rich and unique magnetic quantization phenomena of few-layer group-IV systems, e.g., the unusual quantized Landau levels in graphene, silicone,47 germanene,48 and tinene.49
UNIQUE STACKING CONFIGURATIONS AND INTERCALANT DISTRIBUTIONS
The normal stacking configurations, which are formed by the layered graphene systems, cover AAA, ABA, ABC, and AAB. For example, according to the VASP calculations on the trilayer graphenes, the ground-state energy/the interlayer distance is lowest and highest/shortest and longest for the ABA and AAA stackings, respectively. The similar results are revealed in the AA-, AB-, and ABC-stacked graphites. Each honeycomb structure has two equivalent sublattices with a planar geometry, indicating the orthogonal relation between one 2pz and three (2s, 2px, 2py) orbitals. The sp2-bonding-based graphene systems maintain the flat sheets even under any interlayer couplings (chemical reactions). The significant van der Waals interactions, the interlayer single-orbital hybridizations of 2pz -2pz, account for the stacking configurations and also noticed that the 2D silicene50/germanene51/tinene52 systems
Stage-n Graphite Alkali-Intercalation Compounds
possess the buckled structures, since the π and σ bondings are nonorthogonal to each other. Furthermore, the sp3 bonding might play an important role in the interlayer atomic interactions. Apparently, graphenes are quite different from silicenes/ germanenes/tinenes in various essential properties. The interlayer spacings of graphitic layers are able to provide a very suitable chemical environment for the alkali intercalations and de-intercalations, i.e., they are very useful during the charging and discharging processes. The chemical modifications hardly affect the planar honeycomb lattices and thus do not change the orthogonal feature of π and σ bondings. Very interesting, the optimal geometric properties are rather sensitive to the (x, y)-plane distribution and concentration of alkali atoms, e.g., the interlayer distances of neighboring planes and an enlarged primitive unit cell. According to the highest concentration, the graphite alkali-intercalation materials could be classified into two categories: lithium and non-lithium ones. There exists LiC6n or AC8n for the stage-n materials (Figure 2.1a-d), as examined from the experimental measurements and the theoretical predictions. The specific distance between carbon and intercalant layer is shortest/longest for the Li/Cs (Table 2.1), only directly reflecting the effective atomic radius. Although all the alkali atoms present the hollow-site optimal positions, their distribution symmetries are dominated by Li atoms or non-Li ones. The layered LiC6n and AC8n systems, respectively, possess the three- and four-time enhancement in the unit cell (Figure 2.2a and b); therefore, their reduced first Brillouin zones exhibit different high-symmetry points (Figure 2.3a). This is expected to have a strong effect on the initial π-electronic states of the Dirac-cone structure. More chemical bonds, which arise from the alkali-carbon atoms, are produced in graphite intercalation compounds, compared with pristine systems. Such bondings need to be taken into account for the diversified essential properties. In addition to the intercalant distribution, the stacking configuration of two neighboring graphitic sheets also affects the ground-state energy. The current study clearly shows that only the stage-1 LiC6 presents the AA stacking, and the other compounds possess the AB stacking. That is to say, all the graphite alkali-intercalation materials exhibit the AB-stacked configurations except for the former system.
FIGURE 2.1 Stage-n graphite alkali-intercalation compounds: (a) n = 1, (b) n = 2, (c) n = 3, and (d) n = 4
Lithium-Ion Batteries and Solar Cells
TABLE 2.1 Stage-Dependent Ground State Energies, the Optimal Geometric Properties, the Blueshifts of the Fermi Levels, and the Redshifts of the Initial σ-Electronic States for the Stage-n Graphite Alkali-Intercalation Compounds Stage-1, alkali-doped graphite compounds Distance between alkali metal and carbon layer (Å) Ground-state energy (eV) Blueshift of EF in band structure (eV) Blueshift of EF in DOS Redshifts of the initial σ-electronic (eV)
Stage-2, alkali-doped graphite compounds Distance between alkali metal and carbon layer (Å) Ground-state energy (eV) Blueshift of EF in band structure (eV) Blueshift of EF in DOS Redshifts of the initial σ-electronic (eV)
Stage-3, alkali-doped graphite compounds
Distance between alkali metal and carbon layer (Å) Ground-state energy (eV) Blueshift of EF in band structure (eV) Blueshift of EF in DOS Redshifts of the initial σ-electronic (eV)
Stage-4, alkali-doped graphite compounds
Distance between alkali metal and carbon layer (Å) Ground-state energy (eV) Blueshift of EF in band structure (eV) Blueshift of EF in DOS Redshifts of the initial σ-electronic (eV)
Stage-n Graphite Alkali-Intercalation Compounds
Planar structures of (a) LiC6 and (b) XC8 (X=Na, K, Rb, and Cs)
FIGURE 2.3 Rich band structures of the pristine graphite and stage-1 graphite alkaliintercalation compounds (a) within the corresponding first Brillouin zones: (b) AA and (c) AB stackings without intercalations, (d) LiC6, (e) NaC8, (f) KC8, (g) RbC8, and (h) CsC8
The high-resolution experimental measurements of X-ray scatterings and lowenergy electron diffractions42 are able to examine the intercalant distribution, interlayer distance, and stacking configuration of graphite alkali-intercalation compounds; furthermore, those of scanning tunneling microscopy and tunneling electron
Lithium-Ion Batteries and Solar Cells
microscopy are very suitable for the identifications of optimal geometric structures in few-layer graphene system.49 The previous experiments have shown the AA/AB stacking of the stage-1 LiC6/AC8 material, while the predicted AB stacking in stage-2–4 compounds (LiC12, LiC18, and LiC24) requires the further experimental verifications.
2.4 METALLIC AND SEMIMETALLIC BEHAVIORS Without alkali atom intercalations, a pristine graphite exhibits the unique semimetallic behavior through the weak, but significant van der Waals interactions. It is well known that a monolayer graphitic sheet has the orthogonal π and σ bondings, in which the initial electronic states, respectively, come to exist at the Fermi level (EF = 0) and E ~ −3.10 eV. Obviously, the low-energy physical properties are mainly determined by the intralayer atomic interactions. Such hopping integrals, being accompanied with the uniform three nearest neighbors are responsible for a gapless and isotropic Dirac cone initiated from the K/K’ valleys. The density of states is vanishing at EF because of the specific Dirac points. A semiconducting zero-gap graphene is dramatically changed into a semimetallic system for any few-layer stackings, or infinite-layer graphites. For example, there exist the unusual overlaps of valence and conduction bands along the KH path (or the ΓA path under the reduced Brillouin zone in Figure 2.3a and b) in AA-, AB- and ABC-stacked graphites through the single-orbital interlayer atomic interactions. According to the VASP and tight-binding model calculations, the simple hexagonal/rhombohedral graphite (Figure 2.3a), with the highest/lowest stacking symmetry, presents the largest/lowest free carrier density of the conduction electrons and valence holes. In general, the π valence bands, which are purely related to the C-2pz, show the initial states at the stable K valley, the saddle-point structure near the M point (Ev ~ −3 eV), and its termination in the Γ valley (the whole π-bandwidth more than 7 eV). Very interesting, the band structures of lithium- and non-lithium graphite intercalation compounds sharply contrast with each other, such as those of stage-1 LiC6 and XC8 compounds shown in Figure 2.3d, e, and h, respectively. For the former, the Fermi level is transferred from the middle of the Dirac-cone structures into the conduction ones near the Γ valley after the intercalation of lithium atoms. That is to say, EF presents a blueshift. Apparently, the free carriers are due to the outmost 2s orbitals of lithium atoms. The occupied and unoccupied states are highly asymmetric to each other about the Fermi level. The initial π/π* valence/conduction states are mainly determined by the stacking configurations in the chemical intercalations (the distribution symmetry of Li-intercalants in Figure 2.2a), or the corresponding relation between the original and reduced first Brillouin zone. There exists an observable energy spacing of Ec ~ 0.310.63 eV along the Γ-A path in the modified valence and conduction Dirac-cone structures. The creation of discontinuous states in honeycomb lattices might arise from different ionization energies of Li-2s and C-2pz orbitals (the distinct on-site Coulomb potential energies). The whole π valence-bandwidth of LiC6, being created by the C-2pz orbitals, could be identified to about 7.32/7.40 eV from the electronic energy spectrum along the Γ-M-K-Γ/A-H-L-A (or Γ-K-M-Γ/AL-H-A) paths. This result clearly illustrates the well-behaved π bondings in graphite alkali-intercalation compounds. Another σ bondings behave so, as indicated from the initial states at the Γ point of Ev ~ −4.20 eV. Their orthogonal relation remains
Stage-n Graphite Alkali-Intercalation Compounds
the same after the chemical modification, being very useful in establishing the tightbinding model for graphite alkali-intercalation compounds. The main features of band structure, as clearly indicated in Figure 2.3e–h, are dramatically changed under the other alkali-atom intercalations. Both stage-1 AC8 and LiC6 have totally different distribution configurations (Figure 2.2a and b), and so do the reduced first Brillouin zones (Figure 2.3a). For the former, the Dirac-cone structures of the π and π* bands are initiated from the stable K/K’ valleys, but not the Γ ones. The energy spacing of separated Dirac points is small or almost vanishing; furthermore, the Fermi level is situated above the conduction point about ~1.35–1.50 eV. In addition to EF, whether the second conduction energy sub-band is partially occupied depends on the kinds of alkali atoms, such as the alkali-induced free electrons in the first and second sub-bands for KC8/RbC8/CsC8 (Figure 2.3f–h). The low-energy bands belong to the single states, without the split double degeneracy (Figure 2.3d for LiC6). The whole π-band energy spectra are identified from the K-Γ-K-M-Γ and H-A-H-L-A paths, leading to the width of ~7.31–7.41 eV. Very interesting, one pair of π-valence sub-bands come to exist near Ev ~ −4.0 eV, being accompanied with the initial pair of the σ valence bands. This further illustrates the zone-folding effects on band structure and the good separation of π and σ bondings. Electronic energy spectra strongly depend on the n-stage of graphite intercalation compound, as clearly illustrated in Figure 2.4a–f. The stage-2 LiC12 and AC16 have different first Brillouin zones on the (k x, k y) plane, and their kz -ranges are associated with the distances between two intercalant planes (Figure 2.1). Compared with stage-1 band structures (Figure 2.3d–h), the number of Dirac cones becomes double in the stage-2 cases, in which the further modifications cover the reduced blueshift of the Fermi level, the enhanced anisotropy, the induced energy spacings between valence and conduction Dirac points, and the diversified energy relations near the band-edge states. For example, four/two valence and conduction pairs come to exist from the Γ/K valley (or the A/H valley) for LiC12/AC16 (Figure 2.4d–h). Furthermore, the whole π-bandwidths could be roughly estimated from the ΓKMΓ/KMKΓ path (or the ALHA/HLHA path). The low-energy essential properties are dominated by the π bondings of C-2pz orbitals. The above-mentioned obvious changes directly reflect the great enhancement of the interlayer atomic interactions due to the C-C bonds in two neighboring graphitic sheets/graphene-intercalant layers. Very interesting, all the stage-2 compounds exhibit a pair of σ bands at the Γ and A valleys, and the energy dispersions along Γ–A are negligible. These results indicate the mutual orthogonality of the planar σ and perpendicular π bondings. Such a phenomenon is expected to survive in any stage-n graphite alkali-intercalation compounds. The blueshifts about the Fermi level and the free conduction electrons decline quickly in the increase in the n number. The alkali-concentration is greatly reduced, and do the charge transfer from their outmost s-orbitals to carbon 2pz -ones. Such results are clearly revealed in the stage-3 systems. Figure 2.5a–f shows the slight modifications of the Dirac-cone structures and the intersecting of the Fermi level with most of the conduction bands. LiC18 (Figure 2.5b) and AC24 (Figure 2.5c–f), respectively, possess six and three pairs of linear valence and conduction bands near the Γ–A and K–H valleys. Apparently, there exist the significant changes in the observable energy spacing between valence and conduction Dirac points, the anisotropic Fermi
Lithium-Ion Batteries and Solar Cells
FIGURE 2.4 Unusual electronic energy spectra of the AB-stacked stage-2 graphite alkaliintercalation compounds: (a) the reduced first Brillouin zones of AB stacking, (b) LiC12, (c) NaC16, (d) KC16, (e) RbC16, and (f) CsC16
velocities, and the distinct Fermi momenta slopes. The blueshifts of EF are estimated to be 0.45, 0.58, 0.55, 0.53, and 0.5 eVs. Very interesting, the electronic energy spectra become more complicated under the stronger zone-folding effects. The main features of electronic properties are closely related to the weak, but important Li-C bonds, e.g., the minor contributions of alkali atoms on each of the electronic states. That is, the diversified n-type dopings are created by the critical Li-C and C-C bondings. The conduction electron density, which is created by the alkali-atom doping, is worthy of a closer examination. It is mainly determined by the covered volume (area/length) in the wave-vector space between the lowest conduction state and the Fermi level for 3D graphite alkali-intercalation compounds53 (2D alkaliadsorbed graphenes/1D graphene nanoribbons). In general, the VASP calculations are too heavy to obtain the delicate values because of the strong anisotropic energy dispersions (the nonlinear Dirac-cone structure at higher energies in Figures 2.3h and 2.4e). That a lot of 3D k-points are required for the accurate calculation of free electron density is almost impossible. The similar phenomenon is revealed in the alkali-adatom adsorptions on graphene. However, 1D graphene nanoribbons are very
Stage-n Graphite Alkali-Intercalation Compounds
FIGURE 2.5 Rich band structures for the AB-stacked stage-3 graphite alkali-intercalation compounds: (a) the reduced first Brillouin zone, (b) LiC18, (c) NaC24, (d) KC24, (e) RbC24, and (f) CsC24
suitable for the full exploration of charge transfer and conduction electron density, since the Fermi momenta are proportional to the latter. After examining the critical mechanisms, namely the zigzag/armchair edges, different widths, five kinds of alkali atoms, and their various distributions, the free electron density is almost identical to the adatom concentration.54 It can be deduced that any one alkali adatom contributes the outmost half-occupied s-orbital as a conduction carrier, or it behaves the full charge transfer of −e in the alkali-carbon bonds. Such conclusions might be suitable for 2D and 3D alkali-doped graphite compounds, being supported by the following result. According to the spatial charge distributions and their variations after the chemical modifications, the chemical bondings hardly depend on the distributions and concentrations of alkali adatoms. Generally speaking, only the high-resolution ARPES is capable of detecting the wave-vector-dependent occupied energy spectra below the Fermi level. The up-todate experimental measurements have successfully verified the diversified phenomena for the graphene-related sp2-bonding systems, as clearly observed under the various dimensions, layer numbers, stacking configurations, substrates, and adatom/ molecule chemisorptions. For example, there exist 1D parabolic dispersions with sufficiently wide energy spacings/band gaps in graphene nanoribbons, the linear Dirac cone for monolayer graphene, two parabolic valence bands in bilayer AB stacking,
Lithium-Ion Batteries and Solar Cells
the linear and parabolic dispersions in twisted bilayer systems, one linear and two parabolic bands for tri-layer ABA stacking, the linear, partially flat and Sombreroshaped dispersions in tri-layer ABC stacking, the substrate-created observable energy spacing between the separated valence and conduction bands in bilayer AB stacking/oscillatory bands in few-layer ABC stacking,2 the semimetal-semiconductor/semimetal-metal transitions after the adatom/molecule adsorptions graphene surface, and the bilayer- and monolayer-like energy dispersions, respectively, at the K and H corner points (Figure 2.3a) for the Bernal graphite. The ARPES measurements are available in examining the main features of the occupied band structure in graphite alkali-intercalation compounds, namely the blueshift of the Fermi level, the initial K or Γ valley for the π and π* bands, the separated or almost close Dirac-cone structures, their double or single degeneracy, the whole π band along the Γ-K-M-Γ A-L-H-A paths (or the K-Γ-K-M-Γ/H-A-H-L-A paths), the formation of σ sub-bands at E ~ −4.0 eV from the Γ valley, and the sensitive dependences on the alkali-atom distributions and concentrations. The experimental verifications could provide useful information about the zone-folding effects due to the alkali interaction, the single-orbital hybridizations in alkali-carbon bonds, and the almost full charge transfer (discussed in the previous paragraph). The density of states at E (DOS(E)), the number of states within a very small energy range of dE, is available in thoroughly comprehending the valence and conduction energy spectra simultaneously. In general, its special structures are created by the band-edge states with the vanishing group velocities. The critical points in the energy-wave-vector space include the local extreme points (minima and maxima), the saddle points, and the partially flat energy dispersions. Apparently, the van Hove singularities are greatly diversified under different dimensions, e.g., the important differences in graphite- and graphene-related systems. Of course, the discrete energy levels in 0D quantum dots only present the delta-function-like peaks, as observed in the magnetically quantized Landau levels of the emergent layered materials (fewlayer graphenes in Refs), and any-dimensional dispersionless energy bands. The 1D parabolic and linear bands, respectively, create the asymmetric divergent peaks in the square-root form and the plateau structures. As for the 2D condensed matter systems, the concave-/convex-form energy dispersions, the Dirac-cone structure (the linear valence and conduction bands without energy spacing), the saddle points, and the constant-energy loops, respectively, induce the broadening shoulders, V-shapes, the symmetric peaks related to the logarithmical divergence, and the square-root divergent peaks. Moreover, the higher dimension in 3D materials makes them only show the symmetric/asymmetric peaks and shoulder structures, mainly owing to the absence of quantum confinement. The latter come from the 3D parabolic energy dispersions. The delicate calculations and analyses, which are conducted on the atom- and orbital-dependent density of states (Figure 2.6al), are capable of fully understanding the metallic behavior and the close relations among the different chemical bondings. Although band structures, with many band-edge states, become very complicated under the alkali-atom intercalations, the main features of van Hove singularities are sufficiently clear for the identifications of diversified phenomena through a suitable broadening factor (e.g., energy width of ~0.10 eV). This further illustrates a critical role of zone folding in the fundamental properties. Very interesting, the low-energy
Stage-n Graphite Alkali-Intercalation Compounds
FIGURE 2.6 Atom- and orbital-decomposed density of states for the (a) AA- and (b) AB-stacked graphite systems, (c) LiC6, (d) NaC8, (e) KC8, and (f) RbC8. The black, red, lig and ht blue, pink, green, deep blue, and purple curves, respectively, C-2s, C-2px, C-2py, C-2pz, alkali, carbon, and compound
DOSs in stage-1 and stage-2 graphite alkali-intercalation compounds present a prominent peak just at the Fermi level (EF = 0), regardless of the kind of alkali atoms. Furthermore, there exists a valley structure, with a minimum value, at its left-hand neighbor. When such characteristic is combined with the similar ones at EF) in the pristine AA- and AB-stacked graphite systems (Figure 2.6a and b), the Fermi level is deduced to exhibit a blueshift. That is to say, EF is situated at the conduction energy sub-bands (EF roughly lies in the center of valence and conduction bands) roughly after (before) the alkali-atom intercalations. It should be noticed that the contributions due to the alkali atoms are weak, but rather important. The blueshifts of the stage-1 LiC6, NaC8, KC8, RbC8, and CsC8 and stage-2 LiC12, NaC16, KC16, RbC16 and CsC16 are, respectively, estimated to be 1.90, 1.80, 1.70, 1.60, 1.50, 1.30, 1.20, 1.10, 1.00, and 0.90 eVs.
Lithium-Ion Batteries and Solar Cells
The van Hove singularities in graphite intercalation compounds (Figure 2.6c–l), which survive in the specific energy ranges, are mainly determined by the carbon or alkali atoms and their orbitals. Most important, DOS in the critical energy range of −5.0 eV < E < 3.0 eV, being relatively easily examined from the experimental STS measurements, are dominated by the carbon-2pz orbitals (the pink curves). Furthermore, the minor contributions related to the outmost s-orbital of alkali atoms (the green curves), especially at the conduction energy spectrum, play a critical role in determining the blueshift of the Fermi level. As for the C-(2px, 2py) orbitals (the red and light blue curves), their contributions are initiated from ~E < −4.0 eV, while they are absent in the opposite energy range. The redshift of the initial σ valence bands is about 1.0 eV, compared with those of the pristine simple hexagonal and Bernal graphites (Figure 2.6a and b). Only the LiC6 and LiC12 cases (Figure 2.6c and h) exhibit the split contributions of 2px and 2py orbitals. This result directly reflects the anisotropic distribution configuration. Moreover, the C-2s orbitals come to exist at the deeper energies of ~E < −5.0 eV. Apparently, the above-mentioned features indicate the good separation of C-2pz and C-(2s, 2px, 2py) orbital contributions and thus the normal perpendicular orbital hybridizations of π and σ chemical bonds. That such bonding behavior is strongly linked with the significant interlayer 2pz -orbitals due to the carbon-alkali bonds can account for the featured electronic properties, e.g., the main features of band structures and DOSs in Figures 2.3–2.7. The clear identifications of stage-1 and stage-2 of graphite alkali-intercalation compounds could be achieved from the low-energy features of van Hove singularities, as indicated in Figure 2.6c–l, respectively. Compared with those of the former, the blueshifts of the Fermi levels are relatively small, in which they are, respectively, ~1.20, 1.15, 1.10, 1.06, and 1.03 eV for LiC12, NaC16, KC16, RbC16, and CsC16. Most important, their densities of states at EF do not belong to the local maxima. Such a result directly reflects whether the band-edge states of conduction bands are somewhat away from the Fermi level (Figure 2.4b–f). This significant difference between stage-2 and stage-1 systems further illustrates the intersecting of EF and conduction bands, thus leading to the n-type doping cases after the alkali-atom intercalations. The experimental measurements could be utilized to verify the free conduction electrons due to the alkali-atom intercalations, e.g., the atom-dependent optical threshold absorption frequencies, and the doping-enhanced electrical conductivities. The high-resolution STS measurements are the only method in examining the van Hove singularities due to the valence and conduction energy spectrum, especially for the semimetallic, metallic, or semiconducting behaviors near the Fermi level. Such examinations cover the form, energy, number, and intensity of special structures in the density of states. Apparently, they cannot identify the wave-vector-dependent energy dispersions. The up-to-date measured results have successfully verified the diverse electronic properties in graphene-related systems with the dominating sp2 bondings, e.g., 1D graphene nanoribbons, carbon nanotubes, 2D few-layer graphenes, adatomadsorbed graphenes, and 3D graphite. The main features of graphene nanoribbons, the width- and edge-dependent energy gaps and the square-root-divergent asymmetric peaks of 1D parabolic dispersions, are confirmed from the precisely defined boundary structures. The similar strong peaks are displayed in seamless carbon nanotubes,
Stage-n Graphite Alkali-Intercalation Compounds
FIGURE 2.7 Atom- and orbital-decomposed density of states for the (g) CsC8, (h) LiC12, (i) NaC16, (j) KC16, (k) RbC16, and (l) CsC16. The black, red, light blue, pink, green, deep blue, and purple curves, respectively, C-2s, C-2px, C-2py, C-2pz, alkali, carbon, and compound
in which these structures exhibit the chirality- and radius-dependent band gaps and energy spacings between two neighboring sub-bands. Even with the obvious curvature effects on a cylindrical surface (the misorientation of 2pz orbitals and the significant hybridization of carbon four orbitals), armchair nanotubes belong to 1D metals with a finite density of states at the Fermi level (a sufficiently high free carrier density). A lot of STS measurements, which are made for few-layer and adatom-doped graphenes, clearly illustrate the low-lying characteristics of van Hove singularities: a V-shaped energy dependence vanishing at the Dirac point in monolayer system (a zero-gap semiconductor), the asymmetry-induced peak structures in the logarithmic form for twisted bilayer graphenes, a gate-voltage-created band gap in bilayer AB stacking and tri-layer ABC stacking, a delta-function-like peak centered about the Fermi level related to surface states of the partially flat bands in tri-layer and penta-layer ABC stackings, a sharp
Lithium-Ion Batteries and Solar Cells
dip structure at EF accompanied with a pair of asymmetric peaks in tri-layer AAB stacking (a narrow-gap semiconductor with the low-lying constant-energy loops), and a redshift of Dirac point arising from the n-type electron doping of Bi adatoms. The measured density of states in Bernal graphite is shown to be finite near EF characteristic of the 3D semimetallic property and presents the splitting of π and π* strong peaks at deeper/higher energies. It should be noticed that the well-defined π and σ bandwidths in graphene-related systems are worthy of the further STS examinations. In addition, there are no STS results for AA- and ABC-stacked graphites up to now, mainly owing to few content of natural graphite and the difficulties in sample growth. The experimental examinations on the current predictions, especially for the van Hove singularities near EF and the π and σ bandwidths, are very useful in providing the detailed information about the n-type dopings and the orbital hybridizations of chemical bonds. The close relations between the VASP simulations30 and the tight-binding model/ the effective-mass approximation17,35 in graphite-/graphene-related systems are discussed in detail. The previous theoretical studies show that the electronic properties of pure carbon honeycomb lattices are well characterized by the phenomenological model. According to the calculated results of two different methods, the rich and unique band structures are created by the stacking configuration, layer number, and dimensionality, such as those due to monolayer graphene, bilayer AA/AB stackings,55 trilayer AAA/ABA/ABC/AAB stackings,56,57 3D AA-/AB-/ABC-stacked graphites,11–13 1D achiral/chiral carbon nanotubes,58,59 and graphene nanoribbons. Their outstanding consistence is deduced to be closely related to the good separations of π and σ chemical bondings and the interlayer single-2pz -orbital hybridizations. Very interesting, the generalized tight-binding model,5 which is combined with the static and dynamic Kubo formulas60 and the modified random-phase approximation, is capable of fully exploring the diversified magnetic quantization. As for the emergent 2D group-IV and group-V materials, these theoretical frameworks are successful in studying the unusual magneto-electronic properties, the various magneto-optical selection rules, the unique quantum Hall conductivities, and complex magneto-plasmon modes and inter-Landau-level excitations.61 The low-energy physical properties of graphites and graphite alkali-intercalation compounds are dominated by the single-orbital interactions of C-2pz and A-s orbitals (the outmost one of alkali atom). The AA-, AB-, and ABC-stacked graphites11–13 have two, four, and six carbon atoms in a unit cell, so their Hamiltonians are built from the corresponding tight-binding functions. After the diagonalization of Hermitian matrices, the π- and π*-electronic energy spectra strongly depend on the stacking configurations, especially for the overlap of valence and conduction bands. The highest conduction electron/valence hole density is revealed in the first/third system. Apparently, the stacking-enriched interlayer hopping integrals of C-2pz orbitals are responsible for the diversified semimetallic properties. Most important, the above-mentioned phenomenological methods could cover the alkali intercalation effects, the enlarged unit cells, and the stacking configurations. For example, the modified Hamiltonians of graphite lithium-intercalation compounds include the ionization energy difference between C-2pz and Li-2s orbitals, the intralayer nearest-neighboring interactions of 2pz -2pz /2s-2s orbital in C-C/Li-Li bonds, and the interlayer 2pz -2s/2pz -2pz orbital hybridizations. Specifically, the third ones might be
Stage-n Graphite Alkali-Intercalation Compounds
complicated and very sensitive to the change in the intercalant concentration and arrangement; therefore, they play a critical role in creating the diversified metallic behaviors. It should be noticed that the theoretical models, with the zone-folding effects, are absent up to now. The X-ray diffraction62 is available for thorough investigations of crystalline materials through the atomic lattices. The incident photons, which possess a wavelength comparable to/less than the lattice constants, experience the elastic scatterings with the periodic atom distribution and thus create the constructive and destructive patterns. In this process, the X-rays are scattered elastically by the carrier charge density and create the so-called Thomson scatterings. The valence electrons oscillate like a Hertz dipole at the frequency of incident photons and serve as a source of dipole radiation. The wavelength λ of X-rays is conserved during Thomson scatterings. The spectral intensity at distance R could be roughly expressed as I ( R ) = I 0 ( re /R ) 1 + cos2 2θ /2 in the absence of detailed atomic nuclei, where re = ( μ0 /4π ) e 2 /m is the classical radius of electron (2.818 × 10 −15 m),63 and it also becomes an evidence why the scattering from atomic nuclei has not been considered in the detailed derivations. In fact, the intensity equation would hold even in the presence of specific scatterings from the atomic nuclei, since the nuclei components will only yield a 10 μm), and flake-like morphology is observed for MLGN and its lateral size is 2-5 μm for a single piece with laminar structure. The FETEM (field emission transmission electron microscopy) images reveal that the GO sheets are quite large in dimension (length ~5–7 nm, width ~3–5 nm) with fairly flat edges that suggest that the number of layers of GO aggregates.
FIGURE 8.4 X-ray diffraction pattern of GO and MLGN.
Graphene as Anode in Lithium Ion Battery
FESEM and FETEM images of (a, b) GO and (c, d) MLGN.
BONDING/BINDING ENERGY/FUNCTIONAL GROUPS AND PHONON MODES
Figure 8.6 shows the C1s XPS spectrum for MLGN (multilayer graphene) and GO (graphene oxide) where the C1s spectrum of MLGN shows peaks at 284.74, 285.84, 287.64, and 289.74 eV corresponding to C–C, C–O, C=O, and (C(O)O) functional groups, respectively. Similarly, the C1s spectrum of GO shows characteristic peaks at 284.8, 286.9, and 288.7 eV that are attributed to C–C, C=C, C–H, C–OH, and C=O bonds, respectively (Figure 5b) . Figure 8.7 describes the Fourier transform infrared spectra (FTIR) of MLGN and GO. GO shows several absorption peaks at 3,400, 1,732, 1,620, 1,375, 1,252, and 1,058 cm−1 which are attributed to OH hydroxyl and carboxyl group , COOH , C=O [13,14], unoxidized graphitic domain , C–OH , C–O–C , and C–O stretching vibrations [14,19]. This indicates that the graphene oxide is associated with a large concentration of oxygen-containing functional group. Similarly, FTIR analysis of MLGN also shows different functional groups such as OH (3,400 cm−1), C=C (1,620 cm−1), and C=O (1,732 cm−1); stretching vibrations and the bands at 1,252 and 1,071 cm−1 are attributed to CO stretching vibrations of carboxylic groups [20,21]. The Raman analysis of GO and MLGN is shown in Figure 8.8 that shows three peaks in GO corresponding to D band (1,342 cm−1) that is assigned to the defect peak within the carbon structure, G band (1594.8 cm−1) that is usually attributed to the sp2 bonded carbon atoms in the honeycomb lattice, and the 2D band (2,700 cm−1) that is a characteristic signature of the graphene, respectively [22–24], and is usually used to determine the number of layers of graphene in the sample. MLGN also shows similar peaks at 1,333, 1,580, and 2,680 cm−1 corresponding to D band, G band, and 2D band, respectively (Figures 8.8 and 8.9).
Lithium-Ion Batteries and Solar Cells
C1s XPS spectrum of (a) MLGN and (b) GO.
FTIR spectrum of GO and MLG.
Graphene as Anode in Lithium Ion Battery
FIGURE 8.8 Raman spectrum of GO and MLGN.
FIGURE 8.9 Lithiation and de-lithiation of: (a) MLGN, (b) discharge capacity versus cycle number of MLGN.
Lithium-Ion Batteries and Solar Cells
GRAPHENE AS ANODE IN LITHIUM-ION BATTERIES GRAPHENE
Yoo et al.  have prepared GNSs by exfoliation of bulk graphite and used it as anode material in LIBs. GNS having wrinkled/crumpled paper-like structure is comprised of 10–20 layers of stacked graphene sheets and the thickness varies from 3 to 7 nm. Comparative investigation about the Li-storage properties has been done by incorporating carbon nanotube (CNT) and fullerenes (C60) in GNS. The GNSs could achieve a reversible capacity of 540 mAh g−1 (current density = 0.5 A g−1) that increases to 730 mAh g−1 and 784 mAh g−1 by the incorporation of CNT and C60, respectively, and the capacity is much higher than the theoretical capacity of graphite. The capacity reaches 290 mAh g−1 (GNS), 480 mAh g−1 (GNS + CNT), and 600 mAh g−1 (GNS + C60), respectively, after 20 cycles with the retention of 54%, 66%, and 77% for GNS, GNS + CNT, and GNS + C60, respectively. The enhancement in the capacity is not only due to the formation of the LiC6 compounds but also attributed to the increase in the d-spacing of the GNS (d = 0.365 nm) by 19% in comparison with GNS + CNT (0.40 nm) and GNS + C60 (0.40 nm). This increase in the d-spacing may create more active sites leading to a large change in the structural and electronic changes in GNS and the composites for the insertion of the lithium ions. However, this is the initial result of graphene as a negative electrode in LIBs and the reversible capacity/the Li-storage capability are significantly enhanced by the change in the synthesis of graphene, engineering of the oxygen-containing functional groups, surface/microstructure modification, doping, or by making composite with metal oxides. The GNSs synthesized by the three-step procedure as described by Guo et al.  have shown relatively good lithium-storage capability as compared to the earlier procedure of exfoliation. The GNSs are prepared first by the oxidation of graphite by Hummer’s method, rapidly heating at 1,050°C in the air to form expanded graphite and ultrasonication for 4 h. The first charge–discharge capacities of GNSs are increased to 1,233 and 672 mAh g−1, respectively, at a current density of 0.2 mA cm−2. The high irreversible capacity is attributed to the reaction of Li-ion with oxygen-containing functional groups and the formation of the solid electrolyte interface (SEI). The GNSs maintain the capacity of 554 mAh g−1 and have shown significant potential as anode materials in LIBs. Slight variation in the synthesis procedure yield few-layer GNS having high surface area for better Li-ion adsorption/desorption and consequently the electrochemical performance. Graphite oxide exfoliation at high temperature in a different atmosphere seems to yield varying results. Lian et al.  have prepared graphite oxide by chemically modified procedure but exfoliated the graphite oxide at 1,050°C in nitrogen atmosphere. The first discharge and charge capacities of graphene sheets were as high as 2,035 and 1,264 mAh g−1 (current density = 100 mA g−1), respectively, and the capacity is still maintained at 848 mAh g−1 after 40 cycles. This high electrochemical performance is attributed to the high-quality graphene sheets (∼4 layers) with a curled/wrinkled morphology and a large specific surface area (492.5 m2 g−1). Wang et al.  have synthesized flower-like GNSs by chemical modification procedure that also follows a three-step procedure (oxidation of graphite/ultrasonication
Graphene as Anode in Lithium Ion Battery
to disperse graphene oxide/reduction by hydrazine hydrate under reflux at 100°C). The first discharge (charge) capacity of GNSs anode is 945 mAh g−1 (650 mAh g−1). The irreversible capacity could be associated with the formation of the SEI layer in the first cycle. The capacity is maintained at 460 mAh/g after 100 cycles and that shows good electrochemical performance. Similarly, Vargas et al.  have also prepared graphene by reducing graphite oxide by N2H4 and used it as anode with LiNi0.5Mn1.5O4 (LNMO) as high voltage, spinel-structure cathode and achieved reasonable capacity after 50 cycles.
8.4.2 DOPED GRAPHENE Doping of atoms such as nitrogen, boron, phosphorus seems to improve the electrochemical performance of graphene. The atomic diameter of nitrogen and carbon is almost same but differs in the electronegativity that is higher in nitrogen than carbon that enhances the interaction between a nitrogen-doped carbon material and lithium ions. Nitrogen doping enhances the electrical conductivity of graphene due to the formation of pyridine/bridgehead-like nitrogen. Wu et al.  have prepared nitrogen- and boron-doped graphene and used them as anode in LIBs. The doping was done at high temperature (600°C, 800°C) by using NH3 (∼99.0%) and Ar (1:2 v/v) and BCl3 (∼99.99%) and Ar (1:4 v/v) for N- and B-doping, respectively. The discharge capacity of N-doped graphene in the first cycle is 1,043 mAh g−1, and after 30 cycles, it reaches 872 mAh g−1 (50 mA g−1) that is much higher than the regular graphene. Similarly, for B-doped graphene, the discharge capacity is 1,227 mAh g−1 after 30 cycles (1,549 mAh g−1 in the first cycle). Consequently, the reversible capacity retention is 83.6% for the N-doped graphene and to 79.2% for the B-doped graphene after 30 cycles. The major advantage of these composites is the fast charging at high current rates such as 500 mA g−1, 5 A g−1, and 25 A g−1. At a very high current rate of 25 A g−1, the charge time is ∼28 s/∼33 s for the N-/B-doped graphene and the reversible capacity reaches 199/235 mAh g−1 for the N-/B-doped graphene and these results are far superior to those of the pristine graphene (∼100 mAh g−1 at 25 A g−1). The outstanding electrochemical performance of the doped graphene is due to the increase in the electrical conductivity/electrochemical activity, high thermal stability, increased disordered surface morphology, higher hydrophobicity, and better wettability toward organic electrolytes that can promote ion diffusion at the interface of electrode and electrolyte, ultrathin framework, high surface area, open porous structure, mechanical flexibility, and chemical stability. N-doped GNS can also be obtained by exfoliating graphene oxide in N atmosphere at elevated temperature (~1,000°C) . An interesting phenomenon is observed for this N-GNS, where the discharge capacity of 454 mAh g−1 is observed in the second cycle, continues to decrease till 17th cycle, and reverses thereafter. The capacity continues to increase to 684 mAh g−1 at 501 cycles showing superior electrochemical performance like that with GNS (269 mAh g−1 @ 100 cycles with 66% retention). The N-doping leads to the formation of pyridinic nitrogen, which in turn produces carbon vacancies in the graphene network that increases the Li+ storage sites, resulting in the enhancement in the capacity of the N-GNS anode.
Lithium-Ion Batteries and Solar Cells
8.4.3 POROUS GRAPHENE Recently, hierarchical porous materials have received a lot of attention for their applications as energy storage/conversion devises, photocatalysts, LIBs, and supercapacitors due to the high surface area, better interfacial transport, and reduced diffusion paths. Porous materials are comprised of porous structures with different pore sizes and depending on their dimensions, they are named as micropore (~1–2 nm) for a high concentration of ion adsorption, mesopore (2–100 nm) that facilitate the ion transfer and macropore (~400 nm) which acts as a reservoir to accommodate electrolyte [32,33]. As far as graphene is concerned, porous graphenes having pores either on the sheet or between the sheets are attributed with very high specific surface areas, excellent flexibility, electrical conductivity, specific capacity, outstanding physical and chemical stability, and significantly high concentration of defects/active sites that increase the electrochemical performance [34,35]. Fan et al.  have obtained porous graphene (pore size 3–8 nm) by chemical vapor deposition that presents a high reversible capacity (1,723 mAh g−1 at 0.1°C) and excellent rate capability (203 mAh g−1 at 20°C). Charge–discharge analysis of porous graphene shows very high specific capacity 4,858 mAh g−1 and reversible capacity of 1,827 mAh g−1 in the first cycle which is five times higher than those of graphite (372 mAh g−1) and reduced-GO (453 mAh g−1). The high capacity is due to the presence of curled edges and mesopores on the graphene sheets [37,38]. The cyclic stability investigation shows an increase of capacity from 726 to 926 mAh g−1 (1°C) after 100 cycles and 240-211 mAh g−1 (@ 20°C) after 100 cycles. The increase of capacity with the cycle is due to the activation of porous graphene during the cycling, and the significant cyclic stability is due to the effective control of the volume expansion by the curled edges of porous graphene sheets. The rate capability study also shows a great electrochemical performance of the porous graphene that exhibits reversible capacities of 955, 544, and 203 mAh g−1 at 0.5°C, 5°C and 20°C, respectively. This significant high rate capability and cyclic stability are partly attributed to the presence of the active sites at the edge, the mesopores in the sheets that reduce the diffusion length of lithium ions and the strongly crumpled/scrolled graphene sheet that acts as a buffer to accommodate the volume expansion during Li-insertion/Li-extraction. Fang et al.  have synthesized mesoporous carbon sheets on a template by a typical monomicelle close-packing assembly approach followed by carbonization at high temperature and elimination of template by HCl. The mesoporous graphene layers have high surface area for lithium-ion adsorption and intercalation, which enables better ion transport for enhanced lithium-ion storage capacity and cyclic stability. The mesoporous graphene anode achieved excellent reversible capacity of 1,040 mAh g−1 (@ 100 mA g−1), and the capacity is at 833 mAh g−1 even after 70–80 cycles. The rate capability is also good that reveals a capacity of 255 mAh g−1 at a large current density of 5 A g−1. Therefore, the mesoporous graphene could achieve very good lithium-ion storage capacity as well as cyclic stability, and this excellent electrochemical performance is attributed to the 2D framework of the graphene sheets, large surface area, ordered mesoporous structures that are capable to withstand the high volume expansion and intercalation of the lithium ions on both sides of the graphene sheets.
Graphene as Anode in Lithium Ion Battery
Ren et al.  have designed a typical procedure for the production and engineer the pores in the graphene named as hierarchical porous graphene aerogel (HPGA) prepared by a hydrothermal self-assembly process and an in situ carbothermal reaction. HPGA having different pore sizes such as 50 nm (HPGA-50), 20 nm (HPGA-20) are synthesized that has achieved superior discharge capacity of 1100 mAh g−1 (HPGA-50) and 700 mAh g−1 (HPGA-20) at a current rate of 100 mA g−1 after 100 charge–discharge cycles. This high lithium storage is due to the typical structure of HPGA having pores where the lithium ions can be adsorbed and intercalated on both sides of the graphene sheets and it has also been observed that HPGA having larger mesopores has much higher reversible capacity and cyclic stability. The capacity is also measured at different charge–discharge rates that reveal ultrahigh performance (400 mAh g−1 @ 10 A g−1, 300 mAh g−1 @ 20 A g−1) that is again due to the presence of abundant and uniform mesopores that reduce the lithium-ion diffusion path. The doping of porous graphene with N is an alternative way to enhance the electrochemical properties of graphene. For example, N-doped porous graphene sheets functionalized with polypyrrole by thermal activation has achieved excellent capacity (1336.3 mAh g−1 after 160 cycles @ 100 mA g−1) and rate capability (133.2 mAh g−1 @ current density of 40 A g−1) . Jiang et al.  has reported the synthesis of nitrogen-doped graphene hollow microspheres by a template method that shows very good lithium storage capacity of 753.7 mAh g−1 (after 50 cycles, current density = 100 mA g−1). Hu et al.  have utilized thermal reduction of graphene oxide with ammonium hydroxide and synthesized nitrogen-doped porous graphene that achieved high discharge capacity (453 mAh g−1 @current density of 2 A g−1 after 550 cycles. Sui et al.  have prepared N-doped porous graphene material (NPGM) by a novel method by mixing melamine–formaldehyde resin with graphene oxide that forms a brown-colored graphene oxide/melamine–formaldehyde (GOMF) hydrogel and black-colored graphene/melamine–formaldehyde (GMF) after heating at 140°C for 12 h in an autoclave. The porous materials could be obtained by thermal treatment of GMF aerogel at 800°C for 1 h at a ramp rate of 10°C min−1. Comparative investigation has been done on LIB performance between NPGM and PGM electrodes with initial discharge capacities of 1,279 and 793 mAh g−1, which decrease to 742 and 621 mAh g−1 in the second cycle. The rate capability study shows a high discharge capacity of NPGM electrode (672 mAh g−1 @ 100 mA g−1) at the 10th cycle, which is much higher than that of PGM electrode (450 mAh g−1). At higher current density (1.5 A g−1), NPGM also shows a high discharge capacity of 317 mAh g−1 after 70th cycle. Cyclic stability study of NPGM reveals reasonably high capacity after 200 cycles (496 mAh g−1 @ 400 mA g−1) which is much higher than graphite as well as other potential materials. The enhanced LIB performance is due to the doping of nitrogen, large surface area, and porous structure of NPGM. N-doped porous graphene sheets having high surface area, crumpled structure has been synthesized by Wang et al.  by chemical activation process by using polypyrrole to functionalize the graphene sheets with KOH. These doped graphene sheets have achieved specific capacity of 1516.2 mAh g−1 @100 mA g−1 (~4 times than commercial graphite), cyclic stability (1336.3 mAh g−1 after 160 cycles @100 mA g−1, 1200.4 mAh g−1 @200 mA g−1 even after 300 cycles), and high rate
Lithium-Ion Batteries and Solar Cells
capability (133.2 mAh g−1 @ 40 A g−1). This indicates that the conventional intercalation mechanism may not be the only reason for this high reversible capacity, and the large irreversible capacity is usually due to the formation of the SEI layer, decomposition of the electrolyte by the surface defects generated due to the N-doping or due to the high surface area of the composite or by the presence of N of the pyridinic nitrogen atoms with a lone pair of electrons that may act as the active site.
8.4.4 CHEMICALLY MODIFIED GRAPHENE FOR FAST-CHARGING LITHIUM-ION BATTERY (LIB) Single-layered graphene (SLG), few-layered graphene (FLG), or reduced graphene oxide (rGO), possessing large surface-to-mass ratio, high electrical conductivity, and high mechanical strength, are promising anode materials for high-capacity, fast-charging LIB. It is theoretically considered that SLG can store Li-ions at both sides and then provide a specific capacity (~740 mAh g−1) two times that of graphite. Since 2008, Itaru et al. have introduced macromolecules, like carbon nanotube or fullerenes, into GNS matrix for improving Li-ion intercalation structure, thus significantly enhancing a specific capacity of GNSs . It was not only found that the charging capacity of the assembled battery monotonically increased with the expanding d-spacing perpendicular to the basal plane of graphene, suggesting a possible electrochemically intercalating mechanism, yielding a high specific capacity of ~780 mAh g−1, but also opened a new avenue for investigation of defect structure on Li-ion adsorbing/diffusion phenomena in defective grapheme . The basal plane of pristine SLG is more difficult to adsorb Li-ion than graphite with van der Waals interaction. Li-ion usually adsorbs on the edge of SLG and forms intercalated compounds of LiC6 or Li0.3C6. Up to now, the best specific capacity of ~1,500 mAh g−1 was reached from a graphene-based LIB that was mainly composed of graphene nanoflake with a lateral dimension of YC3) while Y is the weight percent of IL additive. All the products prepared as above are found to be self-standing and translucent appearance (Figure 11.1). After membrane formation, four peaks assigned to the vibration sorption of TFSI anions (va(SO2), va(CF3), vs(SO2), and va(S-N-S)) appear at around 1344, 1177, 1128, and 1050 cm−1 in FT-IR spectra (Figure 11.2a). The result of polymerization for YC138% is also characterized by FT-IR, during which the intensity of the characteristic peak of the vinyl group (1638 cm−1) significantly decreases as shown in Figure 11.2b, suggesting that most of the vinyl moieties had been reacted and incorporated into
FIGURE 11.2 FT-IR spectra of the samples (a) from 400 to 4000 cm−1 and partially enlarged patterns (b) from 1625 to 1650 cm−1.
the entangled polymer matrix. XRD measurements are performed on the LiTFSI, EMIM-TFSI, YC1-60%, YC2-60%, and YC3-60% samples (Figure 11.3). The XRD pattern of LiTFSI exhibits the multiple characteristic peaks indicating its high extent of crystallinity. After undergoing the formation with polymers/IL, most of the peaks corresponding to LiTFSI are disappeared. Compared to pure EMIM-TFSI, the signal intensity of the peak at 2θ = 13° is decreased effectively and the width of the peak at 2θ = 20° becomes broad, indicating the drastic decrease in both grain size and crystallinity. This result gives the suggestion that the prepared samples are mainly in amorphous states and this may attribute that the interactions among the polymers, IL, and lithium salt decrease the crystallinity of LiTFSI. SEM analysis is used to characterize the surface morphologies. All samples are taken out from the glove box, followed by drying at 80°C in vacuum to ensure
FIGURE 11.3 XRD patterns of LiTFSI, 1E3m-TFSI, and the prepared membranes (YC160%, YC2-60%, and YC3-60%).
Lithium-Ion Batteries and Solar Cells
FIGURE 11.4 SEM images of surface of the electrolytes. (a) YC1, (b) YC2, and (c) YC3 series membrane.
that there is no moisture inside the samples before analysis. Figure 11.4a–c exhibits the top surfaces of the YC1, YC2, and YC3 series membranes, respectively. It can be found that these membranes are composed of continuous structures. And the morphology can be referred to the objective evidence of the interactions among the polymer, IL, and LiTFSI domains. For the samples of YC1-38%, YC2-38%, and YC3-38%, some LiTFSI was not dissolved in the matrix completely due to the high crystallinity of the lithium salt, and the corresponding images reveal several particles as well as uneven micropores. With the increase in the IL amount over 60%, their surfaces become homogeneous without any micropores and the LiTFSI particles are well dissolved, which also means most of the added additive can be perfectly trapped inside the polymer matrix. We suggest that the amount of IL influence the miscibility of the composition, and thus, the dispersion of LiTFSI in the polymer matrix can be well improved by adding enough IL. In addition, our previous research claims that the micropores on the membrane surface can be referred to the void spaces that do not facilitate the ion transportation and, instead, increase the interfacial resistance between the electrolytes and the electrodes. Furthermore, the irregular distribution of micropores may result in random deposition of solid electrolyte interphase (SEI) layer during charge–discharge, which is not beneficial to the long-term cycles. Consequently, our SEM images show that the addition of 60 wt% IL not only can improve the solubility of lithium salt but also can afford the formation of membranes without any micropores. It seems that 60 wt% IL can meet a standard and would be regarded as our first choice for further testing.
THERMAL PROPERTIES OF ELECTROLYTES
TGA measurements of the electrolytes are conducted to investigate their thermal properties. The resulting curves exhibit that all of the samples do not have apparent weight loss below 330°C as shown in Figure 11.5a. Their decomposition temperatures (Td5%), which are defined as the temperatures with 5% of weight loss, are found to range between 354°C and 376°C, as listed in Table 11.1. It appears clearly
(a) TGA and (b) DSC thermograms of the prepared membranes.
that these samples exhibit one-step thermal decomposition behavior due to the good mixing of each composition and the whole structures start to decompose at around 330°C. It can be found that their Td values increase with the increment in the IL amount. It sounds a little subversion from our knowledge. This trend is due to the truth that IL possesses higher thermal stability than that of PEG-based polymers
Lithium-Ion Batteries and Solar Cells
even if it is in liquid phase at room temperature. Thus, their thermal stability can be enhanced with the increase in the IL amount. We can also find that the samples with the same amount of IL exhibit the same profiles, which further confirms that their thermal behaviors are mainly dominated by IL. Consequently, the samples exhibit qualified thermal stabilities with the high Td, which would render them to exhibit safety once the batteries are overheating. To realize the phase behaviors as a function of temperature of the prepared electrolytes, DSC analysis is used and the resulting curves are shown in Figure 11.5b. As observed from DSC curves, the melting points (Tm) of the samples are lower than −50°C without any endothermic peaks. The Tm and crystallinity of the materials effectively decrease after the addition of IL and LiTFSI. This decrease can be regarded as the truth that the existence of IL domain can restrict the polymer domains to pack neatly and the polymer/IL/LiTFSI domains exhibit good compatibility with each other, which hence results in lower crystallinity. The results also correspond to those from XRD measurements presented in Figure 11.3.
IONIC CONDUCTIVITY AND ELECTROCHEMICAL WINDOWS
In order to realize how the composition and temperature impact the ionic conductivities of the materials, their ionic conductivities are measured and compared from 30°C to 80°C. The result is shown in Figure 11.6a, and the values at 30°C are shown in Table 11.1. All the electrolytes are found to have higher conductivities with increasing temperature. From our experience, the value of the ionic conductivity should be higher than 10 −4 S cm−1 to meet the requirement of charge–discharge and plays an important factor to affect the performance of batteries.39,40 It is great that our samples demonstrate excellent conductivities over the measured temperature range, which are qualified for further electrical evaluation. Moreover, the increase in IL from 38% to 60% can increase the ionic conductivity to almost one order, given that there are studies showing that IL can serve as the plasticizer to lower
FIGURE 11.6 (a) Ionic conductivity as a function of temperature of the electrolytes. (b) LSV diagram of the electrolytes.
the viscosity and increase the ability of ion transportation. However, the ionic conductivity expected to depend on the contents of IL does not follow the trend in the case of YC1-80%. The continuous addition of IL to 80 wt% only increases the ionic conductivity slightly. Compared to the corresponding SEM images of YC1-60% and YC1-80%, their surfaces have already become homogeneous without obvious difference, and the micro-phase morphologies would not be excessively affected by 60 or 80 wt% of the IL addition. Thus, the ionic conductivity of YC1-80% finally shows no significant enhancement. Referring to the current result, the minimum content of IL, which can construct a homogeneous morphology, dissolve lithium salt completely, and exhibit a relatively high ionic conductivity, is around 60 wt% with respect to the total mass. The further increase in IL would not lead to a significant change in morphology and ionic conductivity. Furthermore, the excess of IL would keep us remain suspicion to the electrochemical stability of the material, which would be explained in the next paragraph. The electrochemical stabilities of the electrolytes are investigated using LSV test (Figure 11.6b). The membranes with higher IL contents result in the decrease in the onset oxidation voltage (YC1-38% > YC1-60% > YC1-80%, YC2-38% > YC2-60%, and YC3-38% > YC3-60%). When the IL addition is adjusted to the same concentration, YC1 series possesses the highest values of the onset oxidation voltage (YC138% > YC2-38% > YC3-38%, and YC1-60% > YC2-60% > YC3-60%), among all. In general, the onset oxidation voltage of the electrolyte should be higher than 4.5 V (vs. Li+/Li) to meet the standard with enough electrochemical stability.41,42 Our results, however, show the onset oxidation voltage in the range from 3.9–to 4.4 V (vs. Li+/ Li), which may cause structural damage at high voltage. To solve this defect, we have improved the step of polymerization as described in the experiment chapter, and the onset oxidation voltage of YC1-60% can increase to about 4.6 V after we perform the photopolymerization directly on the electrode.
CHARGE–DISCHARGE CAPACITY AND CYCLIC PERFORMANCE
The membranes of YC1-60%, YC2-60%, and YC3-60% are assembled in the cells with LiFePO4 and lithium metal as the cathode and anode, respectively. Figure 11.7a–c shows the charge–discharge curves of the batteries based on YC1-60%, YC2-60%, and YC3-60%. Their corresponding discharge capacity values at specific rates are summarized in Figure 11.8. Note that the charge and discharge rates are set from 0.1 to 1 C. As can be seen, all the cells can deliver around 140 mAh g−1 of the capacity at 0.1 and 0.2 C rates without obvious difference. However, the cell with YC1-60% exhibits higher discharge capacities than those with YC2-60% and YC3-60% at high C rates. Considering that they possess similar ionic conductivity, the superior performance of YC1-60% can be referred to its better mechanical stability and electrochemical stability, which has been confirmed by the truth that YC1-60% membrane has the highest degree of cross-linking and the relatively qualified value of onset oxidation voltage shown in Figure 11.6b. As mentioned previously, the low electrochemical stability may cause structural damages at high voltage and that is the fatal flaw our membranes suffer from. Finally, it is difficult to demonstrate long-term charge–discharge without improving the method of polymerization.
Lithium-Ion Batteries and Solar Cells
FIGURE 11.7 Discharge curves of the Li/LiFePO4 cells based on (a) YC1-60%, (b) YC260%, and (c) YC3-60% at different C rates at 80°C.
FIGURE 11.8 Discharge capacities of the Li/LiFePO4 cells based on (a) YC1-60%, (b) YC260%, and (c) YC3-60% at different C rates at 80°C.
Hence, all membranes were polymerized on electrodes directly, and YC1-60% is chosen to demonstrate the charge–discharge test again at 80°C to check if the capacity can be improved. The result is shown in Figure 11.9. The cell based on YC1-60% prepared by the new method exhibits excellent charge–discharge capacities. The discharge capacities at 0.1, 0.2, 0.3, and 0.5 C are measured to be 161.0, 167.0, 165.0, and 164.0 mAh g−1, respectively; these values are almost as high as 97% of the theoretical value of LiFePO4. Their perfect platform of charge–discharge also indicated the improvement of polarization. The gap between the platform of charge and discharge is only around 150 mV even at 0.5 C rate. In addition, the Coulombic efficiency is determined as the ratio of the discharge capacity to the charge capacity. The values of our batteries are always higher than 97% throughout the cycling process, revealing their high charge transfer reversibility. Note that the lower Coulombic efficiencies during the process of 0.1 C rate may be regarded as the reason of incomplete activation. It seems that the increased capacity, improved stability and the lower voltage polarization can be regarded as decreased interfacial resistances between electrolytes/electrodes, which can possibly be attributed to our new method of photopolymerization. Furthermore, the long-term charge–discharge cycling can provide a comprehensive evaluation of the electrolyte system since the thermal stability, mechanical stability, chemical stability, electrochemical stability, ionic conductivity, and durability of the materials are all factors that would affect the cycling performance. As shown in Figure 11.9, the discharge capacities of the cell based on YC1-60% are maintained at a steady value (higher than 160 mAh g−1), confirming that the material can afford more than 20 cycles without faded performance. In summary, polymerization and membrane formation on the cathode directly can effectively decrease the impedance of interface and improve the stability, contributing to the better performance while charging/discharging. We compare the current results with some existing IL-based electrolytes, which can be classified into tetraalkylammonium-based electrolytes, guanidinium-based electrolytes, pyrrolidinium-based electrolytes, and imidazolium-based electrolytes. The battery performances of the above researches are concluded in Table 11.2. For example, tetraalkylammonium-based electrolytes were developed by Li et al., and revealed a discharge capacity of 120 mAh g−1 at 60°C for the assembled Li/ LiFePO4 cell.43 Guanidinium-based electrolytes were also made by the group of Li et al. and the assembled Li/LiFePO4 cell can deliver a capacity to around 130 mAh g−1 at 80°C,44 while Appetecchi et al. prepared the pyrrolidinium-based electrolyte to export a capacity of around 145 mAh g−1 at 40°C.18 And Yin et al. demonstrated the imidazolium-based electrolytes to show a capacity of 160 mAh g−1 at 40°C.16 All these results were conducted at 0.1 C rate. The ionogels used in this research, by contrast, possess a charge–discharge performance of 164.0 mAh g−1 at 0.5 C rate and 60°C, which is superior to the above literatures. Moreover, most of these electrolytes were prepared through thermal polymerization and formed by solvent casting, which is a relatively complicated, costly, and time-consuming process. In this research, the method of photopolymerization is an innovative process of preparation as it combines the steps of polymerization and solvent casting without the use of any organic solvent, which is conducive to shortening the preparation time and increasing the cost-effectiveness.
Lithium-Ion Batteries and Solar Cells
FIGURE 11.9 Charge–discharge curves of the Li/LiFePO4 cell based on YC1-60% prepared by curing on the cathode directly.
TABLE 11.2 Summary of the Performance of Li/LiFePO4 Cells Assembled with Various Types of Ionic Liquid–Based Electrolytes Kinds of Ionic Liquid–Based Electrolytes
Li/LiFePO4 Cell Capacity (mAh g−1)
120 (0.1 C, 60°C)
130 (0.1 C, 80°C)
145 (0.1 C, 40°C)
160 (0.1 C, 40°C)
164 (0.5 C, 60°C)
The imidazolium-based ionogels with various amounts of ionic liquid additive and degrees of cross-linking are prepared via facile photopolymerization and evaluated for application in lithium–ion batteries. The membranes with enough addition of ionic liquid exhibit high ionic conductivity and good miscibility between the components, thus resulting in homogeneous surface without any micropores. Some of the membranes exhibit qualified electrochemical windows, evidenced by the relatively high onset oxidation voltages (4.5 V). Moreover, the discharge capacities of the cell based on YC1-60% can reach 165 mAh g−1 even at 0.5 C rate. The cell also exhibits excellent capacity retention to 20 cycles. The above properties would render these types of membranes to be a promising candidate as the polyelectrolyte for Li/ LiFePO4 batteries.
REFERENCES 1. M. Armand and J. M. Tarascon, Nature, 2008, 451, 652–657. 2. B. Kang and G. Ceder, Nature, 2009, 458, 190–193. 3. Y. K. Sun, S. T. Myung, B. C. Park, J. Prakash, I. Belharouak and K. Amine, Nat Mater, 2009, 8, 320–324. 4. B. Scrosati and J. Garche, J Power Sources, 2010, 195, 2419–2430. 5. P. G. Balakrishnan, R. Ramesh and T. P. Kumar, J Power Sources, 2006, 155, 401–414. 6. J. B. Goodenough and Y. Kim, Chem Mater, 2010, 22, 587–603. 7. S. F. Lux, I. T. Lucas, E. Pollak, S. Passerini, M. Winter and R. Kostecki, Electrochem Commun, 2012, 14, 47–50. 8. M. Smiglak, W. M. Reichert, J. D. Holbrey, J. S. Wilkes, L. Y. Sun, J. S. Thrasher, K. Kirichenko, S. Singh, A. R. Katritzky and R. D. Rogers, Chem Commun, 2006, 2554–2556. doi: 10.1039/b602086k. 9. M. J. Earle, J. M. S. S. Esperanca, M. A. Gilea, J. N. C. Lopes, L. P. N. Rebelo, J. W. Magee, K. R. Seddon and J. A. Widegren, Nature, 2006, 439, 831–834. 10. H. Nakagawa, Y. Fujino, S. Kozono, Y. Katayama, T. Nukuda, H. Sakaebe, H. Matsumoto and K. Tatsumi, J Power Sources, 2007, 174, 1021–1026. 11. Y. D. Jin, S. H. Fang, M. Chai, L. Yang, K. Tachibana and S. Hirano, J Power Sources, 2013, 226, 210–218. 12. X. G. Sun, C. Liao, N. Shao, J. R. Bell, B. K. Guo, H. M. Luo, D. E. Jiang and S. Dai, J Power Sources, 2013, 237, 5–12. 13. H. Sakaebe, H. Matsumoto and K. Tatsumi, Electrochim Acta, 2007, 53, 1048–1054. 14. A. Fernicola, F. Croce, B. Scrosati, T. Watanabe and H. Ohno, J Power Sources, 2007, 174, 342–348. 15. M. Galinski, A. Lewandowski and I. Stepniak, Electrochim Acta, 2006, 51, 5567–5580. 16. K. Yin, Z. X. Zhang, X. W. Li, L. Yang, K. Tachibana and S. I. Hirano, J Mater Chem A, 2015, 3, 170–178. 17. K. Yin, Z. X. Zhang, L. Yang and S. I. Hirano, J Power Sources, 2014, 258, 150–154. 18. G. B. Appetecchi, G. T. Kim, M. Montanina, M. Carewska, R. Marcilla, D. Mecerreyes and I. De Meatza, J Power Sources, 2010, 195, 3668–3675. 19. X. W. Li, Z. X. Zhang, S. J. Li, L. Yang and S. Hirano, J Power Sources, 2016, 307, 678–683. 20. M. Safa, A. Chamaani, N. Chawla and B. El-Zahab, Electrochim Acta, 2016, 213, 587–593.
Lithium-Ion Batteries and Solar Cells
21. P. F. Zhang, M. T. Li, B. L. Yang, Y. X. Fang, X. G. Jiang, G. M. Veith, X. G. Sun and S. Dai, Adv Mater, 2015, 27, 8088–8094. 22. A. S. Shaplov, P. S. Vlasov, E. I. Lozinskaya, D. O. Ponkratov, I. A. Malyshkina, F. Vidal, O. V. Okatova, G. M. Pavlov, C. Wandrey, A. Bhide, M. Schonhoff and Y. S. Vygodskii, Macromolecules, 2011, 44, 9792–9803. 23. X. J. Chen, J. Zhao, J. Y. Zhang, L. H. Qiu, D. Xu, H. G. Zhang, X. Y. Han, B. Q. Sun, G. H. Fu, Y. Zhang and F. Yan, J Mater Chem, 2012, 22, 18018–18024. 24. R. Tejero, D. Lopez, F. Lopez-Fabal, J. L. Gomez-Garces and M. Fernandez-Garcia, Polym Chem-UK, 2015, 6, 3449–3459. 25. S. Yi, W. Leon, D. Vezenov and S. L. Regen, ACS Macro Lett, 2016, 5, 915–918. 26. M. M. Obadia, A. Jourdain, A. Serghei, T. Ikeda and E. Drockenmuller, Polym Chem-UK, 2017, 8, 910–917. 27. M. Yoshizawa, M. Hirao, K. Ito-Akita and H. Ohno, J Mater Chem, 2001, 11, 1057–1062. 28. F. Lind, L. Rebollar, P. Bengani-Lutz, A. Asatekin and M. J. Panzer, Chem Mater, 2016, 28, 8480–8483. 29. F. Lu, X. P. Gao, A. L. Wu, N. Sun, L. J. Shi and L. Q. Zheng, J Phys Chem C, 2017, 121, 17756–17763. 30. N. Sun, X. P. Gao, A. L. Wu, F. Lu and L. Q. Zheng, J Mol Liq, 2017, 248, 759–766. 31. M. E. Taylor and M. J. Panzer, J Phys Chem B, 2018, 122, 8469–8476. 32. Y. Yu, F. Lu, N. Sun, A. L. Wu, W. Pan and L. Q. Zheng, Soft Matter, 2018, 14, 6313–6319. 33. R. X. He, M. Echeverri, D. Ward, Y. Zhu and T. Kyu, J Membr Sci, 2016, 498, 208–217. 34. G. P. Fu, J. Dempsey, K. Izaki, K. Adachi, Y. Tsukahara and T. Kyu, J Power Sources, 2017, 359, 441–449. 35. G. P. Fu and T. Kyu, Langmuir, 2017, 33, 13973–13981. 36. G. P. Fu, M. D. Soucek and T. Kyu, Solid State Ionics, 2018, 320, 310–315. 37. C. Piedrahita, V. Kusuma, H. B. Nulwala and T. Kyu, Solid State Ionics, 2018, 322, 61–68. 38. S. Stalin, S. Choudhury, K. H. Zhang and L. A. Archer, Chem Mater, 2018, 30, 2058–2066. 39. K. S. Liao, T. E. Sutto, E. Andreoli, P. Ajayan, K. A. McGrady and S. A. Curran, J Power Sources, 2010, 195, 867–871. 40. S. Inceoglu, A. A. Rojas, D. Devaux, X. C. Chen, G. M. Stone and N. P. Balsara, ACS Macro Lett, 2014, 3, 510–514. 41. K. Karuppasamy, P. A. Reddy, G. Sriniyas, A. Tewari, R. Sharma, X. S. Shajan and D. Gupta, J Membr Sci, 2016, 514, 350–357. 42. Y. S. Yun, J. H. Kim, S. Y. Lee, E. G. Shim and D. W. Kim, J Power Sources, 2011, 196, 6750–6755. 43. M. T. Li, B. L. Yang, L. Wang, Y. Zhang, Z. Zhang, S. H. Fang and Z. X. Zhang, J Membr Sci, 2013, 447, 222–227. 44. M. T. Li, L. Yang, S. H. Fang, S. M. Dong, S. Hirano and K. Tachibana, J Power Sources, 2011, 196, 8662–8668.
Back-Contact Perovskite Solar Cells Tai-Fu Lin, Ming-Hsien Li, Pei-Ying Lin, Itaru Raifuku, Joey Lin, and Peter Chen National Cheng Kung University
CONTENTS 12.1 Introduction .................................................................................................. 219 12.2 Coplanar Back-Contact Structure ................................................................. 221 12.3 Non-Coplanar Back-Contact Structure......................................................... 223 12.4 Conclusion .................................................................................................... 228 References .............................................................................................................. 230
12.1 INTRODUCTION When the ion-based batteries are charging, batteries can convert electricity into chemical energy which is stored in batteries. While discharging, ion-based batteries undergo a reverse process to convert chemical energy into electricity for charging other devices. The working principle of solar cells is totally different to the ionbased batteries. The solar cells can convert solar light (photon energy) into electricity (chemical potential of electron) which cannot be stored in solar cells. As a result, solar cells cannot work without solar light illumination. It is worth noting that the solar cells have the potential to integrate with ion-based batteries for constructing a renewable energy system with light harvesting and energy storage. The solar cells can serve as a power supply for charging the ion-based batteries. In conventional perovskite solar cells (PSCs), perovskite light absorber with several hundred nanometer thickness is sandwiched by two selective contact electrodes, namely electron-selective layer (ESL) and hole-selective layer (HSL), as revealed in Figure 12.1a. Typically, a transparent conducting oxide (TCO) layer, such as indium tin oxide (ITO) or fluorine-doped tin oxide (FTO), serves as the illumination window. The light enters the solar cells from the glass substrate, TCO layer, HSL, or ESL and is finally absorbed by the perovskite absorber. The electron and hole excited in perovskite active layer will diffuse in the opposite direction and be collected by the ESL and HSL, respectively. The optical transmission loss due to the refractive index mismatch, scattering from rough surface, and parasitic absorption of carrier transport material reduces the incident light intensity along with the optical flux. Moreover, deposition of carrier transport layer on the top of perovskite could require high temperature or harsh chemical process that could damage the perovskite layer. 219
Lithium-Ion Batteries and Solar Cells
The perovskite solar cells employing back-contact architecture, the so-called back-contact perovskite solar cells (BC-PSCs), can resolve the above issues. In the back-contact architecture, the selective contact of ESL and HSL and metal contacts are patterned and positioned on the same side below the perovskite active layer (refer to Figure 12.1b and c). Such device structure prevents the damage of top electrode deposition on the perovskite active layer and allows the light illumination directly on the perovskite absorber to reduce the optical transmission loss. The bottom TCO layer can be replaced with a metal electrode that provides a lower sheet resistance than TCO and reduces the resistive loss of device. According to the position of patterned electrodes, the BC-PSCs can be divided into coplanar and non-coplanar types. Figure 12.1b shows the BC-PSCs with coplanar finger electrodes, namely interdigitated electrode (IDE), in which two finger electrodes are patterned and interdigitated to separately collect carriers. The carrier diffusion length of perovskite is usually within few micrometers . The gap between electron- and hole-selective finger electrodes is highly controlled to collect carrier before recombination. Photolithographic techniques are generally applied to fabricate IDE; however, the integrity of finger electrode is critical to the charge collection. To simplify the fabrication process, Udo Bach’s group proposed BC-PSCs with noncoplanar finger electrodes, namely quasi-interdigitated electrode (QIDE), in which an insulator is inserted between top patterned electrode and bottom planar electrode as shown in Figure 12.1c [2,3]. Inserting an insulator between them can effectively prevent the short-circuit contact between two selective electrodes. Furthermore, we can increase finger density, compared to the IDE structure, to further enhance charge collection capability.
FIGURE 12.1 Device structure of (a) sandwiched PSCs, (b) IDE-based BC-PSCs, and (c) QIDE-based BC-PSCs.
Back-Contact Perovskite Solar Cells
COPLANAR BACK-CONTACT STRUCTURE
T. Ma et al. used a numerical simulation to investigate the structural parameters in terms of finger electrode width and gap on the photovoltaic performance of the coplanar back-contact-type perovskite solar cell . The coplanar back-contact-type structure is shown in Figure 12.2a, in which the finger electrode of HSL and ESL with the same finger width are placed at the same plane and staggered to form a gap between two finger electrodes. Metal oxide semiconductors of TiO2 and NiO are respectively used as ESL and HSL in the simulation. Figure 12.2b shows the calculated J-V
FIGURE 12.2 (a) Structures of the coplanar back-contact-type structure; calculated (b) J-V curves and (c) EQE response of coplanar back-contact-type (black line) and sandwich-type (gray line) perovskite solar cell .
Lithium-Ion Batteries and Solar Cells
curves of PSCs with the sandwich and the coplanar back-contact structures. The short-circuit current density (JSC) of coplanar back-contact structure exhibits an optimized value of 24.3 mA cm−2 when the width and gap are 1 and 0.1 μm, respectively, leading to a power conversion efficiency (PCE) of 22.77%. The traditional sandwich structure delivers a lower efficiency mainly due to a reduced JSC of 21.7 mA cm−2. The increased JSC in BC-PSCs is attributed to the reduced light loss at short wavelength region (300–380 nm) as shown in the calculated external quantum efficiency (EQE) spectra (refer to Figure 12.2c). The authors also identify that the default value of finger electrode width ≤5 μm and gap ≤0.5 μm in coplanar BC-PSCs is acceptable for achieving high-efficiency BC-PSCs and simplifying the fabrication process. It is a common technique to introduce self-assembled monolayers (SAMs) to modify the work function (WF) of metals and semiconductors in organic light-emitting diodes and organic field-effect transistors. The molecular assemblies reorganize into oriented arrange and spontaneously form on surfaces by adsorption. SAMs can affect the energy level by imparting a dipole moment on the surface [5–8]. In order to align the potential difference between two finger electrodes, U. Bach’s group apply SAM treatment at the gold–perovskite interfaces to modulate the work function of gold finger electrodes [9,10]. The interdigitated gold electrode is immersed into a 4-methoxythiophenol (OMeTP) solution, resulting in the formation of OMeTP SAMs on two finger electrodes. The OMeTP SAM on anode is subsequently desorbed electrochemically. The desorbed Au electrode is then exposed to a solution of 4-chlorothiophenol (CITP) in order to form the cathode electrode. Kelvin probe force microscopy (KPFM) is used to measure the surface potential changes of the interdigitated gold electrode after surface modification. The formation of the OMeTP SAM on electrode increases contact potential difference (CPD) of 400 mV relative to the bare electrode, and the CPD relative to the bare electrode further increases to 550–580 mV after CITP treatment. The encapsulated device delivers a VOC of 0.55 V, a JSC of 9.73 mA cm−2 and a FF of 36.7%, leading to a PCE of 1.96%. The much lower photovoltaic performance of SAM-modified back-contact PSC is mainly attributed to the gap between interdigitated fingers. The gap of SAM-modified back-contact PSC is ~4.3 μm, which is almost tenfold the ideal value of 0.5 μm as demonstrated by simulation. The photogenerated carriers would recombine before they reach interdigitated finger electrodes. Moreover, the SAM-modified interdigitated finger electrodes only deliver less than 600 mV in work function difference, leading to a reduction in open-circuit voltage (VOC) of the resultant device . The same group further optimize the device performance by controlling the perovskite grain size, since the charge-carrier diffusion length is related to perovskite grain size . They grow four grain cluster sizes of perovskite which are approximately 6.0, 2.0, 0.99, and 0.23 μm and denoted as large (L), medium (M), small (S), and extra small (XS), respectively. The maximum theoretical VOC from BC-PSCs is determined by the work function difference induced by the self-assembled dipole monolayers coated on the gold electrodes. The VOC increases with the perovskite grain size, showing an average value of 0.46, 0.4, 0.31, and 0.09 V for L, M, S, and XS cluster sizes, respectively. The average JSC values for devices with L, M, S, and XS cluster sizes are 9.44, 7.64, 5.88, and 0.69 mA cm−2, respectively. However, there is no clear
Back-Contact Perovskite Solar Cells
trend in FF for devices with different grain size. It is noted that perovskite films with large cluster sizes exhibit longer charge recombination lifetimes, leading to a higher VOC. Bach’s group provided an approach via SAM treatment and optimized the device performance by improving the quality of the perovskite film and/or reducing the gap between the interdigitated electrodes. These pioneering works give a new insight into further advancing the photovoltaic performance of back-contact perovskite solar cells.
NON-COPLANAR BACK-CONTACT STRUCTURE
A. N. Jumabekov et al. first reported the QIDE-based BC-PSCs in 2016 . Figure 12.3a shows the fabrication process of QIDE-based BC-PSCs. ZnO is sputtered on the ITO substrate to serve as ESL. Photoresist layer is spin-coated onto the substrate and exposed to UV light through a chrome metal photomask. The UV-exposed regions are removed using developer solution, and then, Al2O3, Al, and Ni layers are sequentially evaporated onto the substrate using electron-beam evaporator. Then, residual photoresist was removed by washing the substrates in acetone. HSL finger electrode is formed by oxidizing the surface of Ni and Al layer with an annealing temperature of 300°C. After that, the device was completed by depositing perovskite layer onto the QIDE. Figure 12.3b shows the band diagram of QIDE-based BC-PSCs. Electron and hole generated in perovskite layer are respectively collected by ZnO/ITO and NiOx/
FIGURE 12.3 (a) Fabrication process, (b) band diagram and maximum power point tracking, and (c) J-V characteristic curves of QIDE-based BC-PSCs .
Lithium-Ion Batteries and Solar Cells
Ni/Al electrodes. Al2O3 layer acts as an insulator to prevent direct contact between cathode and anode. Figure 12.3c shows the J-V curves of the QIDE-based BC-PSCs. For the device illuminated from the perovskite layer (top illumination), the BC-PSCs under reverse scan obtain a PCE of 6.54% with a JSC of 12.95 mA cm−2, a VOC of 0.98 V, and a FF of 51.5%. The device under forward scan shows a PCE of 3.68%, indicating the device exhibited a large hysteresis. They also carried out maximum power point tracking to determine the steady-state PCE. The devices show a stable power output with a PCE of around 3.2%, which is similar to the PCE value under forward scan. The origin of hysteresis in common perovskite solar cells has been discussed, and some reasons such as ferroelectric effect, ion migration, and capacitance effect have been suggested [11–13]. However, there is no discussion about the hysteresis in BC-PSCs. Therefore, investigating the origin of hysteresis in BC-PSCs would be one of the interesting topics. When the device is illuminated from the substrate (bottom illumination), the device shows a PCE of 3.52% with a JSC of 7.7 mA cm−2, a VOC of 0.95 V, and a FF of 48.11%. As shown in Figure 12.4a, metal electrode causes the optical loss due to its light absorption and reflection. To overcome the optical losses, G. DeLuca et al. proposed BC-PSCs with semitransparent QIDE by replacing the metal electrodes with the transparent ITO electrodes . The cross-sectional SEM image of the semitransparent QIDE-based BC-PSCs is shown in Figure 12.4b. First, they optimized the deposition process of ITO transparent electrode to deliver a sheet resistance of 25–35 Ω sq−1. CuSCN is applied as HSL to match the work function of ITO. The device illuminated from the perovskite layer achieves a PCE of 1.37% with a JSC of 5.52 mA cm−2, a VOC of 0.84 V, and a FF of 0.30. By contrast, when the device is illuminated from the back side, a higher PCE of 1.66% is obtained with a JSC of 5.60 mA cm−2, a VOC of 0.88 V, and a FF of 0.34. A similar JSC value indicates that the absorption loss by conventional QIDE is successfully improved by substituting the metal electrode with the ITO electrode. They also performed simulations that reveal that the PCE of semitransparent QIDE-based BC-PSCs can be improved up to 11.5% and 13.3% for the front and back illumination, respectively. Recently, G. D. Tainter et al. reported QIDE-based BC-PSCs employing SnO2 and NiOx as ESL and HSL, respectively, whose device architecture is illustrated in Figure 12.5a . Figure 12.5b shows the J-V curve of QIDE-based BC-PSCs with a gap of 1 μm for NiOx finger electrode. The device illuminated from the perovskite
FIGURE 12.4 (a) Light transmission, absorption, and reflection paths in QIDE with metal electrodes (left) and transparent electrodes (right). (b) Cross-sectional SEM of the semitransparent QIDE-based BC-PSCs .
Back-Contact Perovskite Solar Cells
FIGURE 12.5 (a) Schematic illustration of QIDE-based BC-PSCs. (b) J-V curves of QIDEbased BC-PSCs with NiOx finger gap of 1 μm. Dependence of (c) laser-induced photocurrent and (d) rise time with distance from the electrode junction .
layer shows a PCE of 4.1% with a JSC of 18.4 mA cm−2, a VOC of 0.57 V, and a FF of 38%. Figure 12.5c and d represent the laser-induced photocurrent and rise time as a function of electrode position. The calculated surface recombination velocity is 1.7 and 1.1 cm s−1 for the perovskite covered on the NiOx and SnO2 surface, respectively. The hole and electron carrier lifetime for the region of perovskite film coverage on the SnO2 and NiOx electrode are calculated to be 27 and 17 μs, respectively. Low surface recombination velocity along with long carrier lifetime supports high JSC value of QIDE-based BC-PSCs. It is noted that QIDE-based BC-PSCs suffer from lower VOC and FF than the conventional perovskite solar cells due their poor shunt resistance. Further optimization on the device architecture or fabrication process is required to improve the photovoltaic performance. Although the top-down approach for the fabrication of interdigitated electrodes via the photolithography or electron-beam lithography is well established, the finger electrode could be easily broken or even disconnected during the photolithography process. Such damage in finger electrode hinders the charge extraction and collection. Udo Bach’s group replaced the finger electrode with the porous electrode by applying a sacrificial lithographic mask that provides facile, large-area, and cost-effective fabrication for the QIDE-type BC-PSCs . The fabrication process of porous QIDE is shown in Figure 12.6. The authors introduced self-assembled monolayers of (3-aminopropyl)triethoxysilane (APTES) to functionalize the TiO2/FTO substrate
Lithium-Ion Batteries and Solar Cells
FIGURE 12.6 Fabrication process of porous QIDE-based BC-PSCs: (a) patterned FTO/TiO2 anode substrate; (b) APTES SAM treatment on the top of anode; (c) immersion of substrate in the colloidal suspension to assemble the polystyrene microbeads; (d) monolayer of polystyrene microbeads assembled on the surface of TiO2 anode; (e) plasma etching for reducing the size of polystyrene microbeads; (f) deposition of counter electrode and cathode; (g) removal of polystyrene microbeads; (h) photographic image of porous QIDE-based BC-PSCs .
(refer to Figure 12.6a), which facilitates the formation of dense monolayer of microbeads on the substrate (refer to Figure 12.6b). The coverage of microbeads on the substrate surface can be controlled by the pH value of the colloidal solution which adjusts the electrostatic attraction between negatively charged microbeads and positively charged substrate. The colloidal suspension with a pH value of 5.5 is prepared, which contains 1-μm-sized polystyrene microbeads with carboxyl groups. The substrate is dipping into colloidal suspension (refer to Figure 12.6c), on which the microbeads are self-assembled to form a monolayer as presented in Figure 12.6d. The plasma etching for the polystyrene microbeads was employed to define the width of porous electrode (refer to Figure 12.6e). An Al2O3 insulating layer (120 nm), an Al wetting layer (30 nm), and NiCo alloy (50 nm) are sequentially evaporated onto the microbead-coated substrate using electron-beam evaporation (refer to Figure 12.6f). The porous electrode is thus formed by removing the microbeads with toluene or tetrahydrofuran (refer to Figure 12.6g). After the annealing treatment at 300°C for 15 min, the porous electrode was completed by converting NiCo into NiCoOx cathode. The perovskite light absorber is finally deposited on the top of porous electrode to complete the BC-PSCs with an architecture of FTO/TiO2/Al2O3/Al/NiCo/NiCoOx/perovskite. The deprotonation of carboxyl groups on microbeads surface leads to negatively charged microbeads, while the protonation of amine groups of APTES gives rise to the TiO2-coated substrate with positive charge. As a result, the deposition rate of
Back-Contact Perovskite Solar Cells
microbeads on the APTES-treated substrate is higher than that without APTES treatment, resulting in a denser coverage of microbeads as demonstrated in Figure 12.7a (with APTES surface treatment) and b (without APTES surface treatment). After the microbead shrinkage by plasma etching, deposition of Al2O3/Al/NiCo, and removal of microbeads, the surface morphology of porous electrode is thus created as revealed in Figure 12.7c (with APTES surface treatment) and d (without APTES surface treatment). It indicates that APTES-treated substrate exhibits a higher porosity than that without APTES treatment. The enhanced porosity for APTES-treated substrate also increases the transmission across the 300–1100 nm wavelength range (refer to Figure 12.7e). Eventually, the back-contact perovskite solar cells integrated with porous electrode are demonstrated, among which the APES-treated devices deliver a JSC of 7.2 mA cm−2, a VOC of 0.9 V, a FF of 27%, and a PCE of 1.75%. The same group further fabricated a honeycomb QIDE (H-QIDE) in BC-PSC, in which the honeycomb array was well arranged by photolithography . The BC-PSCs integrated with HQIDE are illustrated in Figure 12.8a. The fabrication process and device structure are similar to the previous work except the fabrication of honeycomb QIDE by photolithography. The bottom TiO2 compact layer works as ESL, and the conversion of annealed NiCo into NiCoOx serves as HSL. An Al2O3 insulator is inserted to separate these two electrodes. The electrode dimensions have a dramatic impact on the charge collection and device performance due to the limitation of carrier diffusion length in the perovskite active layer. Two-sized HQIDEs with different diameter and gap are designed and denoted as S-HQIDE (diameter of 2.7 μm and gap of 1.3 μm in Figure 12.8b and c) and L-HQIDE (diameter of 8 μm and gap of 1.5 μm in Figure 12.8d and e). The BC-PSCs integrated with S-HQIDE achieve a better photovoltaic performance (PCE = 5.39%) than the L-HQIDE counterpart (PCE = 1.46%), mainly on the enhanced photocurrent. The result is reasonable since a small-sized HQIDE can enhance the charge collection and thus improve the JSC for the S-HQIDE device.
FIGURE 12.7 SEM images of monolayer polystyrene microbeads on (a) the APTESfunctionalized glass/FTO/TiO2 anode substrate and (b) the glass/FTO/TiO2 anode substrate. SEM images of porous QIDE (c) with and (d) without APTES treatment. The scale bar is 4 μm. (e) UV–Vis–NIR transmission spectra of glass/FTO/TiO2 anode substrate, QIDE without and with APTES treatment .
Lithium-Ion Batteries and Solar Cells
FIGURE 12.8 (a) Fabrication process of HQIDE-based BC-PSCs. (b) AFM and (c) SEM images of S-HQIDE; (d) AFM and (e) SEM images of L-HQIDE .
The same group further demonstrated HQIDE-based BC-PSCs via dipole-field modification on two gold finger electrodes . Two self-assembled benzenethiol derivatives with opposite dipole moments are adsorbed onto the gold electrodes that replace the charge-transporting layers to selectively extract charge due to the work function asymmetry. The fabrication flow is presented in Figure 12.9a. Au/SiO2/Au stacking layer is first deposited on top of the glass substrate. Photo-lithography is employed to define the HQIDE composed of Au/SiO2. Thus, the bottom planar gold layer (denoted as “a”, colored in blue in Figure 12.9b) and top Au/SiO2 mesh (denoted as “b”, colored in red in Figure 12.9b) are separated by SiO2 insulator. The bottom planar gold layer and top gold mesh are surface-modified with monolayer of OMeTP. The honeycomb-shaped top Au/SiO2 electrode is then exposed to CITP solution to undergo oxidative electrochemical reaction and replace OMeTP with CITP SAM. The formation of OMeTP and CITP on bottom planar electrode and top HQIDE, respectively, creates a surface potential difference of 360 mV which is capable of opposite charge extraction. Three feature sizes of HQIDE in terms of honeycomb diagonal length and pitch (denoted as “d” and “p” in Figure 12.9b) are controlled to correlate the device photovoltaic performance. The results indicate that HQIDE-based BC-PSCs having the smallest diagonal length and pitch (d = 5.0 μm and p = 6.2 μm) display the best PCE of 2.61%. Larger feature size limits the charge collection efficiency and the resultant JSC.
In conclusion, we briefly introduce the development of the back-contact perovskite solar cells. The efficiency trend and photovoltaic parameters of back-contact perovskite solar cells are summarized in Figure 12.10 and Table 12.1, respectively. Compared with
Back-Contact Perovskite Solar Cells
FIGURE 12.9 (a) Fabrication flow of HQIDE for BC-PSCs. (b) The work function modification of bottom planar Au electrode (marked by blue) by OMeTP and top HQIDE by CITP (marked by red) .
Efficiency evolution of BC-PSCs.
Lithium-Ion Batteries and Solar Cells
TABLE 12.1 Photovoltaic Parameters of Different Types of BC-PSCs. The Device Illuminated from the Perovskite Layer Is Denoted as “Front,” While that Illuminated from the Substrate Is Denoted as “Back” Type Coplanar
Illumination Side VOC (V) JSC (mA cm−2) FF (%) PCE (%) References IDE
Non-coplanar Porous QIDE QIDE QIDE QIDE HQIDE HQIDE
Front Back Front Back Front Back Front Back Front Front Front Front
0.64 0.64 0.46 0.83 0.98 0.95 0.84 0.88 0.57 0.9 0.7 0.52
9.87 8.77 9.44 7.1 12.95 7.7 5.52 5.6 18.4 7.2 16.4 12.52
37.32 36.69 30.58 66 51.5 48.4 30 34 38 27 46 40.16
2.36 2.23 1.33 3.88 6.54 3.52 1.37 1.66 4.1 1.75 5.39 2.61
        
the conventional sandwiched PSCs, back-contact perovskite solar cells still have much room for improvement in photovoltaic performance. Some key issues are highlighted to improve the performance of back-contact devices. First, in order to increase the charge collection efficiency, the gap of IDE or QIDE should be comparable with the carrier diffusion length of perovskite. Second, the series resistance should be reduced to improve the FF of devices. For instance, ESL and HSL should be well separated by insulator and the metal electrodes are required to be passivated to prevent the carrier recombination at metal electrode/perovskite interface.
REFERENCES 1. Brenner, T.M., et al., Hybrid organic – inorganic perovskites: low-cost semiconductors with intriguing charge-transport properties. Nature Reviews Materials, 2016. 1(1): p. 15007. 2. Jumabekov, A.N., et al., Back-contacted hybrid organic–inorganic perovskite solar cells. Journal of Materials Chemistry C, 2016. 4(15): pp. 3125–3130. 3. DeLuca, G., et al., Transparent Quasi-interdigitated electrodes for semitransparent perovskite back-contact solar cells. ACS Applied Energy Materials, 2018. 1(9): pp. 4473–4478. 4. Ma, T., et al., Unveil the full potential of integrated-back-contact perovskite solar cells using numerical simulation. ACS Applied Energy Materials, 2018. 1(3): pp. 970–975. 5. Goh, C., S.R. Scully, and M.D. McGehee, Effects of molecular interface modification in hybrid organic-inorganic photovoltaic cells. Journal of Applied Physics, 2007. 101(11): p. 114503. 6. Bruening, M., et al., Simultaneous control of surface potential and wetting of solids with chemisorbed multifunctional ligands. Journal of the American Chemical Society, 1997. 119(24): pp. 5720–5728.
Back-Contact Perovskite Solar Cells
7. Liscio, A., et al., Bottom-up fabricated asymmetric electrodes for organic electronics. Advanced Materials, 2010. 22(44): pp. 5018–5023. 8. Kobayashi, S., et al., Control of carrier density by self-assembled monolayers in organic field-effect transistors. Nature Materials, 2004. 3(5): pp. 317–322. 9. Lin, X., et al., Dipole-field-assisted charge extraction in metal-perovskite-metal backcontact solar cells. Nature Communications, 2017. 8(1): p. 613. 10. Lin, X., et al., Effect of grain cluster size on back-contact perovskite solar cells. Advanced Functional Materials, 2018. 28(45): p. 1805098. 11. Wei, J., et al., Hysteresis analysis based on the ferroelectric effect in hybrid perovskite solar cells. The Journal of Physical Chemistry Letters, 2014. 5(21): pp. 3937–3945. 12. Zhang, T., et al., Understanding the relationship between ion migration and the anomalous hysteresis in high-efficiency perovskite solar cells: a fresh perspective from halide substitution. Nano Energy, 2016. 26: pp. 620–630. 13. Cojocaru, L., et al., Origin of the hysteresis in I–V curves for planar structure perovskite solar cells rationalized with a surface boundary-induced capacitance model. Chemistry Letters, 2015. 44(12): pp. 1750–1752. 14. Tainter, G.D., et al., Long-range charge extraction in back-contact perovskite architectures via suppressed recombination. Joule, 2019. 3(5): pp. 1301–1313. 15. Jumabekov, A.N., et al., Fabrication of back-contact electrodes using modified natural lithography. ACS Applied Energy Materials, 2018. 1(3): pp. 1077–1082. 16. Hou, Q., et al., Back-contact perovskite solar cells with honeycomb-like charge collecting electrodes. Nano Energy, 2018. 50: pp. 710–716. 17. Lin, X., et al., Honeycomb-shaped charge collecting electrodes for dipole-assisted backcontact perovskite solar cells. Nano Energy, 2019: p. 104223. 18. Hu, Z., et al., Transparent conductive oxide layer and hole selective layer free backcontacted hybrid perovskite solar cell. The Journal of Physical Chemistry C, 2017. 121(8): pp. 4214–4219.
Engineering of Conductive Polymer Using Simple Chemical Treatment in Silicon Nanowire-Based Hybrid Solar Cells Po-Hsuan Hsiao, Ilham Ramadhan Putra, and Chia-Yun Chen National Cheng Kung University
CONTENTS 13.1 Introduction .................................................................................................. 233 13.2 PEDOT:PSS with Tunable Electrical Conductivity ...................................... 235 13.2.1 PEDOT:PSS Fabricated by “Baytron P” Routes .............................. 235 13.2.2 PSS Functions in Commercial PEDOT:PSS Complex ..................... 236 13.2.3 PSS Investigations of Electrical Conductivity in PEDOT:PSS ........ 237 13.3 Treated PEDOT:PSS for Silicon Nanowires-Based Hybrid Solar Cells.......240 13.4 Conclusion ....................................................................................................246 Acknowledgment ................................................................................................... 247 References .............................................................................................................. 247
The demand for clean energy continues to be followed up by the development of renewable energy coping with the environmentally friendly, cheap, and efficient routes. Solar energy is one of the energy sources offering clean, sustainable, and stable energy. In 2018, the worldwide solar photovoltaic (PV) power was expected to generate approximately 2.8% of the worldwide electricity . In recent years, silicon (Si)-based solar cells have been considered the most widely used type of PV devices. Unfortunately, the manufacturing of this type of solar cells requires a fairly complex process. In this regard, the various types of solar cells followed by the development of alternative materials essentially turn out to be a prospective field on both academic research and industrial applications. The emerging PV structures such as dye-sensitized, organic-based, 233
Lithium-Ion Batteries and Solar Cells
and inorganic thin film-based solar cells are widely being escalated and utilizing various materials. Moreover, one more type of “layer-by-layer” solar cells that possess the potential impact on energy-related applications is hybrid-solar cells. The “hybrid” term is typically known as the sequence of organic–inorganic materials applied for the device with active junction carrying on the charge separation of photogenerated electrons and holes. Further completed device or cell system development utilizing current collector layers as the top and bottom electrodes becomes the main point in various developments of solar cells. The main focus on the device engineering is to build up remarkable performance and efficiency by considering several factors especially the charge transport and separation. These include materials selection, p- and n-type materials, nanostructural approaches, passivation layer, interface contact improvement, and physical engineering techniques such as junction thickness determination. Moreover, several studies spotlighted to other parts, for example, are the electrode materials selection as current collectors and hole (h+) or electron (e−) selective layer applied between the active layer and current collectors. In the organic–inorganic junction, the structure consists of transparent conductive polymer in combination with the inorganic semiconductor, contributing to an adequate transport and separation of photogenerated carriers. From various materials acquired for the cell construction, the arrangement of PEDOT:PSS polymer and n-type crystalline Si was proposed by considering both superiorities. This type of hybrid solar cells has attracted worldwide attention since it was proposed in 2010 and further developed as the potential solar cells at present. Compared with ion-based batteries as the energy-storage system, hybrid solar cells turn out be the efficient way for supplying the electric energy in a stable and reliable way. By combing hybrid solar cells with battery system, this can be an ecofriendly and renewable platform for supplying energy required in use. Thus, this book can be served as the bridge for the readers to fully understand the related technology of energy generation and storage. Poly(3,4-ethylenedioxythiophene):poly(styrenesulfonate) (PEDOT:PSS) is a conductive polymer that offers numerous superiorities such as tunable electrical conductivity by uncomplicated treatments, facile fabrication to form thin film, acceptable thermal stability, material flexibility, and superior transparency in the visible range. In contrast, crystalline Si as the n-type material was considered to offer several advantages such as higher minority carrier lifetime, adjustable doping type, and concentrations, thus making it a preferable candidate for creating p–n junction with p-type organic materials. In this architecture of hybrid solar cells, PEDOT:PSS/planar n-type Si junctions have led to achieving cells efficiency by up to 12%. Later, many approaches to improve the performance of these hybrid solar cells were discovered including nanostructural technique , passivation layer at the interface between PEDOT:PSS/n-type Si, and additional charge selective layer configuration . Interestingly, the PEDOT:PSS material as the p-type layer in this type of cell arrangement surely has an important impact in the junction section, and the study of this organic is substantial to be conducted. Specifically, this polymer in its commercial product has a low applicable electrical conductivity around 0.2–10 S cm−1. This value, of course, becomes a problem when applied it to hybrid solar cells that require a preferable high electrical conductivity. Many studies on the improvement of electrical conductivity in PEDOT:PSS have been widely carried out, such as applying physical
Engineering of Conductive Polymer
treatments by heat or light and chemical treatment including cosolvents, surfactants, acids, and ionic liquids, known to increase its conductivity up to 103 orders for many applications. Furthermore, these chemical utilizations conducted by different combinations of pretreatment, direct addition, and post-treatment may benefit the desired applications based on treated PEDOT:PSS. Specifically, the underlying mechanism regarding the conductivity improvement correlates with the structural and morphological changes. However, in some cases of the post-treatment, the process may influence the thin-film uniformity or even damage the prepared thin film . For these reasons, an easy-and-efficient approach to overcome some of these issues needs to be studied. The use of cosolvents and surfactants is certainly an interesting consideration because it offers simplicity and reliability in the fabrication process. Of the various uses of chemicals, the addition of cosolvents using ethylene glycol (EG) is known to increase the conductivity of PEDOT:PSS to around 620 S cm−1 . In contrast, the addition of surfactants such as fluorosurfactant provides superior wetting properties of the PEDOT:PSS solution, which enables the facile deposition on a variety of hydrophobic substrates . By combining both organic solutions and additional annealing processes, the improvement of both conductivity and uniformity in PEDOT:PSS thin film can actually benefit the deposition of functional PEDOT:PSS on the nanostructured n-type Si. For example, the application of emerging PEDOT:PSS/planar Si for the cell design has been carried out and proven to improve the photovoltaic performance [7,8]. However, the research for combining PEDOT:PSS thin film with nanowires (SiNWs) is still limited. In fact, the SiNWs have various advantages, and one of the well-known applications in solar cells is being able to provide a lighttrapping effect so as to enable the optimization of incoming light transmitted from the transparent PEDOT:PSS layer . Therefore, PEDOT:PSS/SiNW has been considered an efficient way for the construction of high-performance hybrid solar cells.
13.2 PEDOT:PSS WITH TUNABLE ELECTRICAL CONDUCTIVITY 13.2.1
PEDOT:PSS FABRICATED BY “BAYTRON P” ROUTES
PEDOT chains were generally synthesized by the polymerization process of its monomer known as EDOT (3,4-ethylenedioxythiophene) or its derivatives through electrochemical oxidation, transition metal-mediated coupling, or oxidative chemical process. The electrochemical oxidation process of EDOT derivatives is one of the advantageous methods since it needs a short synthetic period, small amounts of EDOT monomer, and can generate free-standing thin films. Several electrolytes, such as polyelectrolytes, or aqueous micellar can be utilized for the electrochemical process. Moreover, the polymerization of substituted EDOTs (alkyl sulfonate, alkylated, etc.) can also be processed by electrochemical routes, and further modification of this process is called electrochemical desilylation [10,11]. Another method termed “transition metal-catalyzed coupling” was utilized to fabricate neutral PEDOT based on the direct formation. The oxidative chemical polymerization has mostly applied in synthesizing PEDOT. The chemical polymerization of EDOT derivatives can be processed using various oxidants. Generally, the oxidizing agents are Fe(OTs)3 or FeCl3, which results in the insoluble and infusible compounds in a film type with black color.
Lithium-Ion Batteries and Solar Cells
Furthermore, the polymerization process of alkoxylated or alkylated EDOT derivatives (the R ≥ C10H21) produced the random-soluble PEDOT derivatives in various organic solvents including THF, CH2Cl2, and CHCl3. Aforementioned, using several fabrication processes above, PEDOT intrinsically not only has insoluble properties but also possesses several sound properties including high conductivity with value around 100 S cm−1, stable in the oxidized state, and relatively high transparency compared with other organic conductors. Since the insolubility of PEDOT becoming a critical issue for the fabrication process, the uncomplicated oxidation chemical routes of Baytron P (P stands for polymer) process were discovered by Bayer AG and further broadened numerous researches related to this conductive polymer . Baytron P synthesis process is known as the most fundamentally convenient PEDOT-based compound fabrication procedure by polymerization method of EDOT in the water-soluble polyelectrolyte solution (generally using template polymers such as polystyrene sulfonic acid or PSSa) by utilizing sodium persulfate (also known as sodium peroxodisulfate – Na2S2O8) as the oxidizing agent. The polymerization can produce aqueous PEDOT/PSS dispersion with dark-blue color and soluble in the water allowing facile practicable conductive polymer. The reaction of Baytron P process is briefly shown in Figure 13.1. It exhibits several interesting properties such as insoluble in many common solvents, transparent, and sound mechanical durability. However, the PEDOT:PSS complex usually possesses reduced conductivity around 10 S cm−1, which is becoming a critical issue for particular applications.
13.2.2 PSS FUNCTIONS IN COMMERCIAL PEDOT:PSS COMPLEX Pristine PEDOT possesses an electronic bandgap in the range of 1.6–1.7 eV owing to the onset π–π* absorption and has the maximum absorption located at 2.0 eV. The maximum absorption wavelength is 610 nm that results in a darkblue color . However, this pristine polymer owns a lower redox potential that
FIGURE 13.1 Baytron P synthesis routes applying sodium peroxodisulfate as the oxidizing agent.
Engineering of Conductive Polymer
intended to be oxidized in air and hard to be processed. The aforementioned Bayer P polymerization routes are offering the stable complex PEDOT:PSS in the aqueous dispersion to clear this issue up. In PEDOT:PSS-based aqueous solutions, PSS brings two functions: the first function is to assist the PEDOT components being dispersed in the aqueous medium, such as water, yields the dark-blue microdispersion, which is facile to process and can be stably utilized. It is certainly beneficial in applications for various ease solutions-based process as the example is thin-film fabrication utilizing simple spin coating, drop casting, or advance process needed. In contrast, by applying Baytron P polymerization procedures, the product of PEDOT chains is known as a positively doped conjugated polymer (PEDOT+). The positive charge or the radical cation was gained through the oxidation process of EDOT monomers. The term p-doping in conducting polymers studies can be described as the process that involves the oxidation treatment of the polymer backbone, and immediately the electronic structure is modified . By this finding, the second function of PSS component is as the anion or charge balancing dopant of cation (PEDOT+). Since PSS is an anionic polyelectrolyte, it results in high stability complex with PEDOT owing to the fact that this ionic set cannot be separated by capillary electrophoresis . These two important functions of PSS attribute to many aspects of PEDOT:PSS behaviors. Specifically, it affects the structural morphology and the electrical conductivity of PEDOT:PSS complex.
13.2.3 PSS INVESTIGATIONS OF ELECTRICAL CONDUCTIVITY IN PEDOT:PSS Although the Baytron P process can achieve facile processing of PEDOT:PSS aqueous solution, the decreasing value of its conductivity becomes the main issue for practical applications. Several reasons are being outlined generally caused by the influence of PEDOT structure and distribution, as well as the PSS existence in the complex. As mentioned earlier, the PEDOT segments as the metallic part inside the complex play an important role in PEDOT:PSS conductivity. As the polythiophene derivative, it consists of main thiophene rings that bring the charges from the conjugated electrons. In the PEDOT:PSS complex, the p-type PEDOT is interpreted as the initial electronic state as the yield of oxidation processes in the polymerization process. As discussed before, the PEDOT segment has its own intermediate electronic structure between quinoid and benzoid that assumed to allow the conjugated arrangement in PEDOT and providing the different distribution of charge carriers on the polymer chains . The benzoid structure is known to give a coiled structure, and the quinoid structure is assumed to promote extendcoiled or linear conformation. The coiled structure of PEDOT in PEDOT:PSS is deliberated to lower the conductivity of the complex because of incompletely distribution of π-electrons over the whole PEDOT chains . In contrast, the prior explanation in PSS structural-morphological investigation is notably that PSS has not only two main functions on the stability of PEDOT:PSS complex but also significantly influences the structural behavior of PEDOT:PSS solution. Therefore, the structural-morphological behavior of conjugated polymer claimed correlates to electrical conductivity properties of PEDOT:PSS.
Lithium-Ion Batteries and Solar Cells
General treatment of pristine PEDOT:PSS can be divided into three procedures, namely pretreatment such as the engineering on polymerization process by chemical oxidation; direct treatment, for example, is the mixing process with various chemical additives; and post-treatment route after the formation of dried-solid PEDOT:PSS. Moreover, in many studies, the combination of these procedures surely exhibits higher and better conductivity values. Interestingly, in several investigations, some grades of PEDOT:PSS mentioned above can produce different final conductivities after the same treatment using certain additives, for example, the study of conductivity improvement of Clevios P and PH1000 with a close initial conductivity in the range of 0.2–0.35 S cm−1. Hydrofluoroacetone trihydrate (HFA) treatments applied in both grades revealed significant difference in final conductivity by the value of 171 S cm−1 for Clevios P and 1164 S cm−1 for Clevios PH1000 . This finding deduced the improvement is because of a longer PEDOT chain arrangement of Clevios PH1000 compared to Clevios P. However, in some studies, other grades of commercial PEDOT:PSS obviously are still be used for preferred applications. The physical source and chemical additive treatments are used to tune the conductivity of pristine PEDOT:PSS. Physical treatments, such as employment of UV irradiation, can manipulate the work function and tune conductivity by reducing the number of charge-trapping defects followed by the conformational change to linear or expanded coil arrangement of PEDOT segments . Moreover, heat-treatment methods can elevate the electrical conductivity due to the change of oxidation state of PEDOT:PSS films . In contrast, chemical treatments, such as polar solvents, surfactants, ionic liquids, and acids, promise a simple and inexpensive treatment that can improve the conductivity value to 103 orders of magnitude higher than the pristine sample . Dimethylsulfoxide (DMSO) and ethylene glycol (EG) are normally used through the direct mixing or the post-treatment procedure that can achieve superior values more than 500 S cm−1. Furthermore, by addition, the mixing treatment using surfactants such as fluorosurfactant or triton-X100 into mixed DMSO/ EG-PEDOT:PSS can offer excellent conductivity performance with the sound film uniformity. The summary of both polar solvents and several other additive treatments in diverse studies is collected in Table 13.1. The utilization of DMSO and EG in diverse routes and the combination can clearly enhance the electrical conductivity of pristine PEDOT:PSS films and applied for many emerging applications such as organic solar cells, thermoelectric devices, and hybrid solar cells in recent years. The enhancement of conductivity value caused by these additives is demonstrated with regard to PEDOT segment’s structural changes from coiled to more linear conformation, removal of excess PSS, and hopping actions among metallic particles identified by Raman spectroscopy, XPS-ESCA, and AFM instruments. Moreover, the current studies claimed that sulfuric acid (H2SO4) can enhance the PEDOT:PSS conductivity achieving around 4300 S cm−1 through posttreatment routes . However, the direct mixing procedures using this acid can lead to the agglomeration of PEDOT:PSS and thus hinder the facile fabrication capability of PEDOT:PSS solution due to dehydrating reaction. Moreover, not all post-treatment processes by chemicals can be applied in PEDOT:PSS-based device fabrication routes because for some cases such as post-treatment using alcohol that degrades the stability of thin film deposited on substrates .
640 (EG); 805 (PEG) 1185 1418
EG, PEG DMSO EG
639 (EG); 620 (DMSO)
Direct addition (mixing) + post treatment (immerse in EG bath) Direct addition (mixing) Post-treatment (drop method) Direct addition + post-treatment (immerse method)
Rs = 1.3 × 106 Ω sq−1 (Clevios PH1000) 0.3 (Clevios PH1000)
0.3 (Clevios PH1000) 0.7 (Clevios PH1000) 0.1–10 (Clevios PH1000)
650 (DMSO-TX); 826 (DMSO-TX-IPA); 908 (DMSO-TX-ethanol); 1105 (DMSO-TX-methanol) Rs = 190 Ω sq−1
Final Conductivity (S cm−1)
Direct addition (DMSO and TX mixing) + posttreatment (dropped alcohols) Direct addition (mixing)
DMSO, Triton X-100, alcohols
0.3 (Clevios PH1000)
Initial Conductivity (S cm−1)
Organic solar cells Liquid crystal display Organic solar cells
Planar silicon/organic hybrid solar cells Thermoelectric
Planar silicon/organic hybrid solar cells
  
TABLE 13.1 Several DMSO and EG Treatments for Commercial Pristine PEDOT:PSS with Regard to Tune Electrical Conductivity in Several Emerging Devices Applications
Engineering of Conductive Polymer 239
Lithium-Ion Batteries and Solar Cells
In a brief description, the following discussion is several points of view regarding the mechanism how the conductivity of pristine PEDOT:PSS can be improved. The first mechanism is proposed by the identification using X-ray photoelectron spectroscopy (XPS) by the mixing of DEG into PEDOT:PSS complex. These findings confirmed that the removal of PSS from PEDOT:PSS complex noticeable by XPS spectra recognition and area calculation of pointed out peaks presenting the sulfur elements in the energy range of 160–170 eV. The sulfur peaks used on the identification are the S2p bands located at 163–167 eV later confirmed as the doublet peaks of sulfur atoms in PEDOT. The intensities of PEDOT peaks identified with respect to S2p bands from PSS constituent showed to increase by the addition of DEG later suggested as the removal of partially PSS in the film . Another study also confirmed the excess PSS washing on the film surface during the additive post-treatment applying post-spin-rinsing method (PSRM) using the DMSO solvent . A further approach based on the identification of PEDOT chain conformational changes before and after EG treatment was obtained by Raman spectroscopy. As-prepared PEDOT:PSS was proclaimed consisting of intermediate structures, there are benzoid and quinoid structures in its PEDOT segments as aforecited above. The resonant structure of benzoid, which is confirming the coiled structure, will change to the quinoid arrangement as the linear or expanded coiled structure results in the conductivity enhancement mechanism. The changes of this conformational arrangement can be observed by the changes of molecules and chemical structural alteration validated by peak shifting of the spectra. The same study also revealed that the conformational change corresponds to the delocalization process of polaron to bipolaron charges over several units in PEDOT chains recognized by the electron spin resonance (ESR). A polaron is conformed as a positive charge on a unit, and a bipolaron is two positive charges delocalized over several units later; both mechanisms are known to enhance the conductivity of pristine PEDOT:PSS . Other assumptions are correlated to phase separation and screening effect constructed after the addition of additives. The phase separation is attributed to the phase separation of PEDOT and PSS by the formation of hydrogen bonding among cosolvents and both PSS and PSSH, resulting in the linearly oriented PEDOT chains . Another study revealed the screening effect occurred due to dielectric properties of solvents that reduce the Coulomb interaction between PEDOT and PSS constituents. Further study in polar solvents including EG and DMSO addition based on THz-TDS measurements confirms the charge screening responsible for the increase of conductivity [27,29]. The conductivity enhancement by hopping, doping effects, and morphological changes was proposed by other investigators. The resistance (R)– temperature (T) relationship of conducting polymers at T < 220 K was particularly analyzed by one-dimensional variable range hopping (VRH) model .
TREATED PEDOT:PSS FOR SILICON NANOWIRESBASED HYBRID SOLAR CELLS
This study was conducted for functioning PEDOT:PSS as the hole transport layer as well as p-type component in hybrid solar cells. A simple route utilizing ethylene glycol (EG-99%) as solvent has been proposed in enhancing the conductivity of pristine
Engineering of Conductive Polymer
PEDOT:PSS thin film. EG was chosen for cosolvent and secondary doping agent since this solvent has two polar groups and superior dielectric constant leading to the phase separation of PEDOT:PSS constituents and further results in the better conductivity. The incorporation of EG studied in different weight percents (wt%) from 1 to 11 wt% with PEDOT:PSS was performed. Moreover, to obtain preferable thinfilm uniformity on the substrate, the surfactant as the wettability improver is needed. Fluorosurfactant zonyl (FS) is not only claimed to provide better adhesive of thin film but also can reduce the sheet resistance providing additional conductivity enhancement of PEDOT:PSS in the film shape . The fabrication route of thin films is proposed by detail in Figure 13.2. The pretreatment of pristine PEDOT:PSS solution was conducted by the filtering process. And then, EG cosolvent was added into the filtered PEDOT:PSS in several amounts from 3, 7, and 11 wt%, and the samples are named as EG3, EG7, and EG11, respectively. As the reference, pristine PEDOT:PSS was used and noted as EG0. Moreover, the small amount of FS incorporated into the PEDOT:PSS/EG followed by the mixing process under atmosphere for several hours. Thin-film fabrication was utilized by applying spin-coating methods on the substrates. Later, the drying process was performed at 140°C for several minutes in creating solidified dispersion. Electrical properties of the treated PEDOT:PSS/EG thin films were evaluated by two approaches using four-point probe (FPP) and Halleffect analyzer for examining the charge carrier concentrations and mobility. The film thickness was estimated by ellipsometry, and its morphology was observed by scanning electron microscopy (SEM). Figure 13.3 presents the transmittance spectra, SEM observation, and thin-filmcoated results of the pristine and treated samples on the glass substrates, respectively. The spectra of the bare glass substrate indicate a quite high transmittance up to 95% and stable in the whole wavelength. Furthermore, the samples from 0 to 11 wt% EG
Thin-film fabrication routes by incorporation of EG and FS.
Lithium-Ion Batteries and Solar Cells
FIGURE 13.3 Optical properties of PEDOT:PSS thin films. The topsides consist of the transmittance percentage of thin films on the glass substrates (a) and the cross-sectional scanning electron microscopy (SEM) figures of EG7 uniform film (b). The bottom side is the figure of fabricated thin films by different wt% EG incorporation.
addition are observed to provide the optical transmittance more than 90% in the whole applied wavelengths. The 300–800 nm wavelength average for each sample is found to be 90.72%, 91.77%, 92.15%, and 91.44% for EG0, EG3, EG7, and EG11, respectively. In detail, it can be noted the pristine PEDOT:PSS has lower average value in comparison with the treated films. Moreover, the thickness confirmation with ellipsometry showed the values of 150.34, 142.93, 129.11, and 137.65 nm, for EG0 to EG11, respectively. Both analyses are confirmed the macro-observation of thin film showed at the bottom side of Figure 13.3. It seems the EG0 (pristine) possesses the light dark-blue color with a darker part at the corner of film in comparison with the treated PEDOT:PSS. The results indicate that all the EG treated samples turn to be more transparent than the pristine one. However, by adding 11 wt% of EG results in the threshold of excess EG where the thickness is significantly increased and thus reduces the transmittance of films. Further electrical analysis confirms the high-elevated improvement values after EG treatment by utilizing two approaches employing surface-sheet resistivity and charge concentration/mobility approaches. Furthermore, Figure 13.4a evidences that the conductivity values of treated PEDOT:PSS are significantly improved. The FPP and Hall-effect approaches bring out supports for each other. The sheet resistance were found to be 160.29 × 103, 91.57, 87.52, and 103.75 Ω sq−1 for EG0, EG3, EG7, and EG11, respectively. Further investigation of Hall-effect analysis clearly described the secondary doping mechanism of EG in PEDOT:PSS. The measurement of pristine PEDOT:PSS shows the high mobility (7.7912 cm2 V−1 s−1) with the low carrier concentration (5.53 × 1017 cm−3) that results in poor conductivity with the value of 0.69 S cm−1. Furthermore, by addition of 3 and
Engineering of Conductive Polymer
FIGURE 13.4 Analysis for the conductivity enhancement by the incorporation of EG including (a) conductivity by four-point probe and Hall-effect approaches, (b) Raman spectroscopy in identifying the structural change in PEDOT chains, and (c) ESCA-XPS analysis for PEDOT:PSS ratio identification.
7 wt%, the mobility experienced to decrease with 0.60251 and 0.061306 cm2 V−1 s−1 that is followed by increasing in charge carrier density to 7.72 × 1021 cm−3 and 9.56 × 1022 cm−3, respectively. Further addition of EG to 11 wt% is found to increase the mobility to 0.32 cm2 V−1 s−1 and decrease the carrier concentration to 1.51 × 1022 cm−3. This results in the film conductivity to 743.75, 938.22, and 770.79 S cm−1 by mixing 3, 7, and 11 wt% of EG, respectively, as shown in Table 13.2.
TABLE 13.2 Several Parameters from Hall-Effect Measurement and the Conductivity Values Sample EG0 (pristine) EG3 EG7 EG11
Mobility (cm2V−1·s−1) 7.79 0.60 0.061 0.32
Bulk Carrier Concentration (cm−3) 5.53 × 1017 7.72 × 1021 9.56 × 1022 1.51 × 1022
Conductivity (S cm−1) 0.6898 743.75 938.22 770.79
Lithium-Ion Batteries and Solar Cells
Further investigation of conductivity improvement in PEDOT:PSS is traced by Raman spectroscopy analysis, which is a useful assessment to observe structural change of conducting polymers chains specifically at the molecular level. The study conducted using 632.8 nm excitation laser with wavenumbers range of 900–1630 cm−1. Figure 13.4b provides the Raman spectra by the comparison of sample including EG0 (pristine), EG3, EG7, and EG11. The intense and sharp particular peaks of PEDOT chains were observed at 987, 1126, 1255, 1363, 1427, 1533, and 1565 cm−1, which are in accordance with previous reports [8,28,31,32]. The peaks centered at 987 and 1126 cm−1 are the oxyethylene ring deformation and C–O–C deformation vibrational modes, respectively. Moreover, peaks at 1255 and 1363 cm−1 are attributed to the Cα=C′α (inter-ring) stretching and Cβ=Cβ stretching, respectively. The notable peak of symmetric Cα=Cβ stretching is the mode at 1427 cm−1, and a pair peaks at 1533 and 1565 cm−1 can be assigned to be the asymmetric Cα=Cβ stretching modes. In the figure, the intensity of EG11 is decreased compared with all other spectra, which is due to the high concentration of excess EG in PEDOT:PSS film. The shifting of symmetric Cα=Cβ stretching modes toward lower wavenumbers is found in comparison with that of the pristine sample, as shown in the inserted figure of Figure 13.4b. It suggests that by mixing EG from 3, 7, and 11 wt%, it attributes to the changes of PEDOT chains from benzoid to quinoid resonant structures. The benzoid resonant structure is suggested to be the favored structure for the coiled conformation; in contrast, the quinoid is the favored structure for linear or expanded-coil conformation of PEDOT chains. In pristine PEDOT:PSS film, both conformations were indicated to exist, and after EG treatment, the benzoid structures are expected to transform to quinoid states. Furthermore, the quinoid arrangement leads the extended coil or linear conformation, which can generate a lower energy barrier for interchain interaction and further result in decreasing the inter-domain charge hopping region . Further analysis to figure out the possible effect of EG incorporation in PEDOT:PSS regarding the conductivity enhancement is by thin-film surface investigation utilizing ESCA-XPS instrument. Figure 13.4c is representing the ESCA spectra of sulfur signals and at the estimated PEDOT to PSS ratio. By the results of curve fitting, the spectra confirmed four main peaks of S(2p) consisting of S(2p3/2) and S(2p1/2) representing the sulfur atoms from PEDOT and PSS. The PEDOT indication peaks are at the low energy at 164 eV for S(2p3/2) and 165 eV for S(2p1/2) . In contrast, the PSS peaks recognized at 168 eV for S(2p3/2) and 169 eV for S(2p1/2) that is detected at the higher binding energy spectra as the influence of the electronegative oxygen connection in the sulfonate moiety. Based on the spectra observation, the shifting of spectra in EG addition samples is noticed in comparison with the EG0 sample. The shifting value is estimated at around 0.3 eV and corresponding to the chemical shift at the surface of the thin films as the consequences of the chemical environment changes promoted by the addition of EG in different concentrations that are correlated with aforementioned discussions from Raman analysis. Advanced investigation of PEDOT:PSS/EG thin films indicates the PEDOT to PSS ratio by calculating the relative areas of PEDOT and PSS peaks. Figure 13.4c at the right side shows the ratio at surfaces indicate that the ratio is slightly increased by adding 3 wt% of EG with the value of 0.36 and then reaches 0.44 by adding 7 wt% of EG. Subsequently, the more addition of EG reduces the PEDOT:PSS ratio to 0.42. From both observations,
Engineering of Conductive Polymer
the addition of EG increases the existence of PEDOT:PSS chains at the surface of the deposited film. The EG solvent is believed to remove the excess PSS and thus modifies the PEDOT:PSS ratio . The proposed mechanism representing the influence of 3–7 wt% EG addition is demonstrated as shown in Figure 13.5. In the pristine condition, the PEDOT:PSS arrangement is mostly attributed to coulombic interactions that result in coiled structures. Moreover, through EG cosolvent addition, the conductivity improvement is found because of structural change in PEDOT chains followed by the phase separation between the PEDOT and PSS chains. The driving force regarding these conformational changes is caused by the polar groups of cosolvents that interact with the PEDOT segment. Since the EG has two or more polar groups, the interaction between the polar groups (–OH) and positive charges on PEDOT chains is occurred. Moreover, the size of PEDOT nanocrystals is increased because of more linear arrangement in the nanocrystals. This linear orientation of PEDOT chains allows the interaction of PEDOT interchains that can lower the energy barrier for charge hopping and in turn facilitates the charge transfer. The p–n heterojunction is formed by combining the treated p-type PEDOT:PSS and n-type Si nanowires (SiNWs). The arrangement of fabricated cells is shown in Figure 13.6a consisting of treated PEDOT:PSS/EG as the p-junction layer, n-type SiNWs as the n-junction layer, aluminum as the bottom electrode, and ITO as the top electrode. The 2 × 2 cm2 cells were measured using the solar simulator, and J–V assessment is presented in Figure 13.6b. The solar cells were made by using different contents of EG from 3 to 11 wt% since this range of the samples possesses the improved electrical conductivity compared with untreated PEDOT:PSS. The involved working mechanism is presented in Figure 13.6c. Since the PEDOT:PSS/EG represents a high transparent hole-transport layer, the solar light is mostly transmitted into the SiNW regions, where the significant light absorption is
FIGURE 13.5 The mechanism of conductivity enhancement influenced by EG cosolvent addition thin films.
Lithium-Ion Batteries and Solar Cells
FIGURE 13.6 (a) Silicon nanowires-based hybrid solar cell arrangement, (b) J–V curve of the cells for different wt% of EG addition, and (c) the working mechanism of hybrid solar cells.
encountered due to the light-trapping effect from the oriented nanowires. It causes the generation of photoexcited carriers, and the holes are transported toward p-type electrodes and collected by the top electrode; in contrast, the electrons are separated from the heterojunction and eventually collected by the aluminum electrode. Since the PEDOT:PSS/EG7 layer possesses the superior light transmittance, which benefits the generation of more photoexcited carriers, while the underlying SiNWs can efficiently absorb the visible light. The theoretical study to unveil the light-absor ption capability of bare SiNWs and perovskite-coated SiNWs was reported, which indicated that the SiNWs possess the significant absorptance of lights covering the wavelengths from 400 to 800 nm . Such preferred structures therefore yield the improved PCE up to 14.12% by well construction of large-area heterojunction and sound light management, as shown in Figure 13.6b.
In conclusion, the synthesis, structure, and electrical properties of PEDOT:PSS layer were studied. The electrical conductivity of pristine PEDOT:PSS is found to be rather low, which is merely under 10 S cm−1. However, it can be adjusted into higher values using diverse methods including physical treatment or chemical process. The enhancement of electrical conductivity can be up to 103 orders of magnitude by utilizing polar solvents, EG and DMSO mostly. The underlying mechanism for conductivity
Engineering of Conductive Polymer
improvement has been studied using XPS, Raman spectroscopy, AFM, Hall-effect, GIWAXS, and many more. Furthermore, the clarification of optimization in treated PEDOT:PSS polymer for constructing hybrid solar cells was achieved by adding 7 wt% of EG and 0.1 wt% of FS additives. The optical transmittance can be achieved more than 90% by testing the addition of various amounts of EG and has an advantage in optimizing the cell performance. The conductivity of thin film can be achieved up to 938 S cm−1 with high uniformity without employing post-treatment after thinfilm fabrication. The Raman analysis and XPS results give more clear evidence about the conductivity enhancement that is attributed to the structural conformation. Also, the reduction of excess PSS chains at the surface is encountered, which can therefore increase the PEDOT/PSS ratio, initiate the phase separation of PEDOT and PSS chains inside the thin film, and positively influence the carrier doping level in the forms of polarons and bipolarons. Based on the optimized design of treated PEDOT:PSS films, the conversion efficiency of hybrid solar cells can reach 14.12% through such facile, inexpensive, and reliable treatment. This can pave ways particularly for energy-based devices such as emerging solar cells, thermoelectric, and electrochromic applications.
ACKNOWLEDGMENT This study was financially supported by the Ministry of Science and Technology of Taiwan (MOST 106-2221-E-006-240) and (MOST 107-2221-E-006-013-MY3), and the Hierarchical Green-Energy Materials (Hi-GEM) Research Center, from the Featured Areas Research Center Program within the framework of the Higher Education Sprout Project by the Ministry of Education (MOE) and the Ministry of Science and Technology (MOST 107-3017-F-006-003) in Taiwan. The authors greatly thank Center for Micro/Nano Science and Technology, National Cheng Kung University with the facilities provided for conducting material characterizations.
REFERENCES 1. Joint Research Centre. European Comission, “PV Status Report 2018,” 2018. 2. W. Lu, C. Wang, W. Yue, and L. Chen, “Si/PEDOT:PSS core/shell nanowire arrays for efficient hybrid solar cells,” Nanoscale, vol. 3, no. 9, pp. 3631–3634, 2011. 3. C.-Y. Chen, T.-C. Wei, P.-H. Hsiao, and C.-H. Hung, “Vanadium oxide as transparent carrier-selective layer in silicon hybrid solar cells promoting photovoltaic performances,” ACS Appl. Energy Mater., 2019. doi: 10.1021/acsaem.9b00565. 4. D. Alemu, H.-Y. Wei, K.-C. Ho, and C.-W. Chu, “Highly conductive PEDOT:PSS electrode by simple film treatment with methanol for ITO-free polymer solar cells,” Energy Environ. Sci., vol. 5, no. 11, p. 9662, 2012. 5. W. Wichiansee and A. Sirivat, “Electrorheological properties of poly(dimethylsiloxane) and poly(3,4-ethylenedioxy thiophene)/poly(stylene sulfonic acid)/ethylene glycol blends,” Mater. Sci. Eng. C, vol. 29, pp. 78–84, 2008. 6. M. Vosgueritchian, D. J. Lipomi, and Z. Bao, “Highly conductive and transparent PEDOT:PSS films with a fluorosurfactant for stretchable and flexible transparent electrodes,” Adv. Funct. Mater., vol. 22, no. 2, pp. 421–428, 2012. 7. Q. Li, J. Yang, S. Chen, J. Zou, W. Xie, and X. Zeng, “Highly conductive PEDOT:PSS transparent hole transporting layer with solvent treatment for high performance silicon/ organic hybrid solar cells,” Nanoscale Res. Lett., vol. 12, pp. 1–8, 2017.
Lithium-Ion Batteries and Solar Cells
8. J. P. Thomas, L. Zhao, D. McGillivray, and K. T. Leung, “High-efficiency hybrid solar cells by nanostructural modification in PEDOT:PSS with co-solvent addition,” J. Mater. Chem. A, vol. 2, no. 7, p. 2383, 2014. 9. C.-Y. Chen and C.-P. Wong, “Unveiling the shape-diversified silicon nanowires made by HF/HNO 3 isotropic etching with the assistance of silver,” Nanoscale, vol. 7, no. 3, pp. 1216–1223, 2015. 10. M. Łapkowski and A. Proń, “Electrochemical oxidation of poly(3,4-ethylenedioxythiophene) – ‘in situ’ conductivity and spectroscopic investigations,” Synth. Met., vol. 110, pp. 79–83, 2000. 11. G. Steiner and C. Zimmerer, “Poly(3,4-ethylenedioxythiophene) (PEDOT).” 2013. doi: 10.1007/978-3-642-32072-9_128. 12. L. Groenendaal, F. Jonas, D. Freitag, H. Pielartzik, and J. R. Reynolds, “Poly(3,4ethylenedioxythiophene) and its derivatives: past, present, and future,” Adv. Mater., vol. 12, no. 7, pp. 481–494, 2000. 13. H. J. Ahonen, J. Lukkari, and J. Kankare, “N- and p-doped poly(3,4-ethylenedioxythiophene): two electronically conducting states of the polymer,” Macromolecules, vol. 33, no. 18, pp. 6787–6793, 2000. 14. S. Ghosh and O. Inganäs, “Self-assembly of a conducting polymer nanostructure by physical crosslinking: applications to conducting blends and modified electrodes,” Synth. Met., vol. 101, no. 1, pp. 413–416, 1999. 15. S. Garreau, G. Louarn, J. P. Buisson, G. Froyer, and S. Lefrant, “In situ spectroelectrochemical Raman studies of poly(3,4-ethylenedioxythiophene) (PEDT),” Macromolecules, vol. 32, no. 20, pp. 6807–6812, 1999. 16. J. Ouyang, C. W. Chu, F. C. Chen, Q. Xu, and Y. Yang, “High-conductivity poly(3,4-eth ylenedioxythiophene):poly(styrene sulfonate) film and its application in polymer optoelectronic devices,” Adv. Funct. Mater., vol. 15, no. 2, pp. 203–208, 2005. 17. Y. Xia and J. Ouyang, “Significant different conductivities of the two grades of poly(3,4ethylenedioxythiophene):poly(styrenesulfonate), Clevios P and clevios PH1000, arising from different molecular weights,” ACS Appl. Mater. Interfaces, vol. 4, no. 8, pp. 4131– 4140, 2012. 18. A. Moujoud, S. H. Oh, H. S. Shin, and H. J. Kim, “On the mechanism of conductivity enhancement and work function control in PEDOT:PSS film through UV-light treatment,” Phys. Status Solidi Appl. Mater. Sci., vol. 207, no. 7, pp. 1704–1707, 2010. 19. Y. Kim, A. M. Ballantyne, J. Nelson, and D. D. C. Bradley, “Effects of thickness and thermal annealing of the PEDOT:PSS layer on the performance of polymer solar cells,” Org. Electron. Phys. Mater. Appl., vol. 10, no. 1, pp. 205–209, 2009. 20. K. Sun, S. Zhang, P. Li, Y. Xia, X. Zhang, D. Du, F. H. Isikgor, and J. Ouyang, “Review on application of PEDOTs and PEDOT: PSS in energy conversion and storage devices,” J. Mater. Sci.: Mater. Electron., vol. 26, no. 7, pp. 4438–4462, 2015. 21. G. H. Kim, L. Shao, K. Zhang, and K. P. Pipe, “Engineered doping of organic semiconductors for enhanced thermoelectric efficiency,” Nat. Mater., vol. 12, no. 8, pp. 719–723, 2013. 22. D. Alemu Mengistie, P. C. Wang, and C. W. Chu, “Effect of molecular weight of additives on the conductivity of PEDOT:PSS and efficiency for ITO-free organic solar cells,” J. Mater. Chem. A, vol. 1, no. 34, pp. 9907–9915, 2013. 23. T. R. Chou, S. H. Chen, Y. Te Chiang, Y. T. Lin, and C. Y. Chao, “Highly conductive PEDOT:PSS films by post-treatment with dimethyl sulfoxide for ITO-free liquid crystal display,” J. Mater. Chem. C, vol. 3, no. 15, pp. 3760–3766, 2015. 24. Y. H. Kim, C. Sachse, M. L. MacHala, C. May, L. Müller-Meskamp, and K. Leo, “Highly conductive PEDOT:PSS electrode with optimized solvent and thermal posttreatment for ITO-free organic solar cells,” Adv. Funct. Mater., vol. 21, no. 6, pp. 1076– 1081, 2011.
Engineering of Conductive Polymer
25. N. Kim, S. Kee, S. H. Lee, B. H. Lee, Y. H. Kahng, Y. R. Jo, B. J. Kim, and K. Lee, “Highly conductive PEDOT:PSS nanofibrils induced by solution-processed crystallization,” Adv. Mater., vol. 26, no. 14, pp. 2268–2272, 2014. 26. X. Crispin, S. Marciniak, W. Osikowicz, G. Zotti, A. D. Van Der Gon, F. Louwet, M. Fahlman, L. Groenendaal, F. De Schryver, and W. R. Salaneck, “Stability of poly (3,4-ethylene dioxythiophene)-poly(styrene sulfonate): a photoelectron spectroscopy study,” Polymer (Guildf)., vol. 41, no. 21, pp. 2561–2583, 2003. 27. X. Zhang, J. Wu, J. Wang, J. Zhang, Q. Yang, Y. Fu, and Z. Xie, “Highly conductive PEDOT:PSS transparent electrode prepared by a post-spin-rinsing method for efficient ITO-free polymer solar cells,” Sol. Energy Mater. Sol. Cells, vol. 144, pp. 143–149, 2016. 28. J. Ouyang, Q. Xu, C. W. Chu, Y. Yang, G. Li, and J. Shinar, “On the mechanism of conductivity enhancement in poly(3,4-ethylenedioxythiophene):poly(styrene sulfonate) film through solvent treatment,” Polymer (Guildf)., vol. 45, no. 25, pp. 8443–8450, 2004. 29. J. Y. Kim, J. H. Jung, D. E. Lee, and J. Joo, “Enhancement of electrical conductivity of poly(3,4-ethylenedioxythiophene)/poly(4-styrenesulfonate) by a change of solvents,” Synth. Met., vol. 126, nos. 2–3, pp. 311–316, 2002. 30. S. Zhang, Z. Fan, X. Wang, Z. Zhang, and J. Ouyang, “Enhancement of the thermoelectric properties of PEDOT:PSS: via one-step treatment with cosolvents or their solutions of organic salts,” J. Mater. Chem. A, vol. 6, no. 16, pp. 7080–7087, 2018. 31. W. W. Chiu, J. Travaš-Sejdić, R. P. Cooney, and G. A. Bowmaker, “Studies of dopant effects in poly(3,4-ethylenedioxythiophene) using Raman spectroscopy,” J. Raman Spectrosc., vol. 37, no. 12, pp. 1354–1361, 2006. 32. S. Garreau, J. L. Duvail, and G. Louarn, “Spectroelectrochemical studies of poly(3,4ethylenedioxythiophene) in aqueous medium,” Synth. Met., vol. 125, pp. 325–329, 2001. 33. S. Funda, T. Ohki, Q. Liu, J. Hossain, Y. Ishimaru, K. Ueno, and H. Shirai, “Correlation between the fine structure of spin-coated PEDOT:PSS and the photovoltaic performance of organic/crystalline-silicon heterojunction solar cells,” J. Appl. Phys., vol. 120, no. 3, p. 33103, 2016. 34. C. Y. Chen, T. C. Wei, Y. C. Lai, and T. C. Lee, “Passivating silicon-based hybrid solar cells through tuning PbI2 content of perovskite coatings,” Appl. Surf. Sci., vol. 511, p. 145541, 2020.
Concluding Remarks Ngoc Thanh Thuy Tran, Sanjaya Brahma, Wen-Dung Hsu, Shih-Yang Lin, Jow-Lay Huang, Masahiro Yoshimura, Jeng-Shiung Jan, Chia-Yun Chen, Peter Chen, and Ming-Fa Lin National Cheng Kung University
Chin-Lung Kuo National Taiwan University
Phung My Loan Le University of Science, Vietnam National University
CONTENT References .............................................................................................................. 256 In general, this book covers the development of the theoretical frameworks, the highresolution measurements, and the excellent performance of batteries. It can significantly promote the full understanding in basic sciences, application engineerings, and commercial products. However, the close combinations of cathode, electrolyte, and anode materials are required to create the best ion transport in batteries [1–3], become an open issue, and are worthy of the systematic investigations. That is, the critical mechanisms, which determine the stationary currents of ions in three core components, are not thoroughly identified from the up-to-date theoretical and experimental results, such as the non-well-verified roles of charged impurities [4,5], vacancies , grain boundaries , interfaces between distinct systems , significantly modulated bond lengths , electronic spin configurations (ferromagnetism or antiferromagnetism) , Coulomb screening behaviors [11,12], active chemical reactions , controllable temperatures , and quantum Bose–Einstein/Fermi–Dirac boson/fermion statistics temperatures . As to lithium-ion-related batteries, the first-principles method [16–22] and the machine learning method  are efficient in exploring the lattice symmetries , energy bands/discrete electronic states , charge transfers , free carrier densities , energy gaps , spatial charge/spin density distributions , van Hove singularities of energy spectra , formation energies of distinct vacancies , ionization energies . The multi-orbital hybridizations in chemical bonds , atom- and orbital-dependent spin configurations ,
Lithium-Ion Batteries and Solar Cells
and the intrinsic geometric symmetries  are deduced to be responsible for the diversified essential properties. The similar simulations would be further developed for the other emergent green energy materials [27–29]. As to the experimental syntheses, measurements, and designs, they have been successfully done for the Li-ion batteries, silicon-nanowire-based hybrid solar cells, and perovskite solar cells. The core materials in the aforementioned devices, with the save, cheap, light, rapid-ion, and long-lifetime characteristics, are the studying focuses in significantly enhancing the operation performances. This can be achieved through the chemical modifications (absorptions, dopings, and substitutions); the physical methods; the optimal changes among the solid-, liquid-, and gel-state electrolytes; and the delicate treatments of junctions/contacts. More high-resolution experiments would be finished in the near-future researches. As the demand for LIBs is increasing, it is critical to increase its specific energy. Archiving high-voltage LIBs has recently gained much attraction as one way to deal with this issue. Theoretical and experimental studies have been carried out to find out the candidate for high-voltage cathode materials [30–32]. Searching for electrolytes that compatible with a low-voltage anode such as graphite and high-voltage cathode about 4.5–5 V plays an important role. In this work, machine learning based on the generation model has been established for screening electrolyte molecules from key factors-electron affinity and ionization energy values. Introducing machine learning into material science is trying to replace expert-based knowledge with data in the material design; however, it is worth to know that even the advancement of machine learning model cannot achieve excellent performance without the assistance of expert-based knowledge. The proposed method developed in this work can significantly reduce the development time and cost for new materials design. The results from first-principles calculations indicate that introducing N-dopants can increase the amount of defects in graphene, which can provide more energetically favorable sites to bind Li or Na atoms. The migration energy barrier of vacancy defects was found to become higher after doping with N, which can effectively avoid the capacity loss due to the suppression of vacancy aggregation. However, introducing many N-dopants near defect sites may lower down the Li/Na reversible capacity. Our results thus suggest that the concentration of N-doping should be carefully controlled in order to obtain optimal Li/Na storage capacity of graphene-based nanomaterials. The 3D ternary Li4Ti5O12, the Li+-based battery anode, presents the unusual lattice symmetry (a triclinic crystal), band structure, charge density, and density of states under the first-principles calculations. It belongs to a large direct-gap semiconductor of Egd ~ 2.98 eV. The atom-dominated valence and conduction bands, the spatial charge distribution, and the atom- and orbital-decomposed van Hove singularities are available in the delicate identifications of multi-orbital hybridizations in Li–O and Ti–O bonds. The extremely nonuniform chemical environment, which induces the very complicated hopping integrals, directly arises from the large bonding fluctuations and the highly anisotropic configurations. Also, the developed theoretical framework is very useful for fully understanding the cathodes and electrolytes of oxide compounds. The rich and unique fundamental properties of the emergent 3D Li2SiO3 compound are thoroughly investigated from the first-principles calculations. The critical
multi-orbital hybridizations, which survive in Li–O and Si–O bonds, are accurately identified from the atom-dominated band structure, the charge density distributions in the significantly modulated chemical bonds, and the atom- and orbital-projected van Hove singularities. The theoretical framework could be further developed for the other electrolyte, anode, and cathode materials of Li+-based batteries , for example, the important differences among the various LiXO-related compounds, and the diversified phenomena driven by the various components . Interestingly, the highly anisotropic and nonuniform environments need to be included in the phenomenological models . For example, the suitable tight-binding model is expected to have the position-dependent hopping integrals and the orbital-create onsite Coulomb potentials in simulating the VASP energy bands and density of states. Whether the intrinsic atomic interactions of Hamiltonian could be expressed in the analytic form is the near-future studying focus; furthermore, they are very useful in exploring the other diverse phenomena, such as the magnetic quantization in a uniform perpendicular magnetic field . The solid-state anode material of Li2SiO3 with 24 atoms in a primitive unit cell is an orthorhombic structure. There are 32 Li–O and 16 O–Si–O chemical bonds, in which each atom has four neighboring other atoms. Their bond lengths, respectively, present the large modulations over 10% and 6% S. Most importantly, the very strong orbital hybridizations create a very wide indirect gap of Eg ≈ 5.077 eV, being close to the largest one in diamond ≈ 5.5 eV. Its magnitude is even lower than the optical threshold absorption frequency. The high-resolution optical reflection/absorption/transmission spectroscopies are available in detecting the obvious insulating property of the transparent material. The occupied valence and the unoccupied conduction bands are highly asymmetric to each other about the Fermi level. Furthermore, there exist the wide energy range of (−8.0 eV, Ev, 8 eV), the strong/various dispersion relations with the wave vector, the high anisotropy, and the frequently noncrossing/crossing/anticrossing behaviors. Moreover, the van Hove singularities, which arise from the band-edge states, appear as the six/three dominating/minor special structures in density of states of the valence/conduction energy spectrum (E > 0, E < 0). They only belong to the broadening asymmetric/symmetric peaks and shoulders and play a critical role in examining the multi-orbital hybridizations of Li–O and Si–O bonds, 2s-(2s, 2px, 2py, 2pz), and (3s, 3px, 3py, 3pz) – (2s, 2px, 2py, 2pz). The diverse covalent bondings are partially supported by the atom-dominated band structure and charge density distributions in modulated chemical bonds. The theoretical predictions on the optimal geometry, occupied wave-vector-dependent valence bands, and valence and conduction density of states could be verified from X-ray elastic scatterings LEED [35,37] and ARPES, respectively. The calculated results clearly illustrate that LiSiO-based compounds have certain metastable configurations and even an infinite intermediate ones during the charging and discharging processes for the Li+ ion transport in batteries. The similar structural transformations between two metastable structures are expected to occur at any time. The optimal evolution paths, which might become an emergent issue, are under the current investigations. The 3D ternary Li xCo/NiO2 compounds, being the well-known cathode materials of Li+-based batteries, are predicted to exhibit the rich and unique lattice symmetries (a trigonal lattice), band structures, charge/spin density distributions, and van Hove
Lithium-Ion Batteries and Solar Cells
singularities. The accurate analyses, which are made from the exact first-principles calculations, are available in identifying the significant multi-orbital hybridizations/ spin configurations in Li–O and Co/Ni–O bonds. Specifically, the spin-dependent many-particle Coulomb interactions need to be included in the numerical evaluations simultaneously, while they are fully absent in the anode and electrolyte materials (e.g., LiTiO and LiSiO). The essential electronic and magnetic properties are very sensitive to the lithium concentration. All the LixCo/NiO2 systems belong to the ferromagnetic metals except that LiCoO2 is a spin-degenerate semiconductor with the energy gap of ~1.05 eV. Three kinds of ferromagnetic configurations are revealed during the variation of x. There are a lot valence and conduction bands with the range of −8.0 eV < Ec,v < 3.0 eV, in which most of them are dominate by transition and oxygen atoms. The intrinsic interactions mainly come from the chemical bondings and the spin-dependent on-site electron–electron Coulomb ones. The theoretical predictions on the optimal geometries, the rich occupied bands, and many van Hove singularities could be verified from the high-resolution measurements of the X-ray diffraction, angle-resolved photoemission spectroscopy, and scanning tunneling spectroscopy, respectively. The stage-n graphite alkali-intercalation compounds present the rich and unique geometric and electronic properties, being directly identified from the first-principles calculations. The diversified phenomena strongly depend on the type, concentration, and distribution of intercalants. By the delicate calculation and analyses on the optimal geometries, band structures, and densities of states, the π and σ bands could be well defined through the interlayer carbon-alkali bondings/the significant van der Waals, or their chemical bondings are almost orthogonal to each other. Most importantly, the interlayer single-orbital atomic interactions, 2pz -3s and 2pz -2pz, play critical roles in modifying the main features of electronic energy spectra. Interestingly, the dramatic transformation of EF is clearly identified from a prominent peak there and a minimum valley of the left-hand neighbor at about E < −1.0 eV. Apparently, the modified π and σ bonds create the diverse fundamental properties. The theoretical predictions on band structures and van Hove singularities could be verified from the high-resolution ARPES  and STS  measurements, respectively. Graphene nanosheets (GNs) prepared by variety of methods including exfoliation and chemical modification are used extensively as anode (negative electrode) in LIBs due to excellent Li storage capability  and have shown significant potential as energy storage material. GNs could achieve significantly high first charge–discharge capacity (1233 and 672 mAh g−1). The high irreversible capacity is due to the reaction of Li ion with oxygen-containing functional groups and formation of the solid electrolyte interface (SEI). Microstructure modification  is also achieved by the chemical modification, where flower-like GNS could be synthesized and the corresponding anode material has maintained high capacity (460 mAh g−1) after 100 cycles and that shows good electrochemical performance. Introduction of the porosity and the doping has significantly enhanced the electrochemical properties. We recently proposed a novel ionic liquid (i.e., 1-ethyl-3-methylimidazolium bis(trifluoromethanesulfonyl)imide) containing a suitable lithium salt (i.e., lithium bis(trifluoromethanesulfonyl)imide, LiTFSI) as advanced electrolyte for lithium batteries. This IL-based electrolyte offers a good compatibility with the lithium metal
electrode while maintaining high thermal stability and acceptable conductivity. Excellent performances were also shown in terms of interface stability, cycle life, and rate capability when the EMITFSI + LiTFSI solution was tested in lithium cells. We also prepared IL-containing polymer membranes by immobilizing a solution of LiTFSI in EMI-TFSI mixed with other organic solvents, such as ethylene carbonate, propylene carbonate, and dimethyl carbonate (EC, PC, and DMC), into a poly(vinylidene fluoride-co-hexafluoropropylene) (PVDF-HFP) matrix. These gel electrolytes showed promising electrochemical performances. Some interesting examples of mixing ionic liquids with aprotic organic solvents to form hybrid electrolytes have been investigated. Our researches observed that by mixing LiTFSI with a reasonable concentration in ethylene carbonate and propylene carbonate with 1-ethyl-3-methylimidazolium bis(trifluoromethanesulfonyl)imide ionic liquid is possible to improve the safety without compromising performances. They observed that electrolytes containing 20% of IL offer the best compromise between viscosity and ionic conductivity, even cycling performance. The stability of electrode-electrolyte interphase (solid electrolyte interphase) as well as ion-diffusion mechanism to improve continuously actual problems in rechargeable batteries should be carried out. Moreover, ionic liquids are also promising candidates for lithium-sulfur or lithium-oxygen. To date, the development of secondary batteries has focused on small electric appliances and portable IT devices. Lithium secondary batteries are expected to build upon these achievements and create new applications, such as green energy, wireless charging, self-development, recycle, from portable to wearable, and flexible. It is an important task to make advance preparations for future batteries by considering the functions of these applications. Among the future applications of secondary batteries, medium- and large-sized cells show significant promise. Energy storage systems, in the form of batteries for electric vehicles and robots, or high-performance lithium secondary batteries capable of storing alternative energy such as solar, wind, and marine energy, are viewed as a key component of next-generation smart grid technology. Microcells and flexible batteries are other types of future secondary batteries. Microcells can be applied to RFID/USN, MEMS/NEMS, and embedded medical devices, while flexible batteries are mainly used in wearable computers and flexible displays. The structural control and manufacturing process of these batteries are different from today’s methods. The development of all-solid-state lithium secondary batteries is also highly anticipated. With massive recalls caused by frequent battery explosions, an important challenge that lies ahead is to resolve the instability problem of existing liquid electrolytes through the application of electrolytes consisting of polymers or organic/inorganic composites, along with the development of suitable electrode materials and processes. A series of polymer electrolytes are prepared through polymerization of 1-ethyl3-vinylimidazolium bis(trifluoromethanesulfonylimide) with poly(ethylene glycol) diacrylate (PEGDA) (Mn = 700 g mol−1), poly(ethylene glycol) methyl ether methacrylate (PEGME) (Mn = 500 g mol−1), and lithium bis(trifluoromethanesulfonyl)imide (LiTFSI) in an ionic liquid to obtain mechanically robust membranes. The prepared samples exhibit high thermal stabilities and display advantageous ionic conductivities
Lithium-Ion Batteries and Solar Cells
[42–47]. It appears that their electrochemical stabilities can be improved after we adjust the process by polymerizing the mixture on the LiFePO4 cathode directly, which is also responsible for the remarkable discharge capacity and improved capacity retention of the Li/LiFePO4 cells based on the prepared electrolytes. In summary, this research demonstrates a simple preparation through the facile photopolymerization method, and the current findings indicate that this type of electrolytes is promising for lithium ion batteries. Interestingly, this chapter covers the synthesis, structure, and electrical properties of pristine and treated PEDOT:PSS layer as well its application in silicon-nanowiresbased solar cells. It can significantly promote the full understanding of fundamental sciences, engineering deliberation, and emerging products. By the delicate facile method through the incorporation of EG as the cosolvents, the direct mixing of 7 wt% EG in precursors results in the optimum conductivity up to 103 orders of magnitude for the reduction of sheet resistance and remarkably improved up to 938 S cm−1 with high uniformity without employing post-treatment after thin-film fabrication. The Raman analysis and XPS results give more clear evidence about the conductivity enhancement that is attributed to the structural conformation. Also, the reduction of excess PSS chains at the surface is encountered, which can, therefore, increase the PEDOT/PSS ratio, initiate the phase separation of PEDOT and PSS chains inside the thin film, and positively influence the carrier doping level in the forms of polarons and bipolarons. Furthermore, the transmittance of deposited PEDOT:PSS films achieves more than 90% for the improvement of corresponding transparency in the visible-frequency region. The successful syntheses, detailed analyses, and well-behaved designs realized the explicit efficiency improvement of photovoltaic cells achieving >14% by the well management of electrical and optical properties of PEDOT:PSS layer. This can pave ways particularly for energy-based devices such as emerging solar cells, thermoelectric, and electrochromic applications [48,49]. However, the further chemical modifications (dopings and substitutions) [50,51], the physical methods, and delicate treatments of junctions/contacts with more comprehensive approaches would be finished in the near-future researches.
REFERENCES 1. Tu, Z., Choudhury, S., Zachman, M. J., Wei, S., Zhang, K., Kourkoutis, L. F., & Archer, L. A. (2017). Designing artificial solid-electrolyte interphases for single-ion and high-efficiency transport in batteries. Joule, 1(2), 394–406. 2. Jiang, F., & Peng, P. (2016). Elucidating the performance limitations of lithium-ion batteries due to species and charge transport through five characteristic parameters. Scientific Reports, 6, 32639. 3. Lin, C. E., Zhang, H., Song, Y. Z., Zhang, Y., Yuan, J. J., & Zhu, B. K. (2018). Carboxylated polyimide separator with excellent lithium ion transport properties for a high-power density lithium-ion battery. Journal of Materials Chemistry A, 6(3), 991–998. 4. Shan, X., Chen, S., Wang, H., Chen, Z., Guan, Y., Wang, Y.,… & Tao, N. (2015). Mapping local quantum capacitance and charged impurities in graphene via plasmonic impedance imaging. Advanced Materials, 27(40), 6213–6219.
5. Walsh, A., Scanlon, D. O., Chen, S., Gong, X. G., & Wei, S. H. (2015). Self‐regulation mechanism for charged point defects in hybrid halide perovskites. Angewandte Chemie International Edition, 54(6), 1791–1794. 6. Wang, J., Ma, A., Li, Z., Jiang, J., Feng, J., & Zou, Z. (2015). Effects of oxygen impurities and nitrogen vacancies on the surface properties of the Ta3N5 photocatalyst: A DFT study. Physical Chemistry Chemical Physics, 17(35), 23265–23272. 7. Huang, S. Z., Zhang, Q., Yu, W., Yang, X. Y., Wang, C., Li, Y., & Su, B. L. (2016). Grain boundaries enriched hierarchically mesoporous MnO/carbon microspheres for superior lithium ion battery anode. Electrochimica Acta, 222, 561–569. 8. Yang, F., Wang, D., Zhao, Y., Tsui, K. L., & Bae, S. J. (2018). A study of the relationship between coulombic efficiency and capacity degradation of commercial lithium-ion batteries. Energy, 145, 486–495. 9. Li, Z. Y., Wang, H., Yang, W., Yang, J., Zheng, L., Chen, D.,… & Liu, X. (2018). Modulating the electrochemical performances of layered cathode materials for sodium ion batteries through tuning coulombic repulsion between negatively charged TMO2 slabs. ACS Applied Materials & Interfaces, 10(2), 1707–1718. 10. Tran, N. T. T., Nguyen, D. K., Lin, S. Y., Gumbs, G., & Fa-Lin, M. (2019). Fundamental properties of transition-metals-adsorbed graphene. ChemPhysChem, 20(19), 2473–2481. 11. Kjellander, R. (2016). Decay behavior of screened electrostatic surface forces in ionic liquids: The vital role of non-local electrostatics. Physical Chemistry Chemical Physics, 18(28), 18985–19000. 12. Ji, H., Joo, M. K., Yi, H., Choi, H., Gul, H. Z., Ghimire, M. K., & Lim, S. C. (2017). Tunable mobility in double-gated MoTe2 field-effect transistor: Effect of coulomb screening and trap sites. ACS Applied Materials & Interfaces, 9(34), 29185–29192. 13. Winsberg, J., Hagemann, T., Janoschka, T., Hager, M. D., & Schubert, U. S. (2017). Redox‐flow batteries: From metals to organic redox‐active materials. Angewandte Chemie International Edition, 56(3), 686–711. 14. Zhang, Q., Wang, W., Wang, Y., Feng, P., Wang, K., Cheng, S., & Jiang, K. (2016). Controllable construction of 3D-skeleton-carbon coated Na3V2(PO4)3 for high-performance sodium ion battery cathode. Nano Energy, 20, 11–19. 15. Wächtler, F., & Santos, L. (2016). Quantum filaments in dipolar Bose-Einstein condensates. Physical Review A, 93(6), 061603. 16. Park, J. H., Liu, T., Kim, K. C., Lee, S. W., & Jang, S. S. (2017). Systematic molecular design of ketone derivatives of aromatic molecules for lithium‐ion batteries: First‐principles DFT modeling. ChemSusChem, 10(7), 1584–1591. 17. Zhang, C., Jiao, Y., He, T., Ma, F., Kou, L., Liao, T.,… & Du, A. (2017). Two-dimensional GeP3 as a high capacity electrode material for Li-ion batteries. Physical Chemistry Chemical Physics, 19(38), 25886–25890. 18. Lu, H., & Sun, S. (2018). Polyimide electrode materials for Li-ion batteries via dispersion-corrected density functional theory. Computational Materials Science, 146, 119–125. 19. Ullah, S., Denis, P. A., & Sato, F. (2017). Beryllium doped graphene as an efficient anode material for lithium-ion batteries with significantly huge capacity: A DFT study. Applied Materials Today, 9, 333–340. 20. Tran, N. T. T., Nguyen, D. K., Glukhova, O. E., & Lin, M. F. (2017). Coverage-dependent essential properties of halogenated graphene: A DFT study. Scientific Reports, 7(1), 17858. 21. Barik, G., & Pal, S. (2019). Energy gap-modulated blue phosphorene as flexible anodes for lithium-and sodium-ion batteries. The Journal of Physical Chemistry C, 123(5), 2808–2819.
Lithium-Ion Batteries and Solar Cells
22. Shiiba, H., Zettsu, N., Nakayama, M., Oishi, S., & Teshima, K. (2015). Defect formation energy in spinel LiNi0. 5Mn1. 5O4-δ using ab initio DFT calculations. The Journal of Physical Chemistry C, 119(17), 9117–9124. 23. Lin, M. F., & Hsu, W. D. (Eds.). (2019). Green Energy Materials Handbook. CRC Press, Boca Raton, FL. ISBN 9781138605916, chapter 7. 24. Tran, N. T. T., Lin, S. Y., Lin, C. Y., & Lin, M. F. (2017). Geometric and Electronic Properties of Graphene-Related Systems: Chemical Bonding Schemes. CRC Press, Boca Raton, FL. ISBN 9781138556522. 25. Niu, Z., Wu, H., Lu, Y., Xiong, S., Zhu, X., Zhao, Y., & Zhang, X. (2019). Orbitaldependent redox potential regulation of quinone derivatives for electrical energy storage. RSC Advances, 9(9), 5164–5173. 26. Liu, J., Zhao, T., Zhang, S., & Wang, Q. (2017). A new metallic carbon allotrope with high stability and potential for lithium ion battery anode material. Nano Energy, 38, 263–270. 27. Eriksson, S. K., Josefsson, I., Ellis, H., Amat, A., Pastore, M., Oscarsson, J.,… & Hagfeldt, A. (2016). Geometrical and energetical structural changes in organic dyes for dye-sensitized solar cells probed using photoelectron spectroscopy and DFT. Physical Chemistry Chemical Physics, 18(1), 252–260. 28. Mohr, T., Aroulmoji, V., Ravindran, R. S., Müller, M., Ranjitha, S., Rajarajan, G., & Anbarasan, P. M. (2015). DFT and TD-DFT study on geometries, electronic structures and electronic absorption of some metal free dye sensitizers for dye sensitized solar cells. Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, 135, 1066–1073. 29. Zhang, L., Liu, X., Rao, W., & Li, J. (2016). Multilayer dye aggregation at dye/TiO2 interface via π…π stacking and hydrogen bond and its impact on solar cell performance: A DFT analysis. Scientific Reports, 6, 35893. 30. Li, J., Klöpsch, R., Stan, M. C., Nowak, S., Kunze, M., Winter, M., & Passerini, S. (2011). Synthesis and electrochemical performance of the high voltage cathode material Li [Li0. 2Mn0. 56Ni0. 16Co0. O8]O2 with improved rate capability. Journal of Power Sources, 196(10), 4821–4825. 31. Zhu, L., Yan, T. F., Jia, D., Wang, Y., Wu, Q., Gu, H. T.,… & Tang, W. P. (2019). LiFePO4-coated LiNi0. 5Co0. 2Mn0. 3O2 cathode materials with improved high voltage electrochemical performance and enhanced safety for lithium ion pouch cells. Journal of the Electrochemical Society, 166(3), A5437–A5444. 32. Zhang, H., Gong, Y., Li, J., Du, K., Cao, Y., & Li, J. (2019). Selecting substituent elements for LiMnPO4 cathode materials combined with density functional theory (DFT) calculations and experiments. Journal of Alloys and Compounds, 793, 360–368. 33. Zhang, S. S. (2006). A review on electrolyte additives for lithium-ion batteries. Journal of Power Sources, 162, 1379–1394. 34. Lin, Y.-T., Lin, S.-Y., Chiu, Y.-H., & Lin, M.-F. (2016). Alkali-induced rich properties in graphene nanoribbons: Chemical bonding. arXiv:1609.05562v1(cond-mat.mes-hall). 35. Du Plessis, A., Yadroitsev, I., Yadroitsava, I., & Le Roux, S. G. (2018). X-ray microcomputed tomography in additive manufacturing: A review of the current technology and applications. doi: 10.1089/3dp.2018.0060. 36. Tang, T., & Luo, D. L. (2010). Density functional theory study of electronic structures in lithium silicates: Li2SiO3 and Li4SiO4. Journal of Atomic and Molecular Sciences, 1, 185. 37. Kuganathan, N., Kordatos, A., & Chroneos, A. (2018). Li2SnO3 as a cathode material for lithium-ion batteries: Defects, lithium ion diffusion and dopants. doi: 10.1038/ s41598-018-30554-y.
38. Rufieux, P., Cai, J., Plumb, N. C., Patthey, L., Prezzi, D., Ferretti, A.,… & Pignedoli, C. A. (2012). Electronic structure of atomically precise graphene nanoribbons. ACS Nano, 6, 6930–6935. 39. Kano, S., Tadaa, T., & Majima, Y. (2015). Nanoparticle characterization based on STM and STS. Chemical Society Reviews, 44, 970. 40. Guo, P., Song, H., & Chen, X. (2009). Electrochemical performance of graphene nanosheets as anode material for lithium-ion batteries. Electrochemistry Communications, 11, 1320–1324. 41. Wang, G., Shen, X., Yao, J., & Park, J. (2009). Graphene nanosheets for enhanced lithium storage in lithium ion batteries. Carbon, 47, 2049–2053. 42. Yin, K., Zhang, Z. X., Li, X. W., Yang, L., Tachibana, K., & Hirano, S. I. (2015). Polymer electrolytes based on dicationic polymeric ionic liquids: Application in lithium metal batteries. Journal of Materials Chemistry A, 3, 170–178. 43. Yin, K., Zhang, Z. X., Yang, L., & Hirano, S. I. (2014). An imidazolium-based polymerized ionic liquid via novel synthetic strategy as polymer electrolytes for lithium ion batteries. Journal of Power Sources, 258, 150–154. 44. Appetecchi, G. B., Kim, G. T., Montanina, M., Carewska, M., Marcilla, R., Mecerreyes, D., & De Meatza, I. (2010). Ternary polymer electrolytes containing pyrrolidiniumbased polymeric ionic liquids for lithium batteries. Journal of Power Sources, 195, 3668–3675. 45. Li, X. W., Zhang, Z. X., Li, S. J., Yang, L., & Hirano, S. (2016). Polymeric ionic liquid-plastic crystal composite electrolytes for lithium ion batteries. Journal of Power Sources, 307, 678–683. 46. Safa, M., Chamaani, A., Chawla, N., & El-Zahab, B. (2016). Polymeric ionic liquid gel electrolyte for room temperature lithium battery applications. Electrochimica Acta, 213, 587–593. 47. Zhang, P. F., Li, M. T., Yang, B. L., Fang, Y. X., Jiang, X. G., Veith, G. M.,… & Dai, S. (2015). Polymerized ionic networks with high charge density: Quasi‐solid electrolytes in lithium‐metal batteries. Advanced Materials, 27, 8088–8094. 48. Kim, G. H., Shao, L., Zhang, K., & Pipe, K. P. (2013). Engineered doping of organic semiconductors for enhanced thermoelectric efficiency. Nature Materials, 12(8), 719–723. 49. Alemu Mengistie, D., Wang, P. C., & Chu, C. W. (2013). Effect of molecular weight of additives on the conductivity of PEDOT:PSS and efficiency for ITO-free organic solar cells. Journal of Materials Chemistry A, 1(34), 9907–9915. 50. Kim, N., Kee, S., Lee, S. H., Lee, B. H., Kahng, Y. H., Jo, Y. R.,… & Lee, K. (2014). Highly conductive PEDOT:PSS nanofibrils induced by solution-processed crystallization. Advanced Materials, 26(14), 2268–2272. 51. Zhang, S., Fan, Z., Wang, X., Zhang, Z., & Ouyang, J. (2018). Enhancement of the thermoelectric properties of PEDOT:PSS: Via one-step treatment with cosolvents or their solutions of organic salts. Journal of Materials Chemistry A, 6(16), 7080–7087.
Open Issues and Potential Applications Thi Dieu Hien Nguyen, Ngoc Thanh Thuy Tran, and Ming-Fa Lin National Cheng Kung University
CONTENT References .............................................................................................................. 269 The theoretical predictions, which are conducted by the numerical simulations and the phenomenological models, are available in understanding the essential properties of green energy materials, especially for the geometric, electronic, optical, and transport properties [1,2] of the Li+-ion-based batteries (LIBs) (Figure 15.1). The former covers the first-principles calculations (e.g., Vienna ab initio simulation package (VASP); [3,4]), molecular dynamics with the empirical intrinsic interactions , and quantum Monte Carlo within the Pauli principle [6,7]. The numerical simulation methods have been frequently utilized in fully exploring the optimal geometries with various chemical bonds ; atom- and spin-dominated energy spectra and wave functions ; spatial charge/spin density distributions; and atom-, orbital-, and spindecomposed density of states , as done for cathode, electrolyte, and anode of Li+-related batteries (Figure 15.1a; details in Chapters 4–7). According to the development of the theoretical framework, the critical multi-/single-orbital hybridizations of the chemical bonds could be delicately identified from the above-mentioned physical quantities. The similar analyses could be generalized to other emergent materials in batteries, e.g., the popular four-component LiFePO cathode [11–13] and silicon/ germanium nanotube anode . They will be completed in the near-future studies. It is well known that the electronic properties, absorption spectra, electrical conductivities, and Coulomb excitations could be understood from the tight-binding model/the effective-mass approximation , the dynamic Kubo formula , the static one (discussed later ), and the random-phase approximation . However, these methods are seldom utilized in the fundamental properties of cathode, electrolyte, and anode materials, mainly owing to a lot of atoms with the various chemicalbonding strengths in a primitive unit cell. For example, there are many oxygen-related chemical bonds under a specific crystal structure (details in Chapters 4–7; [18,19]). The parameters, which are required in the tight-binding model, cover the various orbital-hybridization-dependent hopping integrals  and the different ionization energies (the distinct on-site Coulomb potentials; ). Specifically, the former is very sensitive to the chemical bond lengths . In general, they are obtained from the well-fitting between this model and the first-principles method in the band 261
Lithium-Ion Batteries and Solar Cells
FIGURE 15.1 (a) Lithium-, (b) aluminum-, and (c) iron-ion-based batteries
structure . However, it might be very difficult to achieve this object because of the very complicated results of VASP calculations [3,4,23]. The generalized tightbinding model, which is developed for the magnetic quantization phenomenon , will become meaningless, since the magnetically quantized Landau sub-bands are too complicated to identify from the magnetic-field-dependent energy spectra and localized wave functions . The development of the tight-binding model will be very helpful in providing concise physical properties about the optical properties. The up-to-date optical reflection/absorption/transmission spectroscopies  are available in examining the diversified valence and conduction energy spectra . When any material is perturbed by the external electromagnetic fields, the occupied electronic states are vertically excited to the unoccupied ones under the conservations of momentum and energy. The initial and final states almost have the same wave vectors because of the negligible photon momentum. Such high-resolution optical measurements could provide the threshold absorption frequency (the optical gap; ) and the prominent excitation structures, in which the latter are created by the van Hove singularities of
Open Issues and Potential Applications
the initial and/or final states. From the theoretical viewpoints, one needs to calculate the number of excitation channels and the intensity of vertical transitions. According to the Fermi golden rule  or the linear Kubo formula , the optical absorption spectrum is due to the perturbation of an electric dipole moment. That is, it is proportional to the joint density of states through the initial and final states and each channel intensity, where the former and the latter are, respectively, associated with energy bands and wave functions. How to evaluate the optical transition intensity, or efficiently link the close relations of the tight-binding model and the dynamic Kubo formula, is just the studying focus. Moreover, the systematic studies have been successfully conducted on the layered graphene-related systems for their optical  and magneto-optical properties . More heavy works need to be done to fully explore the diversified absorption behaviors of the multicomponent cathode, electrolyte, and anode materials [29–31]. The dielectric Coulomb screening (details in ) is one of the mainstream topics in any condensed matter systems. This phenomenon, which directly reflects the intrinsic response of macroscopic charge fluctuations, is well characterized by the dimensionless energy loss function (a universal quantity; ). In general, the electronic excitation behaviors, the single-particle electron–hole pairs (the Landau damping; ) and collective excitations (plasmon modes; [34,35]), could be examined/verified from the momentum- and frequency-enriched inelastic scatterings of the incident high-energy electron beam (electron energy loss spectroscopy [EELS]; ). Most important, the high-resolution EELS is capable of identifying the diverse (momentum, frequency)-dependent excitation-phase diagrams with the simultaneous e–h regions and plasmon dispersion relations . The rich and unique Coulomb excitations in layered graphene systems have been presented under the efficient couplings between the generalized tight-binding model and the modified random-phase approximation, where the intralayer and interlayer hopping integrals and Coulomb interactions are included in the calculations simultaneously . The critical factors and the concise physical properties are clearly illustrated in this book . For example, the low-frequency plasmons, which, respectively, arise from the quantization modes of the collective free-carrier and free-electron oscillations, are very sensitive to the direction and magnitude of the transferred momentum . They are greatly diversified by the temperature , carrier doping , layer number , stacking configuration [40,41], dimension , planar or cylindrical symmetry , gate voltage , and magnetic field [34,42]. Very interesting, the dimensionless screened response function is well defined for the coupled 2D structures. The developed theoretical framework is also useful in understanding the Coulomb decay rates of the excited carriers , e.g., the quasiparticle lifetimes due to the Coulomb scatterings with the strong energy and wave-vector dependences for monolayer graphene , silicene [45,46], and germanene . The small first Brillouin zone would lead too much difficulty of the randomphase approximation in the momentum- and frequency-dependent bare and screened response functions, because most of the transferred momenta during the electron– electron interactions are frequently beyond the smallest reciprocal lattice vector . The up-to-date experimental growths show that many emergent materials have large unit cells under the unequal lattice symmetries. For example, the very popular
Lithium-Ion Batteries and Solar Cells
Li+-based batteries are purely made up of the lithium oxide ternary-/four-component compounds in terms of cathode, electrolyte, and anode materials, e.g., corresponding to the 3D LiFe/Co/NiPO [48,49–54], LiSi/Ge/SnO [47,55,56], and LiSc/Ti/VO systems, respectively [57–60]. The chemical bonds could exist only through the multi-orbital hybridizations with oxygen atoms or only the X–O bonds are revealed in the stable 3D optimal geometric structures, such as the 48 Li–O and 52 Ti–O bonds with the great modulated bond lengths in the VASP calculations (Chapter 4; ). Moreover, the complicated multi-orbital mixings are delicately identified from the atom- and orbital-decomposed van Hove singularities, the spatial charge density distribution, and the atom-dominated energy spectrum. Such mechanisms have generated significant energy gaps in various battery materials. Apparently, the orbital-dependent on-site Coulomb energies and a lot of orbital- and bond-lengthrelated hopping integrals need to be covered in the Hamiltonian of the tight-binding model. The Coulomb matrix elements, which come to exist in the dielectric screening effects, might be closely related to (2s, 2px, 2py, 2pz) and (4s, 3d x 2 − y2 , 3dxy, 3dyz, 3dzx, 3d z 2 ) orbitals. Most important, how to efficiently solve the strong local field effects for large unit cells and well characterize the dimensionless energy loss function is the studying focus. Maybe, the development of the dielectric function tensor [59,60] could provide an effective way of exploring the complicated Coulomb screening phenomena. In short, the semiconducting/insulating behaviors with important band gaps and the complex Coulomb scattering processes are expected to become the negative factors in creating the plasmon modes of valence electrons even under the long-wavelength limit. Very interesting, the ion-based batteries present the rich and unique phenomena after the electrical-chemical reactions. During the charging processes, the Li+-/Al+-/ Fe+-ions [61–67] are released from cathode [64–66], transport through electrolyte [64–66], and enter into anode [64–66]. And then, the opposite is true for the discharge processes [64–66]. Apparently, the ion transports have created drastic changes in terms of geometric structures , chemical environments , and scattering events . For example, the reduced Li+-ions and electrons in 3D ternary LiFe/Co/NiO cathode would lead to the dramatic transformation of lattice symmetry. It might exist a lot of intermediate geometric configurations between two metastable ones, in which they possess very large unit cells. How to link the complicated relations of the former and the latter is an important issue. For the well-characterized cathodes, the VASP calculations can investigate the main features of geometric properties, e.g., the various Li–O and Fe–/Co/Ni–O bond lengths under a specific crystal structure with the atom number below 100–200 [69–71]. However, the other simulation methods [70,71] are required to solve the optima geometries for the short-lifetime configurations beyond the critical atom number in a unit cell. The similar geometric transformations are expected to be revealed in electrolyte and anode materials. Specifically, there exist the negatively charged anode systems because of the electron current through the external lead circuit. Such light-free carriers might display outstanding screening abilities, as observed for conduction electrons in metals . Their important roles on the intercalation and de-intercalation phenomena and the fundamental properties, which come to exist in graphite Li+-intercalated compounds/LiTiO , are worthy of the systematic investigations, such as the dielectric effects on the Li+-concentration-dependent
Open Issues and Potential Applications
ground-state energies, band structures, wave functions, and metallic/semimetallic/ semiconducting behaviors. Furthermore, whether the Li+-ions or the neutral Li-atoms survive in the intercalated/de-intercalated anodes is one of the studying focuses [73,74]. Even for the first-principles simulations, the simultaneous consideration of the electron cloud, anode material, and Li+-intercalation/ Li+-de-intercalation will become a serious challenge. It should be noticed that the up-to-date various experimental measurements could not clarify this issue. The experimental examinations might require the techniques and equipment [73,74]. From the theoretical and experimental viewpoints, the ion transports play critical roles in developing lithium-/aluminum-/iron-based batteries [67,75–77] with the outstanding high-rate capability and high power. Their mechanisms and physical, chemical, and material properties need to be clarified in the near-future investigations. For example, the Li+-related batteries consist of the nanostructured materials: (I) cathode of LiFe/Co/NiO [48–54], (II) electrolyte of LiSi/Ge/SnO [47,55,56], and (III) anode of LiSc/Ti/VO [57–60], belonging to the ternary lithium oxide compounds. However, it is very difficult to predict/examine/identify the nature of Li-ion transport behaviors within the core components. Very interesting, recently the high-resolution experimental techniques are developed to study the local Li-ion diffusion , such as the rapid transport through grain boundaries in LixCoO2 using conductive atomic force microscopy with a spatial resolution of 10 nm. They can provide important information of optimizing cathode, electrolyte, and anode materials [23,29–31] and developing nanoionics . Most important, the significant factors, which are closely related to the nanostructures materials, might cover the interlayer spacing or the grain boundary , the concentration of Li+ vacancies , the extremely nonuniform chemical environments (e.g., the great modulation of bond lengths; ), and the Coulomb screening effects due to the valence electrons. How to link them simultaneously in the theoretical framework of the ion transports will become an emergent challenge, such as the prediction of the steady current density in cathode, electrolyte, and anode materials under various scattering events . As to the trivalent and bivalent cases (aluminum and iron ions discussed later; ), the ion transports are getting more complicated because of the large ionic structures [84,85] and the non-negligible chemical reactions at the interfaces between electrolyte and anode or cathode materials . The development of nanoionics is urgently required in the experimental  and theoretical  explorations. Silicon/germanium/carbon nanotubes and nanowires might have high performances or potential applications in Li+-based batteries . The hollow carbon nanotubes were first discovered by I. Iijima in 1991 through an electric arc with specific catalysts . Each single-walled nanotube possesses a perfect cylindrical surface as a result of carbon hexagons (Figure 15.2a; ), leading to the unusual periodical boundary condition [91,92]. All electronic states are described by the longitudinal wave vector and the transverse angular momentum, as measured from the axial direction . The achiral and chiral carbon nanotubes have been clearly examined by the high-resolution scanning tunneling microscopy (STM; [94,95]). Furthermore, the extension of STM and scanning tunneling spectroscopy (STS; ) is capable of identifying the low-energy electronic properties simultaneously. That is, the STS measurements can distinguish the semiconducting and metallic behaviors .
Lithium-Ion Batteries and Solar Cells
FIGURE 15.2 Geometric structures of (a) carbon nanotubes and (b) silicon nanotubes
According to the up-to-date experiment examinations  and theoretical predictions [97,98] about the low-lying electronic energy spectra near the Fermi level, the radius- and chiral-angle-dependent single-walled carbon nanotubes could be classified into three kinds [99,100]: (I) metals, (II) narrow-, and (III) middle-gap semiconductors, in which they, respectively, have 1D linear conduction and valence bands intersecting at EF, and energy gaps inversely proportional to radius and the square of radius. When carbon nanotubes are further synthesized together, the multiwalled [101,102] or bundle systems are almost uniformly grown in experimental laboratories under the large-scale quantity [101,102]. This phenomenon will provide a lot of available positions during the Li+-ion intercalations and de-intercalations. From the viewpoints of mathematics, physics, chemistry, and materials, carbon nanotubes are worthy of the systematic investigations on the basic [101,102] and applied  sciences, e.g., the many-particle Coulomb excitations and decay rates in the current studies [105,106]. The chemical modifications on them are expected to greatly diversify the application functionalities, e.g., the enhanced storage of atoms or molecules or ions by the intercalation , chemisorption , and substitution . It should have certain important differences and similarities between 1D silicon or germanium [110,111] and carbon nanotubes . Silicon nanotubes and nanowires have been successfully synthesized through the chemical vapor deposition by using an electric in the absence of any catalysts [113,114]. Each silicon nanotube could be regarded as a cylindrically rolled-up monolayer silicene (Figure 15.2b), as clearly
Open Issues and Potential Applications
illustrated between carbon nanotube and graphene [114,115]. Geometric structures of any nanotubes are well characterized by the radius and chirality; therefore, the essential physical, chemical, and material properties are very sensitive to these two critical factors. However, a buckling structure (a nonplanar honeycomb lattice; [45–47]), corresponding to different heights of the A and B sublattices, is induced by significant competition of the sp2 and sp3 bondings on a monolayer silicene ; the absence of the latter on carbon nanotubes). This will be directly reflected on a cylindrical surface, further leading to the enhancement of the bonding misorientation and the Si-four-orbital hybridization. Moreover, the spin-orbital couplings (the quantum effect under the relative theory; [116,117]) need to be taken into consideration during the calculations of electronic properties. As a result, how many kinds of silicon nanotubes in terms of band gaps might require the delicate calculations and analyses, as done for carbon nanotubes . The first-principles method  and the tightbinding model  would be suitable in fully exploring the low-energy fundamental properties. For example, they are reliable in investigating whether the metallic silicon nanotubes  could survive under the specific geometries. Most important, the potential applications on ion-based batteries are closely related to the intercalations/ de-intercalations of the metallic ions or atoms. Only the VASP calculations can deal with the chemical modifications on the essential properties and thus provide the full information about the useful transport functionalities of silicon nanotubes, e.g., the optimal geometric structure, the highest ion concentration, the spatial charge density distributions, and the semiconducting or metallic property for the ion-intercalated silicon nanotube compounds. The detailed comparisons with the carbon nanotube intercalation compounds would be completed under the accurately numerical simulations [103,112] and the concise physical, chemical, and material properties [105,108]. Obviously, the storage of atoms and molecules inside silicon nanotubes or silicon nanotube bundles [122,123] becomes very meaningful for the potential applications of green energies, such as the capture of hydrogen gases [124,125] and carbon oxides [125–127] and the intercalation of Li+-ions/Li-atoms. The active chemical environments  and the important orbital hybridizations  of various chemical bonds are predicted to play critical roles in the basic  and applied  sciences. The theoretical framework under the numerical simulations  and the phenomenological modes  will be developed or proposed in the near-future researches. One big drawback of currently used LIBs is its safety and fire hazards due to the volatility of conventional organic liquid electrolytes inside the battery. To address this issue, solid electrolytes have been developed to eliminate the use of flammable liquids. All-solid-state battery is considered as the next-generation batteries with high power, high energy density, and high intrinsic safety storage system, in which the solid electrolyte is one of the key components that determine its performance [131–133]. Solid electrolytes can be divided into two categories, namely solid inorganic electrolyte and solid polymer electrolyte. The former consists of various types of structures, including crystalline electrolytes (perovskite , NASICON , garnet , and LISICON types ), amorphous electrolytes (oxide  and sulfide glassy  types), thio-LISICON-type , LiPON-type , and glassceramic  electrolytes. For the case of solid polymer electrolytes, polyethylene oxide (PEO) is the most commonly used. Despite the advantages of solid electrolytes
Lithium-Ion Batteries and Solar Cells
exhibit over liquid electrolytes, there is still intrinsic challenges such as low ionic conductivity, grain boundary resistance, and dendrite formation with Li metal anodes. The search for stable solid electrolytes with high conductivity is currently an important issue to compete the liquid ones in commercial batteries. Among all the solid electrolytes, NASICON (natrium superionic conductor), garnet, and LISICON (lithium superionic conductor) exhibit the high ionic conductivities at the room temperature . Specifically, the garnet-type Li7La3Zr2O12 (LLZO) solid electrolyte is commonly observed in two phases (tetragonal and cubic), in which its ionic conductivity is higher than that of tetragonal LLZO by two orders of magnitude . Cubic LLZO is considered as one of the best solid electrolytes due to its remarkable chemical and thermal stability. Thermodynamic simulations in terms of the phase diagram and phase stability are expected to provide a better understanding of the solid electrolyte interface problems with electrode materials, including Li-dendrite penetration on anode side (Li-metal) and bad interfacial connection on the cathode side. Further improvements to select the compatibility combination of electrode and electrolyte materials for solid-state LIBs are necessary to satisfy the rapidly increasing demand, especially electric vehicles and mass energy storage systems. In addition to lithium-ion-related batteries, aluminum-ion-based ones are successfully applied in the commercial products, such as hybrid electric vehicles (HEVs) [132,133], plug-in hybrid electric vehicles (PHEVs) , and the electrical grid [146–148]. In general, they principally consist of the anode, electrolyte, and cathode materials, respectively, corresponding to the metallic aluminum , the ionic liquid, and the semimetallic/semiconducting graphite/MoS2 [65,149–155]. Specifically, the first condensed matter system is a thin Al foil with a thickness of ~20 −6 m. Very interesting, an ionic liquid electrolyte (an ionically conductive medium) comes to exist by mixing 1-ethyl-3-methylimidazolium chloride ((EMIm)Cl) and aluminum chloride (AlCl3), being able to produce redox active chloroaluminate anions (AlCl −4 and Al 2 Cl −7 ). These two kinds of anions are responsible for the ion transport; furthermore, the experimental processes need to prevent the electrolyte from being modified by chemical reactions. A thin-film pristine graphite of thickness ~50–100 10 −6 m provides the enough and at spaces for the intercalations/de-intercalations of the anion ions, since the interlayer 3pZ orbital interactions of the graphitic sheets belong to the weak but significant van der Waals forms. The intercalation effects on the optimal geometric structures and the fundamental electronic properties could be investigated through the VASP calculations, e.g., the combined distribution configuration of AlCl −4 and Al 2 Cl −7 anions [151,152,156,157], and the dramatic changes in the spatial charge density distributions [65,158,159] and the low-lying valence and conduction bands near the Fermi level . Most important, the aluminum-ion batteries belong to a class of rechargeable ones, where Al-related ions can provide energy by transporting from the anode to cathode materials. In the recharging processes, the aluminumrelated ions come back to the negative electrode and can exchange three electrons per ion. This clearly illustrates that the insertion of one Al3+ is equivalent to three Li+-ions in conventional intercalation cathodes . The trivalent charge carrier in Al3+ is just merit and drawback, where the transfer of three-unit charges by one ion greatly enhances energy storage capacity [156–161] but creates too strong electrostatic intercalation for the host materials under the well-defined electrochemical behavior.
Open Issues and Potential Applications
Recently, the third kind of secondary batteries, the iron-ion-based one (Figure 15.1c), has been successfully developed for the first time under a specific capacity of 207 mAh g−1 at 30 mA g−1. The most important merit is quite cheap, and the other characteristics require high-resolution experimental examinations . Very interesting, this new kind of battery mainly consists of mild steel, layered vanadium pentoxide (V2O5; ), and tetraethylene glycol dimethylether (TEGDME; ), respectively, corresponding to anode, cathode, and electrolyte solvent. The first material is mostly made up of iron (99.33% in weight), while few components mainly originate from carbon (0.15%) and manganese (0.52%). Apparently, the 3D ternary iron compound possesses a superlarge unit cell, since the concentrations of the substitution atoms are very dilute. This will result in a rather high barrier in the first-principles calculations of the optimal geometric structures , and thus, the other essential physical, chemical, and material properties , for example, how many chemical bonds and the great bond-length modulations have to be determined in the numerical simulations, mainly owing to the creation of the extremely nonuniform chemical environment in a primitive unit cell . As to the binary V2O5 cathode, the pristine system has a well-behaved crystal structure  and belongs to an interesting ferroelectric semiconductor . However, the multi-orbital hybridizations in oxygen-related chemical bonds are worthy of the thoroughly theoretical investigations through the spatial charge density distributions around vanadium and oxygen atoms and atom- and orbital-decomposed density of states , as done earlier in Chapters 4–7 for Li+-ion-battery cathode or electrolyte or anode materials using the VASP calculations. The intercalations/de-intercalations of Fe2+ ions into/from the cathode material would be very interesting topics, e.g., the existence of metastable and intermediate configurations and the diversified electronic properties. Moreover, the replacement of cathode and electrolyte materials in Fe2+related batteries might greatly enhance the performance of ion transport, i.e., the optimal combinations of the cathode, electrolyte, and anode materials need a series of experimental tests .
REFERENCES 1. Tarascon, J.-M.; Armand, M. Issues and challenges facing rechargeable lithium batteries. Nature 2001, 414, 359–367. 2. Salvadori, A.; Grazioli, D.; Geers, M. G. D.; Danilov, D.; Notten, P. H. L. A multiscalecompatible approach in modeling ionic transport in the electrolyte of Lithium-ion batteries. Journal of Power Sources 2015, 293, 892–911. 3. Vaderbilt, D. Soft self-consistent pseudopotential in a generalized eigenvalue formalism. Physics Review B 1990, 41, 7892–7895. 4. Krese, G.; Furthmuller, J. Efficient iterative schemes for ab ratio total-energy calculations using a plane-wave basis set. Physics Review B 1996, 54, 11169–11186. 5. Kashammer, P.; Sinno, T. Interactions of twin boundaries with intrinsic point defects and carbon in silicon. Journal of Applied Physics 2013, 114, 083505. 6. Austin, B. M.; Zubarev, D. Y.; Lester, W. A. Quantum Monte-Carlo and related approaches, Chemical Reviews 2012, 112(1), 263–288. 7. Needs, R. J.; Towler, M. D.; Drummond, N. D. Continuum variational and diffusion quantum Monte-Carlo calculations. Journal of Physics: Condensed Matter 2010, 22(2), 023201.
Lithium-Ion Batteries and Solar Cells
8. Kitta, M.; Akita, T.; Maeda, Y.; Kohyama, M. Preparation of a spinel Li4Ti 5O12(1 1 1) surface from a rutile TiO2 single crystal. Applied Surface Science 2012, 258, 3147–3151. 9. Shih, P.-H.; Do, T.-N.; Gumbs, G.; Huang, D.; Pham, H. D.; Lin, M. F. Rich magnetic quantization phenomena in AA bilayer silicene. Scientific Reports 2019, 9, 14799. 10. Kitta, M.; Matsuda, T.; Maeda, Y.; Akita, T.; Tanaka, S.; Kido, Y.; Kohyama, M. Atomistic structure of a spinel Li4Ti5O12(1 1 1) surface elucidated by scanning tunneling microscopy and medium energy ion scattering spectrometry. Surface Science 2014, 619, 5–9. 11. Yi, T.-F.; Li, X.-Y.; Liu, H.; Shu, J.; Zhu, Y.-R.; Zhu, R.-S. Recent developments in the doping and surface modification of LiFePO4 as cathode material for power lithium ion battery. Ionics 2012, 18(6), 529–539. 12. Zaghib, K.; Goodenough, J. B.; Mauger, A.; Julien, C. Unsupported claims of ultrafast charging of LiFePO4 Li-ion batteries. Journal of Power Sources 2009, 194(2), 1021–1023. 13. Sun, C.; Rajasekhara, S.; Goodenough, J. B.; Zhou, F. Monodisperse porous LiFePO4 microspheres for a high-power Li-ion battery cathode. Journal of the American Chemical Society 2011, 133, 2132–2135. 14. Bensalah, N.; Kamand, F. Z.; Mustafa, N.; Matalqeh, M. Silicon-germanium bilayer sputtered onto a carbon nanotube sheet as anode material for lithium-ion batteries. Journal of Alloys and Compounds 2019, 152088. 15. Kittel, C. Introduction to Solid State Physics, 8th Edition, Wiley, New York, 2004. 16. Nakayama, T.; Shima, H. Computing the Kubo formula for large systems. Physical Review E 1998, 58(3), 3984–3992. 17. Chen, G. P.; Voora, V. K.; Agee, M. M., Balasubramani, S. G.; Furche, F. Random-phase approximation methods. Annual Review of Physical Chemistry 2017, 68, 421–445. 18. Ouyang, C. Y.; Zhong, Z. Y.; Lei, M. S. Ab initio studies of structural and electronic properties of Li4Ti5O12 spinel. Electrochemistry Communications 2007, 9, 1107–1112. 19. Sun, X.; Radovanovic, P. V.; Cui, B. Advances in spinel Li4Ti5O12 anode materials for lithium-ion batteries. New Journal of Chemistry 2015, 39, 38–63. 20. Silva-Guillen, J.; San-Jose, P.; Roldan, R. Electronic band structure of transition metal dichalcogenides from ab initio and Slater-Koster tight-binding model. Applied Sciences 2016, 6(10), 284. 21. Lin, C.-Y.; Wu, J.-Y; Chiu, C.-W; Lin, M.-F. Coulomb Excitations and Decays in Graphene-Related Systems, 1st Edition, CRC Press, Boca Raton, FL, 2019. 22. Veerapandian, M.; Lee, M. H.; Krishnamoorthy, K.; Yun, K. Synthesis, characterization and electrochemical properties of functionalized graphene oxide. Carbon 2012, 50, 4228–4228. 23. Ullah, A.; Majid, A.; Rani, N. A review on first principles-based studies for improvement of cathode material of lithium ion batteries. Journal of Energy Chemistry 2018, 27(1), 219–237. 24. Lin, C.-Y.; Wu, J.-Y.; Ou, Y.-J.; Chiu, Y.-H.; Lin, M.-F. Magneto-electronic properties of multilayer graphenes. Physical Chemistry Chemical Physics 2015, 17(39), 26008–26035. 25. Suzuki, S.; Takamura, M.; Yamamoto, H. Transmission, reflection, and absorption spectroscopy of graphene microribbons in the terahertz region. Japanese Journal of Applied Physics 2016, 55, 06GF08. 26. Zhang, J. M.; Liu, Y. Fermi’s golden rule: Its derivation and breakdown by an ideal model. European Journal of Physics 2016, 37, 6. 27. Oughstun, K. E. Electromagnetic and Optical Pulse Propagation. Springer Series in Optical Sciences, 1st Edition, Springer, New York, 2019.
Open Issues and Potential Applications
28. Tran, N. T. T.; Lin, S.-Y.; Lin, C.-Y.; Lin, M.-F. Geometric and Electronic Properties of Graphene-Related Systems: Chemical Bonding Schemes, 1st Edition, CRC Press, Boca Raton, FL, 2017. 29. Stanley Whittingham, M. Lithium batteries and cathode materials. Chemical Reviews 2004, 104(10), 4271–4302. 30. Mekonnen, Y.; Sundararajan, A.; Sarwat, A. I. A Review of Cathode and Anode Materials for Lithium-Ion Batteries. Southeast Conference, IEEE, Norfolk, VA, 2016, pp. 1–6. 31. Khan, S. A.; Ali, S.; Saeed, K.; Usman, M.; Khan, I. Advanced cathode materials and efficient electrolytes for rechargeable batteries: Practical challenges and future perspectives. Journal of Materials Chemistry A 2019, 7, 10159–10173. 32. Friedberg, R.; Zhao, H. S. Short-range Coulomb screening in a dielectric crystal. Physical Review B 1991, 44(5), 2297–2305. 33. Ou, Y. C.; Sheu, J. K.; Chiu, Y. H.; Chen, R. B.; Lin M. F. Influence of modulated fields on the Landau level properties of graphene. Physics Review B 2011, 83, 195405. 34. Chen, R. B.; Chiu, C. W.; Lin, M. F. Magneto plasmons in simple hexagonal graphite. RSC Advances 2015, 5, 53736–53740. 35. Chuang, Y. C.; Wu, J. Y.; Lin, M. F. Electric field induced plasmon in AA stacked bilayer graphene. Annals of Physics 2013, 339, 198. 36. Hart, J. L.; Lang, A. C.; Le, A. C.; Longo, P.; Trevor, C.; Twesten, R. D.; Taheri, M. L. Direct detection electron energy-loss spectroscopy: A method to push the limits of resolution and sensitivity. Scientific Reports 2017, 7(1), 8243. 37. Hwang, E. H.; Sensarma, R.; Sarma, D. S. Plasmon-phonon coupling in graphene. Physics Review B 2010, 82(19), 195406. 38. Chiu, Y. H.; Lai, Y. H.; Ho, J. H; Chuu, D. S.; Lin, M. F. Electronic structure of a twodimensional graphene monolayer in a spatially modulated magnetic field: Peierls tightbinding model. Physical Review B 2008, 77, 045407(6). 39. Lin, M. F.; Shyu, F. L. Temperature-induced plasmons in a graphite sheet. Journal of Physical Society Japan 2000, 69, 607–610. 40. Lin, M. F.; Shyu, F. L. Plasmons and optical properties of semimetal graphite. Journal of Physical Society Japan 2000, 69, 3781–3784. 41. Shyu, F. L.; Lin, M. F.; Lu, Y. T. Electronic excitations in cylinder superlattices. Journal of Physical Society Japan 1999, 68, 3352–3359. 42. Wu, J. Y.; Gumbs, G.; Lin, M.-F. Combined effect of stacking and magnetic field on plasmon excitations in bilayer graphene. Physics Review B 2014, 89, 165407. 43. Lin, C. Y.; Lee, M. H.; Lin, M.-F. Coulomb excitations in ABC-stacked trilayer graphene. Physical Review B 2018, 98(4), 041408. 44. Ou, Y. C.; Chiu, Y. H.; Lu, J. M.; Su, W. P.; Lin, M.-F. Electric modulation effect on magneto-optical spectrum of monolayer graphene. Computer Physics Communications 2013, 184, 1821–1826. 45. Lin, C.-L.; Arafune, R.; Kawahara, K.; Kanno, M.; Tsukahara, N.; Minamitani, E.; Kim, Y.; Kawai, M.; Takagi, N. Substrate-induced symmetry breaking in silicene. Physical Review Letters 2013, 110, 076801. 46. Tabert, C. J.; Nicol, E. J. Magneto-optical conductivity of silicene and other buckled honeycomb lattices. Physical Review B 2013, 88, 085434. 47. Davila, M. E.; Xian, L.; Cahangirov, S.; Rubio, A.; Le Lay, G. Germanene: A novel two-dimensional germanium allotrope akin to graphene and silicene. New Journal of Physics 2014, 16, 095002. 48. Devaraju, M. K.; Honma, I. Hydrothermal and solvothermal process towards development of LiMPO4 (M = Fe, Mn) nanomaterials for lithium-ion batteries. Advanced Energy Materials 2012, 2, 284–297.
Lithium-Ion Batteries and Solar Cells
49. Huang, H.; Yin, S.-C.; Nazar, L. F. Approaching theoretical capacity of LiFePO4 at room temperature at high rates. Electrochemical and Solid-State Letters 2001, 4, A170–A172. 50. Devaraju, M. K.; Truong, Q. D.; Tomai, T.; Hyodo, H.; Honma, I. Antisite defects in LiCoPO4 nanocrystals synthesized via a supercritical fluid process. RSC Advances 2014, 4, 52410–52414. 51. Devaraju, M. K.; Truong, Q. D.; Hyodo, H.; Tomai, T.; Honma, I. Supercritical fluid methods for synthesis of LiCoPO4 nanoparticles and their application to lithium ion battery. Inorganics 2014, 2, 233–247. 52. Truong, Q. D.; Devaraju, M. K.; Tomai, T.; Honma, I. Controlling the shape of LiCoPO4 nanocrystals by supercritical fluid process for enhanced energy storage properties. Scientific Reports 2014, 4, 3975. 53. Devaraju, K.; Truong, Q. D.; Hyodo, H.; Sasaki, Y.; Honma, I. Synthesis, characterization and observation of antisite defects in LiNiPO4 nanomaterials. Scienetific Reports 2015, 5(1), 11041. 54. Manickam, M.; Pritam, S.; Dominique, A.; Danielle, E. M. Synthesis of olivine LiNiPO4 for aqueous rechargeable battery. Electrochimica Acta 2011, 56, 4356–4360. 55. Tang, T.; Chen, P.; Luo, W.; Luo, D.; Wang, Y. Crystalline and electronic structures of lithium silicates: A density functional theory study. Journal of Nuclear Materials 2012, 420, 31–38. 56. Ma, S.-G.; Shen, Y.-H.; Kong, X.-G.; Gao, T.; Chen, X.-J.; Xiao, C.-J.; Lu, T.-C. A new interatomic pair potential for the modeling of crystalline Li2SiO3. Materials and Design 2017, 118, 218–225. 57. Liu, Z.; Deng, H.; Zhang, S.; Hu, W.; Gao, F. Theoretical prediction of LiScO2 nanosheets as a cathode material for Li-O2 batteries. Physical Chemistry Chemical Physics 2018, 20, 22351–22358. 58. Lu, X.; Gu, L.; Hu, Y. S. New insight into the atomic-scale bulk and surface structure evolution of Li4Ti5O12 anode. Journal of the American Chemical Society 2015, 137, 1581–1586. 59. Yi, T. F.; Yang, S. Y.; Xie, Y. Recent advances of Li4Ti5O12 as a promising next generation anode material for high power lithium-ion batteries. Journal of Materials Chemistry A 2015, 3, 5750–5777. 60. Nair, V. S.; Sreejith, S.; Borah, P.; Hartung, S.; Bucher, N.; Zhao, Y.; Madhavi, S. Crystalline Li3V6O16 rods as high-capacity anode materials for aqueous rechargeable lithium batteries (ARLB). RSC Advances 2014, 4, 28601–28605. 61. Goodenough, J. B.; Kim, Y. Challenges for rechargeable Li batteries. Chemistry of Materials 2010, 22, 587. 62. John B.; Park, G.-S. The Li-ion rechargeable battery: A perspective. Journal of the American Chemical Society 2013, 135(4), 1167–1176. 63. Wu, J.; Fenech, M.; Webster, R. F.; Richard, D.; Sharma, N. Electron microscopy and its role in advanced lithium-ion battery research. Sustainable Energy Fuels 2019, 3, 1623. 64. Wang, D.-Y.; Wei, C.-Y.; Lin, M.-C.; Pan, C.-J.; Chou, H.-L.; Chen, H.-A.; Gong, M.; Wu, Y.-P.; Yuan, C.; Angell, M.; Hsieh, Y.-J.; Chen, Y.-H.; Wen, C.-Y.; Chen, C.-W.; Hwang, B.-J.; Chen, C.-C.; Dai, H. Advanced rechargeable aluminium ion battery with a high-quality natural graphite cathode. Nature Communications 2017, 8, 14283. 65. Leisegang, T.; Meutzner, F.; Zschornak, M.; Munchgesang, W.; Schmid, R.; Nestler, T.; Meyer, D. C. The aluminum-ion battery: A sustainable and seminal concept? Frontiers in Chemistry 2019, 7, 268. 66. Rani, J. V.; Kanakaiah, V.; Dadmal, T.; Rao, M. S.; Bhavanarushi, S. Fluorinated natural graphite cathode for rechargeable ionic liquid-based aluminum-ion battery. Journal of the Electrochemical Society 2013, 160, A1781–A1784.
Open Issues and Potential Applications
67. Ramaprabhu, S.; Samantaray, S. S. A room temperature multivalent rechargeable Iron ion battery with ether-based electrolyte: New type of post-lithium ion battery. Chemical Communications 2019, 55, 10416–10419. 68. Kuganathan, N.; Iyngaran, P.; Chroneos, A. Lithium diffusion in Li5FePO4. Scientific Report 2018, 8, 5832. 69. Okumura, T.; Shikano, M.; Kobayashi, H. Effect of bulk and surface structural changes in Li5FeO4 positive electrodes during first charging on subsequent lithium-ion battery performance. Journal of Materials Chemistry A 2014, 2, 11847–11856. 70. Zhu, J.; Zu, W.; Yang, G.; Song, Q. A novel electrochemical supercapacitor based on Li4Ti5O12 and LiNi/Co/Mn/O2. Materials Letters 2014, 115, 237–240. 71. Thackeray, M. M.; Kang, S. H.; Johnson, C. S.; Vaughey, J. T.; Benedek, R.; Hackney, S. A. Li2MnO3-stabilized LiMO2 (M = Mn, Ni, Co) electrodes for lithium-ion batteries. Journal of Materials Chemistry A 2007, 17, 3112–3125. 72. Samin, A.; Kurth, M.; Cao, L. Ab initio study of radiation effects on the Li4Ti5O12 electrode used in lithium-ion batteries. AIP Advances 2015, 5, 047110. 73. Laubach, S.; Laubach, S.; Schmidt, P. C.; Ensling, D.; Schmid, S.; Jaegermann, W.; Thißen, A.; Nikolowski, K.; Ehrenberg, H. Changes in the crystal and electronic structure of LiCoO2 and LiNiO2 upon Li intercalation and deintercalation. Physical Chemistry Chemical Physics 2009, 11(17), 3278. 74. Ensling, D.; Cherkashinin, G.; Schmid, S.; Bhuvaneswari, S.; Thissen, A.; Jaegermann, W. Nonrigid band behavior of the electronic structure of LiCoO2 thin film during electrochemical Li deintercalation. Chemistry of Materials 2014, 26(13), 3948–3956. 75. Kim, T.; Song, W.; Son, D.-Y.; Ono, L. K.; Qi, Y. Lithium-ion batteries: Outlook on present, future, and hybridized technologies. Journal of Materials Chemistry A 2019, 7, 2942. 76. Lin, M.-C.; Gong, M.; Lu, B.; Wu, Y.; Wang, D.-Y.; Guan, M.; Dai, H. An ultrafast rechargeable aluminium-ion battery. Nature 2015, 520(7547), 324–328. 77. Das, S. K.; Mahapatra, S.; Lahan, H. Aluminium-ion batteries: Developments and challenges. Journal of Materials Chemistry A 2017, 5(14), 6347–6367. 78. Fallahzadeh, R.; Farhadian, N. Molecular dynamics simulation of lithium ion diffusion in LiCoO2 cathode material. Solid State Ionics 2015, 280, 10–17. 79. Wu, X.; Song, K.; Zhang, X.; Hu, N.; Li, L.; Li, W.; Zhang, H. Safety issues in lithium ion batteries: Materials and cell design. Frontiers in Energy Research 2019, 7, 65. 80. Balke, N.; Jesse, S.; Morozovska, A. N.; Eliseev, E.; Chung, D. W.; Kim, Y.; Kalinin, S. V. Nanoscale mapping of ion diffusion in a lithium-ion battery cathode. Nature Nanotechnology 2010, 5(10), 749–754. 81. Macedo, L. J. A.; Lima, F. C. D. A.; Amorim, R. G.; Freitas, R. O.; Yadav, A.; Iost, R. M.; Crespilho, F. N. Interplay of non-uniform charge distribution on the electrochemical modification of graphene. Nanoscale 2018, 10(31), 15048–15057. 82. Gauthier, M.; Carney, T. J.; Grimaud, A.; Giordano, L.; Pour, N.; Chang, H.-H.; Shao-Horn, Y. Electrode-electrolyte interface in Li-ion batteries: Current understanding and new insights. The Journal of Physical Chemistry Letters 2015, 6(22), 4653–4672. 83. Sun, P.; Ma, R.; Ma, W.; Wu, J.; Wang, K.; Sasaki, T.; Zhu, H. Highly selective chargeguided ion transport through a hybrid membrane consisting of anionic graphene oxide and cationic hydroxide nanosheet superlattice units. NPG Asia Materials 2016, 8(4), e259–e259. 84. Ji, H.; Urban, A.; Kitchaev, D. A.; Kwon, D.-H.; Artrith, N.; Ophus, C.; Ceder, G. Hidden structural and chemical order controls lithium transport in cation-disordered oxides for rechargeable batteries. Nature Communications 2019, 10(1), 592. 85. Morimoto, T.; Nagai, M.; Minowa, Y.; Ashida, M.; Yokotani, Y.; Okuyama, Y.; Kani, Y. Microscopic ion migration in solid electrolytes revealed by terahertz time-domain spectroscopy. Nature Communications 2019, 10(1), 2662.
Lithium-Ion Batteries and Solar Cells
86. Fitzhugh, W.; Ye, L.; Li, X. The effects of mechanical constriction on the operation of sulfide based solid-state batteries. Journal of Materials Chemistry A 2019, 7, 23604–23627. 87. Zhu, X.; Ong, C. S.; Xu, X.; Hu, B.; Shang, J.; Yang, H.; Li, R.-W. Direct observation of lithium-ion transport under an electrical field in LixCoO2 nanograins. Scientific Reports 2013, 3(1), 1084. 88. Zhang, L.; Gong, T.; Wang, H.; Guo, Z.; Zhang, H. Memristive devices based on emerging two-dimensional materials beyond graphene. Nanoscale 2019, 11(26), 12413–12435. 89. Liu, J.; Song, K.; Zhu, C.; Chen, C.-C.; van Aken, P. A.; Maier, J.; Yu, Y. Ge/C nanowires as high-capacity and long-life anode materials for Li-ion batteries. ACS Nano 2014, 8(7), 7051–7059. 90. Iijima, S. Synthesis of carbon nanotubes. Nature 1991, 354, 56–58. 91. Zhang, M.; Li, J. Carbon nanotube in different shapes. Materials Today 2009, 12(6), 12–18. 92. Liu, C.; Cheng, H.-M. Carbon nanotubes: Controlled growth and application. Materials Today 2013, 16(1–2), 19–28. 93. Marganska, M.; Schmid, D. R.; Dirnaichner, A.; Stiller, P. L.; Strunk, C.; Grifoni, M.; Huttel, A. K. Shaping electron wave functions in a carbon nanotube with a parallel magnetic field. Physical Review Letters 2019, 122(8), 086802. 94. Odom, T. W.; Huang, J.-L.; Kim, P.; Ouyang, M.; Lieber, C. M. Scanning tunneling microscopy and spectroscopy studies of single wall carbon nanotubes. Journal of Materials Research 1998, 13(9), 2380–2388. 95. Meunier, V.; Lambin, P. Scanning tunneling microscopy and spectroscopy of topological defects in carbon nanotubes. Carbon 2000, 38(11–12), 1729–1733. 96. Giusca, C. E.; Tison, Y.; Silva, S. R. P. Inter-layer interaction in double-walled carbon nanotubes evidenced by scanning tunneling microscopy and spectroscopy. Nano 2008, 3(2), 65–73. 97. Boumia, L.; Zidour, M.; Benzair, A.; Tounsi, A. A Timoshenko beam model for vibration analysis of chiral single-walled carbon nanotubes. Physica E: Low-Dimensional Systems and Nanostructures 2014, 59, 186–191. 98. MacFarlane, W.; Chakhalian, J.; Kie, R.; Dunsiger, S.; Miller, R.; Sonier, J.; Fischer, J. A SR study of single-walled carbon nanotubes. Physica B: Condensed Matter 2000, 289–290, 589–593. 99. Liu, B.; Wu, F.; Gui, H.; Zheng, M.; Zhou, C. Chirality-controlled synthesis and applications of single-wall carbon nanotubes. ACS Nano 2017, 11(1), 31–53. 100. Wu, B.; Geng, D.; Liu, Y. Evaluation of metallic and semiconducting single-walled carbon nanotube characteristics. Nanoscale 2011, 3(5), 2074. 101. Pillai, S. K.; Ray, S. S.; Moodley, M. Purification of multi-walled carbon nanotubes. Journal of Nanoscience and Nanotechnology 2008, 8(12), 6187–6207. 102. Eatemadi, A.; Daraee, H.; Karimkhanloo, H.; Kouhi, M.; Zarghami, N.; Akbarzadeh, A.; Abasi, M.; Hanifehpour, Y.; Joo, S. Carbon nanotubes: Properties, synthesis, purification, and medical applications. Nanoscale Research Letters 2014, 9(1), 393. 103. Pillewan, V. J.; Raut, D. N.; Patil, K. N.; Shinde, D. K. Carbon to carbon nanotubes synthesis process: An experimental and numerical study. Materials Today: Proceedings 2018, 5(2), 6444–6452. 104. Zhang, Z.; Mu, S.; Zhang, B.; Tao, L.; Huang, S.; Huang, Y.; Zhao, Y. A novel synthesis of carbon nanotubes directly from an indecomposable solid carbon source for electrochemical applications. Journal of Materials Chemistry A 2016, 4(6), 2137–2146. 105. Kanemitsu, Y. Excitons in semiconducting carbon nanotubes: Diameter-dependent photoluminescence spectra. Physical Chemistry Chemical Physics 2011, 13(33), 14879. 106. Velizhanin, K. A. Exciton relaxation in carbon nanotubes via electronic-to-vibrational energy transfer. The Journal of Chemical Physics 2019, 151(14), 144703.
Open Issues and Potential Applications
107. Chacon-Torres, J. C.; Dzsaber, S.; Vega-Diaz, S. M.; Akbarzadeh, J.; Peterlik, H.; Kotakoski, J.; Reich, S. Potassium intercalated multiwalled carbon nanotubes. Carbon 2016, 105, 90–95. 108. Chakrapani, N.; Zhang, Y. M.; Nayak, S. K.; Moore, J. A.; Carroll, D. L.; Choi, Y. Y.; Ajayan, P. M. Chemisorption of acetone on carbon nanotubes. The Journal of Physical Chemistry B 2003, 107(35), 9308–9311. 109. Sankaran, M.; Viswanathan, B. Hydrogen storage in boron substituted carbon nanotubes. Carbon 2007, 45(8), 1628–1635. 110. Bai, J.; Zeng, X. C.; Tanaka, H.; Zeng, J. Y. Metallic single-walled silicon nanotubes. Proceedings of the National Academy of Sciences 2004, 101(9), 2664–2668. 111. Li, X.; Meng, G.; Xu, Q.; Kong, M.; Zhu, X.; Chu, Z.; Li, A.-P. Controlled synthesis of germanium nanowires and nanotubes with variable morphologies and sizes. Nano Letters 2011, 11(4), 1704–1709. 112. Khalilov, U.; Bogaerts, A.; Neyts, E. C. Atomic scale simulation of carbon nanotube nucleation from hydrocarbon precursors. Nature Communications 2015, 6(1), 10306. 113. Carreon, M. L.; Thapa, A. K.; Jasinski, J. B.; Sunkara, M. K. The capacity and durability of amorphous silicon nanotube thin film anode for lithium ion battery applications. ECS Electrochemistry Letters 2015, 4(10), A124–A128. 114. Casiello, M.; Picca, R.; Fusco, C.; D’Accolti, L.; Leonardi, A.; Lo Faro, M.; Nacci, A. Catalytic activity of silicon nanowires decorated with gold and copper nanoparticles deposited by pulsed laser ablation. Nanomaterials 2018, 8(2), 78. 115. Tserpes, K. I.; Silvestre, N. Modeling of Carbon Nanotubes, Graphene and Their Composites, 1st Edition, Springer, New York, 2014. 116. Molle, A.; Grazianetti, C.; Tao, L.; Taneja, D.; Alam, M. H.; Akinwande, D. Silicene, silicene derivatives, and their device applications. Chemical Society Reviews 2018, 47(16), 6370–6387. 117. Ezawa, M. Quantum hall effects in silicene. Journal of the Physical Society of Japan 2012, 81(6), 064705. 118. Correa, J. D.; da Silva, A. J. R.; Pacheco, M. Tight-binding model for carbon nanotubes from ab initio calculations. Journal of Physics: Condensed Matter 2010, 22(27), 275503. 119. Zhang, R. Q.; Lee, H.-L.; Li, W.-K.; Teo, B. K. Investigation of possible structures of silicon nanotubes via density-functional tight-binding molecular dynamics simulations and ab initio calculations. The Journal of Physical Chemistry B 2005, 109(18), 8605–8612. 120. White, C. T.; Mintmire, J. W. Fundamental properties of single-wall carbon nanotubes. The Journal of Physical Chemistry B 2005, 109, 1, 52–65. 121. Ezawa, M. Dirac theory and topological phases of silicon nanotube. Europhysics Letters 2012, 98(6), 67001. 122. Ahmadi, N.; Shokri, A. A.; Elahi, S. M. Optical transition of zigzag silicon nanotubes under intrinsic curvature effect. Silicon 2015, 8(2), 217–224. 123. Chen, J.; Liu, M.; Sun, J.; Xu, F. Templated magnesiothermic synthesis of silicon nanotube bundles and their electrochemical performances in lithium ion batteries. RSC Advances 2014, 4(77), 40951–40957. 124. Chitsazan, A.; Monajjemi, M.; Aghaei, H.; Sayadian, M. Neutral gases adsorption with hydrogen on silicon nanotubes: A fuel cell investigation. Oriental Journal of Chemistry 2017, 33(3), 1366–1374. 125. Yan, Y.; Miao, J.; Yang, Z.; Xiao, F.-X.; Yang, H. B.; Liu, B., Yang, Y. Carbon nanotube catalysts: Recent advances in synthesis, characterization and applications. Chemical Society Reviews 2015, 44(10), 3295–3346. 126. Lan, J.; Cheng, D.; Cao, D.; Wang, W. Silicon nanotube as a promising candidate for hydrogen storage: From the first principle calculations to grand canonical Monte Carlo simulations. The Journal of Physical Chemistry C 2008, 112(14), 5598–5604.
Lithium-Ion Batteries and Solar Cells
127. Khalili, S.; Asghar, A.; Ghoreyshi; Jahanshahi, M. Carbon dioxide captured by multiwalled carbon nanotube and activated charcoal: A comparative study. Chemical Industry & Chemical Engineering Quarterly 2013, 19(1), 153–164. 128. Gao, W.; Kono, J. Science and applications of wafer-scale crystalline carbon nanotube films prepared through controlled vacuum filtration. Royal Society Open Science 2019, 6(3), 181605. 129. Grabowski, K.; Zbyrad, P.; Uhl, T.; Staszewski, W. J.; Packo, P. Multiscale electromechanical modeling of carbon nanotube composites. Computational Materials Science 2017, 135, 169–180. 130. Fathi, D. A review of electronic band structure of graphene and carbon nanotubes using tight binding. Journal of Nanotechnology 2011, 2011, 1–6. 131. Yue, L.; Ma, J.; Zhang, J.; Zhao, J.; Dong, S., Liu, Z.; Chen, L. All solid-state polymer electrolytes for high-performance lithium ion batteries. Energy Storage Materials 2016, 5, 139–164. 132. Kim, J. G.; Son, B.; Mukherjee, S.; Schuppert, N.; Bates, A.; Kwon, O.; Park, S. A review of lithium and non-lithium based solid state batteries. Journal of Power Sources 2015, 282, 299–322. 133. Li, J.; Ma, C.; Chi, M.; Liang, C.; Dudney, N. J. Solid electrolyte: The key for high‐voltage lithium batteries. Advanced Energy Materials 2015, 5(4), 1401408. 134. Zheng, J. Q.; Li, Y. F.; Yang, R.; Li, G; Ding, X. K. Lithium ion conductivity in the solid electrolytes (Li0.25La0.25)1−xM0.5xNbO3 (M = Sr, Ba, Ca, x = 0.125) with perovskite-type structure. Ceramics International 2017, 43(2), 1716–1721. 135. Kim, H. S.; Oh, Y.; Kang, K. H.; Kim, J. H.; Kim, J.; Yoon, C. S. Characterization of sputter-deposited LiCoO2 thin film grown on NASICON-type electrolyte for application in all-solid-state rechargeable lithium battery. ACS Applied Materials and Interfaces 2017, 9(19), 16063–16070. 136. Han, F.; Zhu, Y.; He, X.; Mo, Y.; Wang, C. Electrochemical stability of Li10GeP2S12 and Li7La3Zr2O12 solid electrolytes. Advanced Energy Materials 2016, 6(8), 1501590. 137. Deng, Y.; Eames, C.; Fleutot, B.; David, R.; Chotard, J. N., Suard, E.; Islam, M. S. Enhancing the lithium ion conductivity in lithium superionic conductor (LISICON) solid electrolytes through a mixed polyanion effect. ACS Applied Materials Interfaces 2017, 9(8), 7050–7058. 138. Tron, A., Nosenko, A., Park, Y. D.; Mun, J. Synthesis of the solid electrolyte Li2O-LiFP2O5 and its application for lithium-ion batteries. Solid State Ionics 2017, 308, 40–45. 139. Liu, D.; Zhu, W.; Feng, Z.; Guerfi, A.; Vijh, A.; Zaghib, K. Recent progress in sulfidebased solid electrolytes for Li-ion batteries. Materials Science and Engineering: B 2016, 213, 169–176. 140. Tarhouchi, I.; Viallet, V.; Vinatier, P.; Ménétrier, M. Electrochemical characterization of Li10SnP2S12: An electrolyte or a negative electrode for solid state Li-ion batteries? Solid State Ionics 2016, 296, 18–25. 141. Le Van-Jodin, L.; Claudel, A.; Secouard, C.; Sabary, F.; Barnes, J. P.; Martin, S. Role of the chemical composition and structure on the electrical properties of a solid-state electrolyte: Case of a highly conductive LiPON. Electrochimica Acta 2018, 259, 742–751. 142. Xu, R. C.; Xia, X. H.; Yao, Z. J.; Wang, X. L.; Gu, C. D.; Tu, J. P. (2016). Preparation of Li7P3S11 glass-ceramic electrolyte by dissolution-evaporation method for all-solid-state lithium ion batteries. Electrochimica Acta 2016, 219, 235–240. 143. Meesala, Y. Recent advancements in Li-ion conductors for all-solid-state Li-ion batteries. ACS Energy Letters 2017, 2(12), 2734–2751. 144. Larraz, G.; Orera, A.; Sanjuan, M. L. Cubic phases of garnet-type Li7La3Zr2O12: The role of hydration. Journal of Materials Chemistry A 2013, 1(37), 11419–11428. 145. Jayaprakash, N.; Das, S. K.; Archer, L. A. The rechargeable aluminum-ion battery. Chemical Communications 2011, 47, 12610–12612.
Open Issues and Potential Applications
146. Yang, Z.; Zhang, J.; Kintner-Meyer, M. C. W.; Lu, X., Choi, D; Lemon, J. P.; Liu, J. Electrochemical energy storage for green grid. Chemical Reviews 2011, 111(5), 3577–3613. 147. Hudak, N. S. Chloroaluminate-doped conducting polymers as positive electrodes in rechargeable aluminum batteries. The Journal of Physical Chemistry C 2014, 118(10), 5203–5215. 148. Li, Z.; Xiang, K.; Xing, W.; Carter, W. C.; Chiang, Y. Reversible aluminum-ion intercalation in Prussian blue analogs and demonstration of a high-power aluminum-ion asymmetric capacitor. Advanced Energy Materials 2015, 5, 1401410. 149. Wang, H. L.; Gu, S. C.; Bai, Y.; Chen, S.; Wu, F.; Wu, C. High-voltage and noncorrosive ionic liquid electrolyte used in rechargeable aluminum battery. ACS Applied Materials & Interfaces 2016, 8, 27444–27448. 150. Wang, H. L.; Gu, S. C.; Bai, Y.; Chen, S.; Zhu, N.; Wu, F.; Wu, C. Anion-effects on electrochemical properties of ionic liquid electrolytes for rechargeable aluminum batteries. Journal of Materials Chemistry A 2015, 3, 22677–22686. 151. Sun, H.; Wang, W.; Yu, Z.; Yuan, Y.; Wang, S.; Jiao, S. A new aluminium-ion battery with high voltage, high safety and low cost. Chemical Communications 2015, 51(59), 11892–11895. 152. Jiao, H.; Wang, C.; Tu, J.; Tian, D.; Jiao, S. A rechargeable Al-ion battery: Al/molten AlCl3-urea/graphite. Chemical Communications 2017, 53, 2331–2334. 153. Zhang, Y. U.; Liu S.; Ji, Y., Ma, J.; Yu, H. Emerging nonaqueous aluminum-ion batteries: Challenges, status, and perspectives. Advanced Materials 2018, 30, 17063. 154. Li, Z.; Niu, B.; Liu, J.; Li, J.; Kang, F. Rechargeable aluminum-ion battery based on MoS2 microsphere cathode. ACS Applied Materials & Interfaces 2018, 10(11), 9451–9459. 155. Chen, J.; Kuriyama, N.; Yuan, H.; Takeshita, H. T.; Sakai, T. Electrochemical hydrogen storage in MoS2 nanotubes. Journal of the American Chemical Society 2001, 123, 11813–11814. 156. Nestler, T.; Fedotov, S.; Leisegang, T.; Meyer, D. C. Towards Al3+ mobility in crystalline solids: Critical review and analysis. Critical Reviews in Solid State and Materials Sciences 2019, 44(4), 298–323. 157. Wang, H.; Gu, S.; Bai, Y.; Chen, S.; Zhu, N.; Wu, C.; Wu, F. Anion-effects on electrochemical properties of ionic liquid electrolytes for rechargeable aluminum batteries. Journal of Materials Chemistry A 2015, 3(45), 22677–22686. 158. Elia, G. A.; Marquardt, K.; Hoeppner, K.; Fantini, S.; Lin, R.; Knipping, E.; Peters, W.; Drillet, J. F.; Passerini, S.; Hahn, R. An overview and future perspectives of aluminum batteries. Advanced Materials 2016, 28(35), 7564–7579. 159. Zafar, Z. A.; Imtiaz, S.; Razaq, R.; Ji, S.; Huang, T.; Zhang, Z. Cathode materials for rechargeable aluminum batteries: Current status and progress. Journal of Materials Chemistry A 2017, 5, 5646–5660. 160. Liu, C.; Neale, Z. G.; Cao, G. Understanding electrochemical potentials of cathode materials in rechargeable batteries. Materials Today 2016, 19(2), 109–123. 161. Gu, S. C.; Wang, H. L.; Wu, C.; Bai, Y.; Li, H.; Wu, F. Confirming reversible Al3+ storage mechanism through intercalation of Al3+ into V2O5 nanowires in a rechargeable aluminum battery. Energy Storage Materials 2017, 6, 9–17. 162. Yue, Y.; Liang, H. Micro- and nano-structured vanadium pentoxide (V2O5) for electrodes of lithium-ion batteries. Advanced Energy Materials 2017, 7, 1–32.
Problems Thi Dieu Hien Nguyen, Ngoc Thanh Thuy Tran, and Ming-Fa Lin National Cheng Kung University
CONTENT References .............................................................................................................. 283 The featured physical, chemical, and material properties could be solved by the firstprinciples method (the VASP calculations) and the phenomenological model (the tight-binding model). 1. Exploring the low-lying band structure for a monolayer graphene (Figure 16.1a: ) by the tight-binding model under the carbon-2pz orbital bondings. Determine (a) a primitive unit cell and two lattice vectors, (b) the first Brillouin zone and two reciprocal lattice vectors, (c) a 2 × 2 Hamiltonian matrix, (d) valence and conduction energy dispersions, and (e) wave-vectordependent wave functions. 2. The similar calculations, as revealed in problems 1(a)–1(e), applied for a monolayer silicene/germanene with buckling in A and B sublattices (Figure 16.1b; [2–5]). Here, the spin-orbital coupling plays a critical role in the electronic properties through the 4 × 4 Hamiltonian matrix. (f) The gatevoltage effects, being induced a uniform perpendicular electric field, could be achieved by changing its diagonal matrix elements. (g) A detailed comparison is also made between grapheme and silicene.
FIGURE 16.1 The geometric structures for monolayer: (a) graphene and silicene with the (b)/(c) top/side view. 279
Lithium-Ion Batteries and Solar Cells
3. The above-mentioned phenomenological model is suitable for studying the electronic properties of AA-, AB-, and ABC-stacked graphites [6–13], in which the second system serves as the anode material of lithium-ion-based batteries. Thoroughly investigate (a) their primitive unit cells under the different stacking configurations, (b) the distinct overlaps in valence and conduction bands, (c) the different densities of states across the Fermi level, (d) the existence of Dirac-cone structures, and (e) the important differences between 3D and 2D layered honeycomb lattices. 4. The rich and unique magnetic quantization in monolayer graphene and bulk graphites through the generalized tight-binding model . The vector potential, being created by a uniform perpendicular magnetic field, leads to the periodical Peierls phases, and thus an extra magnetic-field-dependent period characterizes/evaluates/discusses (a) an enlarged magnetic unit cell, (b) the modifications on the intralayer and interlayer hopping integrals of the Hamiltonian matrix elements, (c) the Landau levels/sub-bands in 2D/3D systems, (d) the localized magnetic wave functions, and (e) the dimensionand stacking-diversified phenomena . 5. The generalized tight-binding model is also reliable for the electronic and magneto-electronic properties of the AAA-[14,15], ABA-[14,16,17], ABC[14,17,18], and AAB-stacked [14,19] trilayer graphene systems (Figure 16.2). Fully explore (a) the low-energy features in terms of energy dispersions, band overlaps, and electron and hole energy spectra, (b) the diverse van Hove singularities of density of states, (c) the unusual Landau levels with the high degeneracy, (d) the normal or irregular magnetic wave functions with the well-behaved or undefined modes, (e) the abnormal anti-crossing behaviors in the field-induced energy spectra, and (f) the combined effects due to the perpendicular magnetic and electric fields. 6. The VASP calculations for studying the lithium-based battery anode materials of the 1D silicene/germanene nanotubes [20–24]. Delicately identify/characterize/calculate (a) the arm-chair, zigzag, and chiral hexagon arrangement on a hollow cylinder with the buckled A and B sublattices, (b) angular-momentum-decoupled band structures under the periodical boundary condition, (c) the standing waves along the azimuthal direction, (d) the critical roles of orbital hybridizations on a cylindrical surface, and (e) the radius- and chiral-angle-dependent band gaps and compare (f) the significant similarities and differences between silicene and germanene nanotubes. 7. Using the first-principles method to fully investigate the quantum-confinement effects in 1D silicene/germanene nanoribbons in the presence or absence of hydrogen passivation [25–27]. Define/evaluate/illustrate (a) the armchair, zigzag, and chiral open edges, (b) the modulated bond lengths near two boundaries, (c) the feature band structures with the transverse translation symmetry, (d) the unique wave functions under the open boundary condition, (e) the strong dependences of energy gaps on the spin-orbital coupling, buckled structure, edge structure, and ribbon widths, (f) the rich chemical bondings from the spatial charge density distributions, (g) the
multi-orbital hybridizations through the atom- and orbital-decomposed van Hove singularities of density of states, and (h) the dimensionality-enriched phenomena. Intercalations/de-intercalations of Li + /AlCl −4 /Al 2 Cl 7− into/from the interlayer spacings of graphitic sheets, serving as the anode or cathode materials in the lithium-/aluminum-ion-based batteries [28–31]. The delicate VASP calculations and analyses on graphite intercalation ion compounds are able to provide (a) the diverse geometric symmetries, (b) the semimetallic or metallic behaviors, (c) the spin-degenerate or spin-split energy bands near the Fermi level, (d) the chemical bonding strengths of carbon-ion bonds from the spatial charge density distributions, (e) the existence of ferromagnetic spin configurations related to the anions, and (f) the minor or major modifications after the cation or anion intercalations. The 3D binary V2O5 could be utilized as the cathode material of iron-ionbased batteries . Its rich properties of vanadium pentoxide will be clearly revealed under the first-principles calculations: (a) the crystal symmetry with or without the modulation of bond length, (b) the band gap of semiconductor, (c) the existence of the vanadium-induced spin configuration, (d) the multi-orbital hybridizations in V–O chemical bonds and their drastic changes after certain substitutions of vanadium by iron (or the important differences between binary and ternary compounds). The 3D LiFeO2 and LiFePO4 materials are used as cathodes in lithium-ionbased batteries [33–36]. The VASP numerical simulations are capable of identifying (a) the extremely nonuniform physical and chemical environments (e.g., the great modulation of bond lengths), (b) the strong three-/fouratom dependences for each energy band, (c) the multi-orbital hybridization in Li–O, Fe–O, and P–O bonds from the significant overlaps in the spatial charge density distributions, (d) the atom-dominated energy ranges due to the different strengths of van Hove singularities, (e) the atom- and orbitaldecomposed magnetic moments, (f) the spin-split energy band close to the Fermi level, (g) the ferromagnetic metals or semiconductors, (h) the ferromagnetic spin density arrangements around Li, Fe, P, and O atoms, and (i) the enhanced battery functionalities after the dramatic transformation from three into four components. The 3D ternary LiGe/SnO compounds are used as electrolytes in lithiumion-based batteries [37–39]. The VASP numerical simulations could calculate/examine/illustrate (a) the highly anisotropic chemical environments in the presence of various chemical bonds, (b) the strong correlations of Li–O and Ge–/Sn–O bonds from the atom-dominated valence and conduction bands, (c) the different contributions of oxygen orbitals from the spatial charge densities and van Hove singularities, and (d) the important differences or similarities among LiGeO, LiSnO, and LiSiO (details in Chapter 5) compounds. The unusual essential properties in binary 3D silicon carbide (SiC; [40,41]). The diverse phenomena are created by the different silicon/carbon concentrations and dimensionalities. The VASP calculations are mainly focused on
Lithium-Ion Batteries and Solar Cells
FIGURE 16.2 The geometric structures of the (a) AAA-, (b) ABA-, (c) ABC-, and (d) AABstacked trilayer graphene systems.
(a) the modulated chemical bonds, (b) band gaps, (c) featured energy spectra/wave functions, (d) atom- and orbital-generated charge densities, (e) concise multi-orbital hybridizations, (f) distinct special structures of van Hove singularities, and (g) significant differences among 3D, 2D (honeycomb lattices; ), and 1D (nanotubes and nanoribbons; [43–46]) compounds. 13. The rich and unique phenomena in 3D silicon/germanium/diamond [47–51]. Concerning mono-element crystals, the delicate VASP simulations are thoroughly made on (a) the symmetric geometries with the sp3 chemical
bondings, (b) the atom- and orbital-diversified energy bands, (c) the unusual charge density distributions, (d) the different van Hove singularities, and (e) the similarities and differences among three kinds of materials, especially for the significant effects being induced by the spin-orbital couplings. Also, a detailed comparison is made for the first-principles method and the tightbinding model in terms of the essential properties , such as the hole bands nearest to the Fermi level. 14. The exact identification of multi-orbital hybridizations in 3D SiO2 . This material frequently serves as a very stable substrate; therefore, its intrinsic properties play a critical role in the crystal growth. The first-principles simulations will examine/solve/identify the optimal crystal structure, (b) the distinct Si–, O– or (Si, O)-dominated energy ranges, the highly anisotropic charge density distribution associated with the strong chemical bondings, and (d) the concise orbital hybridizations from the atom- and orbital-projected density of states. Very interestingly, (e) geometric structures and (f) electronic properties are significantly diversified by the two- and threecomponent compounds, respectively, corresponding to SiO2 and LiSiO2 [54–56]. 15. The VASP calculations are very suitable for the rich properties of 3D binary iron/cobalt/nickel oxide compounds : (a) the distinct bond lengths and ground state energies, (b) the atom- and orbital-created magnetic moments, (c) the atom- and spin-dependent energy bands, the different spin densities around transition metal and oxygen atoms, (e) the multi-orbital overlaps in charge density distributions, and (f) the atom-, orbital-, and spin-dominated energy ranges. Such characteristics are dramatically changed under the transformation from binary materials into ternary ones (lithium transition metal oxide compounds; problem 10).
REFERENCES 1. Torbatian, Z.; Asgari, R. Plasmonic physics of 2D crystalline materials. Applied Sciences 2018, 8(2), 238. 2. Roome, N. J.; Carey, J. D. Beyond graphene: Stable elemental monolayers of silicene and germanene. ACS Applied Materials & Interfaces 2014, 6(10), 7743–7750. 3. Ye, X.; Shao, Z.; Zhao, H.; Yang, L.; Wang, C. Intrinsic carrier mobility of germanene is larger than graphene’s: First-principle calculations. RSC Advances 2014, 4, 21216–21220. 4. Dimoulas, A. Silicene and germanene: Silicon and germanium in the “flatland”. Microelectronic Engineering 2015, 131, 68–78. 5. Ezawa, M. Monolayer topological insulators: Silicene, germanene, and stanene. Journal of the Physical Society of Japan 2015, 84(12), 121003. 6. Chuang, Y. C.; Wu, J. Y.; Lin, M. F. Analytical calculations on low-frequency excitations in AA-stacked bilayer graphene. Journal of Physical Society Japan 2012, 81, 124713. 7. Lin, M. F.; Chuang, Y. C.; Wu, J. Y. Electrically tunable plasma excitations in AA-stacked multilayer graphene. Physics Review B 2012, 86, 125434. 8. Chuang, Y. C.; Wu, J. Y.; Lin, M. F. Electric-field-induced plasmon in AA-stacked bilayer graphene. Annals of Physics 2013, 339, 298.
Lithium-Ion Batteries and Solar Cells
9. Ho, J. H.; Lu, C. L.; Hwang, C. C.; Chang, C. P.; Lin, M. F. Coulomb excitations in AAand AB-stacked bilayer graphites. Physics Review B 2006, 74, 085406. 10. Chuang, Y. C.; Wu, J. Y.; Lin, M. F. Electric field dependence of excitation spectra in AB-stacked bilayer graphene. Scientific Reports 2013, 3, 1368. 11. Sugawara, K.; Yamamura, N.; Matsuda, K.; Norimatsu, W.; Kusunoki, M.; Sato, T.; Takahashi, T. Selective fabrication of free-standing ABA and ABC trilayer graphene with/without Dirac-cone energy bands. NPG Asia Materials 2018, 10(2), e466. 12. Shan, Y.; Li, Y.; Huang, D.; Tong, Q.; Yao, W.; Liu, W.-T.; Wu, S. Stacking symmetry governed second harmonic generation in graphene trilayers. Science Advances 2018, 4(6), eaat0074. 13. Yelgel, C. Electronic structure of ABC-stacked multilayer graphene and trigonal warping: A first principles calculation. Journal of Physics 2016, 707, 012022. 14. Lin, C.-Y.; Wu, J.-Y.; Ou, Y.-J.; Chiu, Y.-H.; Lin, M.-F. Magneto-electronic properties of multilayer graphenes. Physical Chemistry Chemical Physics 2015, 17(39), 26008–26035. 15. Redouani, I.; Jellal, A.; Bahaoui, A.; Bahlouli, H. Multibands tunneling in AAAstacked trilayer graphene. Superlattices and Microstructures 2018, 116, 44–53. 16. Lin, C.-Y.; Wu, J.-Y.; Chiu, Y.-H.; Chang, C.-P.; Lin, M.-F. Stacking-dependent magnetoelectronic properties in multilayer graphene. Physical Review B 2014, 90, 205434–205444. 17. Van Duppen, B.; Sena, S. H. R.; Peeters, F. M. Multiband tunneling in trilayer graphene. Physical Review B 2013, 87(19), 195439(10). 18. Lin, Y.-P.; Lin, C.-Y.; Ho, Y.-H.; Do, T.-N.; Lin, M.-F. Magneto-optical properties of ABC-stacked trilayer graphene. Physical Chemistry Chemical Physics 2015, 17(24), 15921–15927. 19. Do, T.-N.; Shih, P.-H.; Chang, C.-P.; Lin, C.-Y.; Lin, M.-F. Rich magneto-absorption spectra of AAB-stacked trilayer graphene. Physical Chemistry Chemical Physics 2016, 18(26), 17597–17605. 20. Ezawa, M. Dirac theory and topological phases of silicon nanotube. Europhysics Letters 2012, 98(6), 67001. 21. Lima, M. P. Double-walled silicon nanotubes: An ab initio investigation. Nanotechnology 2018, 29(7), 075703. 22. Zhang, R. Q.; Lee, S. T.; Law, C.-K., Li, W.-K. and Teo, B. K. Silicon nanotubes: Why not? Chemical Physics Letters 2002, 364, 251–258. 23. Srimathi, U.; Nagarajan, V.; Chandiramouli, R. Adsorption studies of volatile organic compounds on germanene nanotube emitted from banana fruit for quality assessment-A density functional application. Journal of Molecular Graphics and Modelling 2018, 82, 129–136. 24. Snehha, P.; Nagarajan, V.; Chandiramouli, R. Germanene nanotube electroresistive molecular device for detection of NO2 and SO2 gas molecules: A first-principles investigation. Journal of Computational Electronics 2018, 18(40), 308–318. 25. Monshi, M. M.; Aghaei, S. M.; Calizo, I. Edge functionalized germanene nanoribbons: Impact on electronic and magnetic properties. RSC Advances 2017, 7(31), 18900–18908. 26. Yagmurcukardes, M.; Peeters, F. M.; Senger, R. T.; Sahin, H. Nanoribbons: From fundamentals to state-of-the-art applications. Applied Physics Reviews 2016, 3(4), 041302. 27. Mehdi Aghaei, S.; Calizo, I. Band gap tuning of armchair silicene nanoribbons using periodic hexagonal holes. Journal of Applied Physics 2015, 118(10), 104304. 28. Abe, T.; Sagane, F.; Ohtsuka, M.; Iriyama, Y.; Ogumi, Z. Lithium-ion transfer at the interface between lithium-ion conductive ceramic electrolyte and liquid electrolyte – A key to enhancing the rate capability of lithium-ion batteries. Journal of the Electrochemical Society 2005, 152(11), A2151.
29. Maruyama, S.; Fukutsuka, T.; Miyazaki, K.; Abe, Y.; Yoshizawa, N.; Abe, T. Lithiumion intercalation and deintercalation behaviors of graphitized carbon nanospheres. Journal of Materials Chemistry A 2018, 6(3), 1128–1137. 30. Das, S. K.; Mahapatra, S.; Lahan, H. Aluminium-ion batteries: Developments and challenges. Journal of Materials Chemistry A 2017, 5(14), 6347–6367. 31. Angell, M.; Pan, C.-J.; Rong, Y.; Yuan, C.; Lin, M.-C.; Hwang, B.-J.; Dai, H. High Coulombic efficiency aluminum-ion battery using an AlCl3-urea ionic liquid analog electrolyte. Proceedings of the National Academy of Sciences 2017, 114(5), 834–839. 32. Ramaprabhu, S.; Samantaray, S. S. A room temperature multivalent rechargeable iron ion battery with ether-based electrolyte: New type of post-lithium ion battery. Chemical Communications 2019, 55, 10416–10419. 33. Li, J.; Luo, J.; Wang, L.; He, X. Recent advances in the LiFeO2-based materials for Li-ion batteries. International Journal of Electrochemical Science 2011, 6(5), 1550–1561. 34. Li, K.; Chen, H.; Shua, F.; Chen, K.; Xue, D. Low temperature synthesis of Fe2O3 and LiFeO2 as cathode materials for lithium-ion batteries. Electrochimica Acta 2014, 136, 10–18. 35. Yuan, L.-X.; Wang, Z.-H.; Zhang, W.-X.; Hu, X.-L.; Chen, J.-T.; Huang, Y.-H.; Goodenough, J. B. Development and challenges of LiFePO4 cathode material for lithium-ion batteries. Energy & Environmental Science 2011, 4(2), 269–284. 36. Guo, K. W. Urgency of LiFePO4 as cathode material for Li-ion batteries. Advances in Materials Research 2015, 4(2), 63–76. 37. Xiao, R.; Li, H.; Chen, L. Candidate structures for inorganic lithium solid-state electrolytes identified by high-throughput bond-valence calculations. Journal of Materiomics 2015, 1(4), 325–332. 38. Zhu, Y.; He, X.-F. Mo, Y.-F. Origin of outstanding stability in the lithium solid electrolyte materials: Insights from thermodynamic analyses based on first principles calculations. ACS Applied Materials & Interfaces 2018, 7, 23685–23693. 39. Park, J. S.; Park, Y. J. Surface modification of a Li[Ni0:8Co0:15Al0:05]O2 cathode using Li2SiO3 solid electrolyte. Journal of Electrochemical Science and Technology 2017, 8(2), 101–106. 40. Kim, K.; Ju, H.; Kim, J. Vertical particle alignment of boron nitride and silicon carbide binary filler system for thermal conductivity enhancement. Composites Science and Technology 2016, 123, 99–105. 41. Fan, Q.; Chai, C., Wei, Q.; Yang, Y. The mechanical and electronic properties of carbon-rich silicon carbide. Materials 2016, 9(5), 333. 42. Milowska, K.; Magdalena Birowska, M.; Majewski, J. A. Mechanical and electrical properties of carbon nanotubes and graphene layers functionalized with amines. Diamond and Related Materials 2012, 23, 167–171. 43. Wu, X.-J.; Pei, Y.; Zeng, X. Z. B2C graphene, nanotubes, and nanoribbons. Nano Letters 2009, 9(4), 1577–1582. 44. Soldano, C.; Talapatra, S.; Kar, S. Carbon nanotubes and graphene nanoribbons: Potentials for nanoscale electrical interconnects. Electronics 2013, 2(4), 280–314. 45. Zheng, W.-T.; Sun, C. Q. Underneath the fascinations of carbon nanotubes and graphene nanoribbons. Energy Environmental Science 2011, 4, 627–655. 46. Hartmann, R. R.; Saroka, V. A.; Portnoi, M. E. Interband transitions in narrow-gap carbon nanotubes and graphene nanoribbons. Journal of Applied Physics 2019, 125(15), 151607. 47. Guo, Y.; Wang, Q.; Kawazoe, Y.; Jena, P. A new silicon phase with direct band gap and novel optoelectronic properties. Scientific Reports 2015, 5(1), 14342. 48. Malone, B. D.; Sau, J. D.; Cohen, M. L. Ab initio survey of the electronic structure of tetrahedrally bonded phases of silicon. Physical Review B 2008, 78, 035210.
Lithium-Ion Batteries and Solar Cells
49. Deinzer, G.; Birner, G.; Strauch, D. Ab initio calculation of the line width of various phonon modes in germanium and silicon. Physical Review B 2003, 67, 144304. 50. Kiefer, F.; Karttunen, A. J.; Doblinger, M.; Fassler, T. F. Bulk synthesis and structure of a microcrystalline allotrope of germanium (m-allo-Ge). Chemistry of Materials 2011, 23, 4578–86. 51. Shenderova, O. A.; Shames, A. I.; Nunn, N. A.; Torelli, M. D.; Vlasov, I.; Zaitsev, A. Review article: Synthesis, properties, and applications of fluorescent diamond particles. Journal of Vacuum Science & Technology B 2019, 37(3), 030802. 52. Zolyomi, V.; Wallbank, J. R.; Fal’ko, V. I. Silicane and germanane: Tight-binding and first-principles studies. 2D Materials 2014, 1(1), 011005. 53. Sciuto, E. L.; Bongiorno, C.; Scandurra, A.; Petralia, S.; Cosentino, T.; Conoci, S.; Libertino, S. Functionalization of bulk SiO2 surface with biomolecules for sensing applications: Structural and functional characterizations. Chemosensors 2018, 6(4), 59. 54. Martin-Samos, L.; Bussi, G.; Ruini, A.; Molinari, E.; Caldas, M. J. SiO2 in density functional theory and beyond. Physica Status Solidi 2010, 248(5), 1061–1066. 55. Zhang, Y.; Li, Y.; Wang, Z.; Zhao, K. Lithiation of SiO2 in Li-ion batteries: In situ transmission electron microscopy experiments and theoretical studies. Nano Letters 2014, 14(12), 7161–7170. 56. Wang, J.-Q.; Kang, H.-L.; Zhang, Y. Simulation calculation and analysis of electronic structure and electrical properties of metal-doped SnO2. Advances in Materials 2018, 6, 1–10. 57. Zhang, J.; Liu, F.; Cheng, J. P.; Zhang, X. B. Binary nickel-cobalt oxides electrode materials for high-performance supercapacitors: Influence of its composition and porous nature. ACS Applied Materials & Interfaces 2015, 7(32), 17630–17640.
Index Note: Bold page numbers refer to tables and italic page numbers refer to figures. aliphatic quaternary ammonium (AQA) cations 186 aliphatic quaternary phosphonium (AQP) cations 186 angle-resolved photoemission spectroscopy (ARPES) 20, 36, 36, 61, 82 anisotropic energy 28 anti-crossing region 65 application programming interface (API) 110 argon-filled glove box 205 autoencoder (AE) 108, 109 back-contact perovskite solar cells (BC-PSCs) 220 band structures atom-dominated 8, 20, 60, 61, 95, 96, 130, 142, 253 features 27 low-energy 22 BAT-700 battery testing system 208 battery cell assembly 208 Bernal graphite 8 Bernal system 141 Bombarelli’s model 110 Bragg angle 72 Brillouin zone 61, 64, 83, 85, 88, 123, 124, 126, 263 carbon nanofibers (CNF) 2 carbon nanosphere (CNS) 168 Carlo methods 81 charge density carrier 35 Friedel 37 spatial 5, 8, 20, 21, 60, 61, 64, 66, 71, 72, 73, 81, 83, 85, 89, 120, 121, 130, 131, 137, 142, 264, 267, 268, 269, 280, 281 charge–discharge cycling performance 208 charge–discharge tests 208 chemical bonding 29, 30, 34, 65, 68, 71, 80, 83, 84, 85, 86, 88, 90, 91–93, 95, 118, 123, 129, 131, 137, 138, 142, 161, 254, 280, 281, 283 chemical VAE (chemVAE) 110, 111 chemical vapor deposition (CVD) technique 45 climbing image-nudged elastic band (CI-NEB) method 47, 56 conditional variational autoencoder (CVAE) 109 contact potential difference (CPD) 222
convolution neural network (CNN) jointing 108 coplanar back-contact structure 221–223 Coulombic matrix (CM) methods 106 Coulomb screening 251 3D binary V2O5 281 Debye-Scherrer/Guinier techniques 35 deep generative machine learning model 108–109, 109 DeLuca, G. 224 density functional theory (DFT) 21, 46, 61, 82 density of states (DOS) 1, 5, 8, 20, 21, 26, 30–34, 51, 60, 61, 64, 67, 70–73, 81, 120, 121, 126, 130, 137–142, 252, 253, 263, 269, 280, 281, 283 der Waals interactions 122 3D geometry 106 2D graphene systems 62 3D graphite systems 19 2D honeycomb lattice 150, 151 dimethyl carbonate (DMC) 183 Dirac-cone band structures 129 Dirac-cone structures 23, 26, 280 discharge-process energy 60 divacancy (DV) 47 3D Li2SiO3 unique fundamental properties of 252 2D molecular graphs 106 doped graphene 157 1D silicene/germanene nanoribbons 280 3D silicon/germanium/diamond 282 3D ternary LiGe/SnO compounds 281 3D ternary Li2SiO3 compound applications 94–95 chemical bond lengths 85, 87 comparisons with 94–95 electrode-electrolyte boundary 80 experimental measurements 94–95 geometric projections 84, 85 geometric structures 84, 84–86, 85–86, 87, 88, 89 Hamiltonian matrix elements 83 lattice constant 84 numerical simulations 82–83 rich and unique fundamental properties 95–96 rich electronic properties 82, 87–94, 88, 90 3D ternary LixCo/NiO2 compounds atom-dominated band structures 130
288 3D ternary LixCo/NiO2 compounds (cont.) 3D lithium oxide compounds 118 electron–electron Coulomb interactions 129 ferromagnetic configurations 131 first-principles calculations 141 graphene-related systems 140 non-magnetic semiconductors 126 phenomenological model 125 rich and unique electronic properties 125–141, 127, 128, 130, 132, 133–136, 138, 139, 140 Spin density distributions 132, 132 tight-binding model 120 unusual crystal structures 124–125, 125 VASP calculations 120–124, 122, 123, 124 X-ray elastic scatterings 117 electric hybrid vehicles 149, 150 electrochemical storage device 45 electrochemical testing 112 electrochemical windows 212, 212–213 electrode-electrolyte boundary 3D ternary Li2SiO3 compound 80 electrolyte molecular selection 104, 104–105 electrolytes deep generative machine learning model 108–109, 109 first-principles calculation 105 inverse design 108–109 machine learning regression model 105–107 material development experiments 105 molecular selection 104, 104–105 online accessible databases 110 our generative model 110–113 prediction performance 107, 107–108 electron affinity (EA) 5, 104, 252 electron-beam lithography 225 electronic energy spectrum 64, 65 electronic properties rich and unique 125–141, 127, 128, 130, 132, 133–136, 138, 139, 140 electron-selective layer (ESL) 219 electron spin resonance (ESR) 240 energy formation 48–50, 49 energy-storage system 234 ethylene carbonate (EC) 183 ethylene glycol (EG) 10 1-Ethyl-3-Vinylimidazolium Bis (Trifluoromethanesulfonylimide) (1E3V-TFSI) 205 extended-connectivity fingerprint (ECFP) 106 external quantum efficiency (EQE) 222 fabrication process 226, 226 Fang, Y. 158, 160 Fan, Z. 158 Fermi golden rule 263 Fermi level position 51, 52
Index Fermi momenta slopes 28 few-layered graphene (FLG) 160 Feynman force 21 field emission scanning electron microscopy (FESEM) 152, 207 field emission transmission electron microscopy (FETEM) 152 first-principles calculations 3D ternary LixCo/NiO2 compounds 141 electrolytes 105 nitrogen doped defective graphene computational details 47–48, 47–49 energy formation 48–50, 49 Fermi level position 51, 52 Li-storage capacity 52–55, 53–55, 55 migration energy barrier 55–57, 56, 56 single Li-adsorption 50, 50–51, 51, 52 first-principles method 68 fluorine-doped tin oxide (FTO) 219 Fossil fuels 8 Fourier transform infrared spectra (FTIR) 153 Fourier transform infrared (FT-IR) spectroscopic measurements 207 frontier molecular orbital theory 104 Fujinami, T. 184 Fukui, K. 104 Gaussian distribution 109 generalized gradient approximation (GGA) 47 generative adversarial network (GAN) 108 geometric projections 3D ternary Li2SiO3 compound 84, 85 geometry structures 72 global energy demand 45 Gomez-Bombarelli, R. 109, 110, 111 graphene bonding/binding energy/functional groups 153, 154, 155 green synthesis of 163 in lithium-ion batteries 156–162, 161, 162 microstructure analysis 152, 152, 153 phonon modes 153, 154, 155 scanning electron microscopy images of 150, 151 structure analysis 152, 152, 153 synthesis 151–152 graphene/melamine–formaldehyde (GMF) 159 graphene nanosheets (GNSs) 152, 254 Graphene oxide (GO) Raman analysis 153, 155 X-ray diffraction pattern 152, 152, 153 graphene oxide/melamine–formaldehyde (GOMF) 159 graphite-related systems 21 fundamental properties 20 grid energy storage 45 Guo, P. 156
Index Hall conductivities 34 Hellmann–Feynman force 21, 61, 83 heteroatom-doped graphenes 161, 162 hierarchical porous graphene aerogel (HPGA) 159 high electrical conductivities 8 highest occupied molecular orbital (HOMO) 104, 182 high-resolution X-ray elastic scatterings (HR-XES) 86 high-throughput virtual screening (HTVS) 108 hole-selective layer (HSL) 219 Hubbard tight-binding model 136, 142 Hummer’s method 151, 156 hybrid electric vehicles (HEVs) 9, 45, 268 hybrid solar cells 10, 11, 234, 235, 238, 240–246 Iijima, I. 265 imidazolium-based ionogel photopolymerization anion substitution 205 battery cell assembly 208 charge–discharge capacity 213–215, 214, 216, 216 charge–discharge cycling performance 208 charge–discharge tests 208 cyclic performance 213–215, 214, 216, 216 electrochemical windows 212, 212–213 electrolytes preparation 205–206, 206, 207 1E3V-TFSI 205 experimental process 206, 206 FT-IR spectroscopic measurements 207 ionic conductivity 207–208 linear sweep voltammetry 207–208 materials 205 multiple characteristic 208–210, 209, 210 products preparation 208–210, 209, 210 sample characterization 207 thermal properties electrolytes 210–212, 211 indium tin oxide (ITO) 219 interdigitated electrode (IDE) 220 ion-gels 191 ionic conductivities 3, 10, 192, 204, 212, 255, 268 ionic liquids (ILs) 182 anion and cations comprising 183, 183 classification 183–184, 184 eco-friendly applications 183 ionic liquid synthetic route metathesis reaction 195–196 synthetic route 1 193–195, 194, 195 LI–ion/Na–ion batteries Li+-conducting polymer electrolytes 191–192
low-melting alkaline salts 184–185 organic cations and counter anions 185, 186 organic ionic liquids 185–190, 189 solvent-in-salt electrolytes 191 synthetic route 192–196, 194, 195 ionic liquid synthetic route metathesis reaction 195–196 synthetic route 1 193–195, 194, 195 ionization energy (IE) 5, 34, 104, 252 Itaru, R. 160 Jumabekov, A. N. 223 Kang, S. 109, 110, 111 Kelvin probe force microscopy (KPFM) 222 Kohn–Sham equations 21, 121 Kubo formula 3, 20, 81, 261 Lee, H. 173 Le, M. L. P. 183 Le, P. 186, 188 Lian, P. 156 light-free carriers 264 Li+-ion-based batteries (LIBs) 45 anode material 2, 4, 8 cathodes 2, 4 charging processes 118, 119 chemically modified grapheme 160–162 chemical potential 104, 104 discharging processes 118, 119 doped graphene 157 electrochemical performance of 150 electrolytes characteristics 2, 4, 184, 184 grapheme 156–157 mechanism of 151, 151 physical methods 252 porous grapheme 158–160 potential applications Brillouin zone 263 Coulomb scattering processes 264 Fermi golden rule 263 graphene-related systems 263 Kubo formula 263 light-free carriers 264 rapid charging/discharging processes 7 solid-/liquid-state electrolyte 119 solid-state secondary 80 LI–ion/Na–ion batteries ILS for 196–198 Li+-conducting polymer electrolytes 191–192 low-melting alkaline salts alkaline imide salts mixtures 185 Li salts 184–185 organic cations and counter anions 185, 186 organic ionic liquids anion structure effects 187–190, 189
290 LI–ion/Na–ion batteries (cont.) cation structure effects 186–187 effects of 190 solvent-in-salt electrolytes 191 linear sweep voltammetry (LSV) 207–208 liquid plasma process cyano-aromatic molecules 175 different forms 168 EDX mapping analysis 173, 173 gas plasma process 170 nanocarbon formation 168–174, 169, 170–173, 174 nanocarbon hybrids/composites fuel cell applications 174–175 specific capacitance applications 175–176, 176 nitrogen-functionalized grapheme 172–174, 172–174 nitrogen polymer in 171, 171 unconventional polymers formation 170–171 Li-storage capacity 52–55, 53–55, 55 lithium secondary batteries 255 Li4Ti5O12 compound chemical bond lengths 68, 69–70 electronic energy spectrum 64, 65 rich electronic properties 64–72, 65–67, 69–70 rich geometric symmetries 62–64, 63– 64, 67 STS measurement 71 theoretical simulation methods 61–62 tight-binding model 61, 62, 64, 68, 70, 71, 72 unique electronic properties 64–72, 65–67, 69–70 Li+ transports 118 low-energy electron diffraction (LEED) 61, 82, 86 lowest unoccupied molecular orbital (LUMO) 104, 182 Ma, C. 46 machine learning method 5, 6, 103, 105–109, 252 machine learning regression model 105–107, 109 Ma, T. 221 Material Project (MP) 107 mean absolute error (MAE) 108 metathesis reaction 195–196 Monkhorst–Pack scheme 21, 61, 83 monolayer geometric structures 279, 279 SEM images 227, 227 monovacancy (MV) 47 Morishita, T. 169 multilayer graphene (MLGN) discharge capacity 153, 155
Index Fourier transform infrared spectra 153, 154 X-ray diffraction pattern 152, 152, 153 nanocarbon hybrids/composites fuel cell applications 174–175 specific capacitance applications 175–176, 176 natural language processing (NLP) models 106 N-doped porous graphene material (NPGM) 159 net magnetic moments 131, 133–136 neural network 1, 5 next-generation batteries 267 nitrogen doped defective graphene computational details 47–48, 47–49 energy formation 48–50, 49 Fermi level position 51, 52 Li-storage capacity 52–55, 53–55, 55 migration energy barrier 55–57, 56, 56 single Li-adsorption 50, 50–51, 51, 52 nitrogen doping 6 nitrogen-functionalized graphene (NFG) 168, 172 non-coplanar back-contact structure 223–228, 223–229, 230 non-magnetic semiconductors 126 numerical simulations 3D ternary Li2SiO3 compound 82–83 online accessible databases 110 orbital hybridizations multi- 5, 8, 61, 64, 67, 68, 70–73, 81, 86, 87, 90, 92–96, 119, 120, 125, 129, 131, 137, 141, 142, 251, 252, 253, 254, 264, 269, 281, 282, 283 single- 3, 22, 30, 60, 61, 81, 83, 120, 261 strong 95, 253 Panomsuwan, G. 175 Perdew–Burke–Ernzerhof (PBE) 21, 47, 61, 82 perovskite solar cells (PSCs) coplanar back-contact structure 221–223 non-coplanar back-contact structure 223–228, 223–229, 230 photo-lithography 220, 225, 228 photopolymerization anion substitution 205 battery cell assembly 208 charge–discharge capacity 213–215, 214, 216, 216 charge–discharge cycling performance 208 charge–discharge tests 208 cyclic performance 213–215, 214, 216, 216 electrochemical windows 212, 212–213 electrolytes preparation 205–206, 206, 207 1E3V-TFSI 205 experimental process 206, 206 FT-IR spectroscopic measurements 207
Index ionic conductivity 207–208 linear sweep voltammetry 207–208 materials 205 multiple characteristic 208–210, 209, 210 products preparation 208–210, 209, 210 sample characterization 207 thermal properties electrolytes 210–212, 211 Phung Le, M. L. 190 plug-in hybrid electric vehicles (PHEVs) 9, 268 poly(3,4-ethylenedioxythiophene): poly(styrenesulfonate) (PEDOT:PSS) arrangement of 234 hall-effect approaches 242, 243 hybrid solar cells 240–246, 241–243, 245, 246 light and chemical treatment 235 light-trapping effect 246 spin-coating methods 241 tunable electrical conductivity Baytron P synthesis process 235–236 PSS functions in 236–237 PSS investigations 237–238, 239, 240 porous graphene 158–160 potential applications LIBs Brillouin zone 263 Coulomb scattering processes 264 Fermi golden rule 263 graphene-related systems 263 Kubo formula 263 light-free carriers 264 powder X-ray diffraction (PXRD) 94 power conversion efficiency (PCE) 222 projector augmented-wave (PAW) method 47, 61, 82 propylene carbonate (PC) 183 quasi-interdigitated electrode (QIDE) 220 Raman spectroscopy 11, 244 Reddy, A. L. M. 45, 161 reduced graphene oxide (rGO) 160 reinforcement learning (RL) 108 Ren, L. 159, 160 rich electronic properties 64–72, 65–67, 69–70 rich geometric symmetries 62–64, 63–64, 67 scanning electron microscopy (SEM) 72, 94 scanning transmission electron microscopy (STEM) 46 scanning tunneling microscopy (STM) 61, 82, 86, 94 scanning tunneling spectroscopy (STS) 20, 92 Schrodinger equation 105, 113 secondary electrolyte interphase (SEI) 161 self-assembled monolayers (SAMs) 222
291 Senthilnathan, J. 171–177 silicene-and graphene-related systems 60 silicon nanowires based hybrid solar cells 240–246 simplified molecular-input line-entry system (SMILES) 106 Si-nanowire-based hybrid cells 11 single-layered graphene (SLG) 160 sodium-ion batteries (SIBs) 9 solid electrolyte interface (SEI) 254 solid electrolyte interphase (SEI) layer 210 solid state electrolyte 4, 80, 87, 93 solvents acetonitrile 171 molecular 183, 187, 196 nonpolar 168 organic 9, 168, 171, 182, 183, 188, 190, 191, 196, 198, 205, 215, 236, 255 polar 187, 190, 238, 240, 246 stage-n graphite alkali-intercalation compounds 23, 23 electronic properties 20 geometric properties 20 metallic behaviors 26–38 rich band structures 23, 25 semimetallic behaviors 26–38 theoretical calculations 21–22 tight-binding model 21 unique stacking configurations 22–26 Stone–Wales (SW) defects 47 submerged liquid plasma 5, 172 Sui, Z. Y. 159 Tainter, G.D. 224 thermal gravimetric analysis (TGA) 207 thin-film fabrication 241, 241, 256 Thomson scatterings 35 tight-binding models 61, 62, 64, 68, 70, 71, 72, 81, 279 total density of states (TDOS) 51, 51 transparent conducting oxide (TCO) 219 trial-and-error experimental method 105 trilayer graphene systems 280 tunable electrical conductivity Baytron P synthesis process 235–236 PSS functions in 236–237 PSS investigations 237–238, 239, 240 tunneling electron microscopy (TEM) 86 van der Waals interactions 19 Vargas, O. 157 variable range hopping (VRH) model 240 Variational autoencoder (VAE) 108 VASP calculations 120–124, 122, 123, 124 Vienna ab initio simulation package (VASP) 47, 60, 82
292 Wang, G. 156 Wang, H. G. 159 Watanabe, M. 185 Wu, Z. S. 45, 53, 157 X-ray diffraction (XRD) analysis 207 X-ray elastic scatterings 117
Index X-ray photoelectron spectroscopy (XPS) 46 X-ray scatterings 25 Yen, H. J. 161 Yoo, E. J. 156 Yoon, D. 160 Yoshimura, M. 171